#------------------------------------------------------------------------------
#$Date: 2025-07-01 14:22:46 +0300 (Tue, 01 Jul 2025) $
#$Revision: 1237 $
#$URL: svn://crystallography.net/testcod/cif/4/10/00/4100017.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4100017
loop_
_publ_author_name
'Bowman, Amy'
'Allix, Mathieu'
'Pelloquin, Denis'
'Rosseinsky, Matthew J.'
_publ_section_title
;
 Three-Coordinate Metal Centers in Extended Transition Metal Oxides
;
_journal_issue                   39
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              12606
_journal_page_last               12607
_journal_paper_doi               10.1021/ja064083g
_journal_volume                  128
_journal_year                    2006
_chemical_formula_sum            'Co0.75 Fe0.75 La0.5 O3.78 Sr1.5'
_chemical_formula_weight         347.43
_space_group_IT_number           139
_space_group_name_Hall           '-I 4 2'
_space_group_name_H-M_alt        'I 4/m m m'
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_H-M   'I 4/m m m'
_audit_creation_date             2006-06-08T15:19
_audit_creation_method           'from EXP file using GSAS2CIF'
_audit_update_record
' 2006-06-08T15:19  Initial CIF as created by GSAS2CIF'
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                90.0
_cell_formula_units_Z            4
_cell_length_a                   3.82416(12)
_cell_length_b                   3.82416
_cell_length_c                   29.3269(12)
_cell_measurement_temperature    443
_cell_volume                     428.88(2)
_computing_structure_refinement  GSAS
_diffrn_measurement_device_type  'D20 ILL'
_diffrn_radiation_type           neutron
_diffrn_radiation_wavelength     1.8885
_exptl_absorpt_correction_T_max  0.91993
_exptl_absorpt_correction_T_min  0.91877
_exptl_absorpt_process_details
;   GSAS Absorption/surface roughness correction: function number 0
 Debye-Scherrer absorption correction
Term (= MU.r/wave) =     0.26460E-01
Correction is not refined.
;
_exptl_crystal_density_diffrn    5.381
_exptl_crystal_density_method    'not measured'
_pd_block_id
2006-06-08T15:19|FINAL_POST_FOURIER_F|Amy|D20_ILL
_pd_calc_method                  'Rietveld Refinement'
_pd_char_colour                  black
_pd_instr_location               ' ?'
_pd_meas_2theta_range_inc        0.1
_pd_meas_2theta_range_max        154.9
_pd_meas_2theta_range_min        0.0
_pd_meas_number_of_points        1550
_pd_phase_name                   Sr3LaFe1.5Co1.5O7.5
_pd_proc_2theta_range_inc        0.1
_pd_proc_2theta_range_max        154.4924
_pd_proc_2theta_range_min        -0.4076
_pd_proc_info_datetime           2006-06-08T15:19:53
_pd_proc_info_excluded_regions   ' ?'
_pd_proc_ls_background_function
;   GSAS Background function number 1 with  6 terms.
 Shifted Chebyshev function of 1st kind
      1:    607.560     2:   -62.5850     3:   -9.69350     4:   -11.5373    
      5:   -1.55479     6:   -4.75016    
;
_pd_proc_ls_peak_cutoff          0.00100
_pd_proc_ls_pref_orient_corr
;   March-Dollase
 AXIS  1 Ratio=   1.09594  h= 0.000  k= 0.000  l= 1.000
 Prefered orientation correction range: Min=   0.75963, Max=   1.14736
;
_pd_proc_ls_profile_function
;
 CW Profile function number 2 with  18 terms
 Profile coefficients for Simpson's rule integration of pseudovoigt function
 C.J. Howard (1982). J. Appl. Cryst.,15,615-620.
 P. Thompson, D.E. Cox & J.B. Hastings (1987). J. Appl. Cryst.,20,79-83.
 #1(GU)   =  310.201 #2(GV)   = -641.243 #3(GW)   =  495.219
 #4(LX)   =    4.053 #5(LY)   =   12.617 #6(trns) =    0.000
 #7(asym) =   0.0000 #8(shft) =   0.0000 #9(GP)   =    0.000
 #10(stec)=     0.00 #11(ptec)=     0.00 #12(sfec)=     0.00
 #13(L11) =    0.000 #14(L22) =    0.000 #15(L33) =    0.000
 #16(L12) =    0.000 #17(L13) =    0.000 #18(L23) =    0.000
 Peak tails are ignored  where the intensity is below 0.0010 times the peak
   Aniso. broadening axis   0.0   0.0   1.0
;
_pd_proc_ls_prof_R_factor        0.0298
_pd_proc_ls_prof_wR_expected     0.0372
_pd_proc_ls_prof_wR_factor       0.0377
_pd_proc_number_of_points        1550
_pd_spec_mounting                ' ?'
_refine_ls_goodness_of_fit_all   1.03
_refine_ls_matrix_type           full
_refine_ls_number_parameters     40
_refine_ls_number_restraints     0
_refine_ls_R_Fsqd_factor         0.07703
_refine_ls_shift/su_max          0.02
_refine_ls_shift/su_mean         0.00
_reflns_d_resolution_high        1.009
_reflns_d_resolution_low         7.332
_reflns_limit_h_max              3
_reflns_limit_h_min              0
_reflns_limit_k_max              2
_reflns_limit_k_min              0
_reflns_limit_l_max              30
_reflns_limit_l_min              0
_reflns_number_total             99
_cod_data_source_file            ja064083gsi20060609_015619.cif
_cod_data_source_block           FINAL_POST_FOURIER_F_publ
_cod_original_cell_volume        428.88(4)
_cod_original_formula_sum        'Co0.75 Fe0.75 La0.50 O3.78 Sr1.50'
_cod_database_code               4100017
_gsas_exptl_extinct_corr_t_min   1.00000
_gsas_exptl_extinct_corr_t_max   1.00000
loop_
_symmetry_equiv_pos_site_id
_symmetry_equiv_pos_as_xyz
1 +x,+y,+z
2 -y,+x,+z
3 -x,-y,+z
4 +y,-x,+z
5 -x,+y,+z
6 -y,-x,+z
7 +x,-y,+z
8 +y,+x,+z
-1 -x,-y,-z
-2 +y,-x,-z
-3 +x,+y,-z
-4 -y,+x,-z
-5 +x,-y,-z
-6 +y,+x,-z
-7 -x,+y,-z
-8 -y,-x,-z
101 +x+1/2,+y+1/2,+z+1/2
102 -y+1/2,+x+1/2,+z+1/2
103 -x+1/2,-y+1/2,+z+1/2
104 +y+1/2,-x+1/2,+z+1/2
105 -x+1/2,+y+1/2,+z+1/2
106 -y+1/2,-x+1/2,+z+1/2
107 +x+1/2,-y+1/2,+z+1/2
108 +y+1/2,+x+1/2,+z+1/2
-101 -x+1/2,-y+1/2,-z+1/2
-102 +y+1/2,-x+1/2,-z+1/2
-103 +x+1/2,+y+1/2,-z+1/2
-104 -y+1/2,+x+1/2,-z+1/2
-105 +x+1/2,-y+1/2,-z+1/2
-106 +y+1/2,+x+1/2,-z+1/2
-107 -x+1/2,+y+1/2,-z+1/2
-108 -y+1/2,-x+1/2,-z+1/2
loop_
_atom_site_type_symbol
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_thermal_displace_type
_atom_site_U_iso_or_equiv
_atom_site_symmetry_multiplicity
Fe Fe1 0.0 0.0 0.0 0.418(23) Uani 0.03578 2
Fe Fe2 0.0 0.0 0.14307(26) 0.541(12) Uani 0.016 4
La La1 0.0 0.0 0.57577(26) 0.25 Uiso 0.0212(12) 4
Sr Sr1 0.0 0.0 0.57577(26) 0.75 Uiso 0.0212(12) 4
La La2 0.0 0.0 0.70288(20) 0.25 Uiso 0.0212(12) 4
Sr Sr2 0.0 0.0 0.70288(20) 0.75 Uiso 0.0212(12) 4
O O1 0.0 0.5 0.13728(31) 0.758(10) Uani 0.02532 8
O O2 0.0 0.0 0.06093(25) 1.0 Uani 0.04968 4
O O3 0.0 0.0 0.21369(28) 0.963(22) Uiso 0.0152(23) 4
O O4 0.264(10) 0.436(12) 0.0 0.054(5) Uiso 0.0152(23) 16
Co Co1 0.0 0.0 0.0 0.576(23) Uani 0.03578 2
Co Co2 0.0 0.0 0.14307(26) 0.462(12) Uani 0.016 4
O O5 0.5 0.0 0.0 0.082(13) Uiso 0.0152(23) 4
loop_
_atom_type_symbol
_atom_type_number_in_cell
_atom_type_scat_length_neutron
_atom_type_scat_source
Fe+3 3.0 0.9450 International_Tables_Vol_C
La+3 2.0 0.8240 International_Tables_Vol_C
Sr+2 6.0 0.7020 International_Tables_Vol_C
O 15.116 0.5805 International_Tables_Vol_C
Co 3.0 0.2490 International_Tables_Vol_C
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_2
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O2 Fe1 O2 180.0 1_555 . -1_555 N
O2 Fe1 O4 90.0 1_555 . 1_555 N
O2 Fe1 O4 90.0 1_555 . 2_555 N
O2 Fe1 O4 90.0 1_555 . 3_555 N
O2 Fe1 O4 90.0 1_555 . 4_555 N
O2 Fe1 O4 90.0 1_555 . 5_555 N
O2 Fe1 O4 90.0 1_555 . 6_555 N
O2 Fe1 O4 90.0 1_555 . 7_555 N
O2 Fe1 O4 90.0 1_555 . 8_555 N
O2 Fe1 O5 90.0 1_555 . 1_455 N
O2 Fe1 O5 90.0 1_555 . 1_555 N
O2 Fe1 O5 90.0 1_555 . 2_545 N
O2 Fe1 O5 90.0 1_555 . 2_555 N
O2 Fe1 O4 90.0 -1_555 . 1_555 N
O2 Fe1 O4 90.0 -1_555 . 2_555 N
O2 Fe1 O4 90.0 -1_555 . 3_555 N
O2 Fe1 O4 90.0 -1_555 . 4_555 N
O2 Fe1 O4 90.0 -1_555 . 5_555 N
O2 Fe1 O4 90.0 -1_555 . 6_555 N
O2 Fe1 O4 90.0 -1_555 . 7_555 N
O2 Fe1 O4 90.0 -1_555 . 8_555 N
O2 Fe1 O5 90.0 -1_555 . 1_455 N
O2 Fe1 O5 90.0 -1_555 . 1_555 N
O2 Fe1 O5 90.0 -1_555 . 2_545 N
O2 Fe1 O5 90.0 -1_555 . 2_555 N
O4 Fe1 O4 90.0 1_555 . 2_555 N
O4 Fe1 O4 180.0 1_555 . 3_555 N
O4 Fe1 O4 90.0 1_555 . 4_555 N
O4 Fe1 O4 62.4(23) 1_555 . 5_555 N
O4 Fe1 O4 152.4(23) 1_555 . 6_555 N
O4 Fe1 O4 117.6(23) 1_555 . 7_555 N
O4 Fe1 O4 27.6(23) 1_555 . 8_555 N
O4 Fe1 O5 121.2(12) 1_555 . 1_455 N
O4 Fe1 O5 58.8(12) 1_555 . 1_555 N
O4 Fe1 O5 148.8(12) 1_555 . 2_545 N
O4 Fe1 O5 31.2(12) 1_555 . 2_555 N
O4 Fe1 O4 90.0 2_555 . 3_555 N
O4 Fe1 O4 180.0 2_555 . 4_555 N
O4 Fe1 O4 27.6(23) 2_555 . 5_555 N
O4 Fe1 O4 62.4(23) 2_555 . 6_555 N
O4 Fe1 O4 152.4(23) 2_555 . 7_555 N
O4 Fe1 O4 117.6(23) 2_555 . 8_555 N
O4 Fe1 O5 31.2(12) 2_555 . 1_455 N
O4 Fe1 O5 148.8(12) 2_555 . 1_555 N
O4 Fe1 O5 121.2(12) 2_555 . 2_545 N
O4 Fe1 O5 58.8(12) 2_555 . 2_555 N
O4 Fe1 O4 90.0 3_555 . 4_555 N
O4 Fe1 O4 117.6(23) 3_555 . 5_555 N
O4 Fe1 O4 27.6(23) 3_555 . 6_555 N
O4 Fe1 O4 62.4(23) 3_555 . 7_555 N
O4 Fe1 O4 152.4(23) 3_555 . 8_555 N
O4 Fe1 O5 58.8(12) 3_555 . 1_455 N
O4 Fe1 O5 121.2(12) 3_555 . 1_555 N
O4 Fe1 O5 31.2(12) 3_555 . 2_545 N
O4 Fe1 O5 148.8(12) 3_555 . 2_555 N
O4 Fe1 O4 152.4(23) 4_555 . 5_555 N
O4 Fe1 O4 117.6(23) 4_555 . 6_555 N
O4 Fe1 O4 27.6(23) 4_555 . 7_555 N
O4 Fe1 O4 62.4(23) 4_555 . 8_555 N
O4 Fe1 O5 148.8(12) 4_555 . 1_455 N
O4 Fe1 O5 31.2(12) 4_555 . 1_555 N
O4 Fe1 O5 58.8(12) 4_555 . 2_545 N
O4 Fe1 O5 121.2(12) 4_555 . 2_555 N
O4 Fe1 O4 90.0 5_555 . 6_555 N
O4 Fe1 O4 179.9802 5_555 . 7_555 N
O4 Fe1 O4 90.0 5_555 . 8_555 N
O4 Fe1 O5 58.8(12) 5_555 . 1_455 N
O4 Fe1 O5 121.2(12) 5_555 . 1_555 N
O4 Fe1 O5 148.8(12) 5_555 . 2_545 N
O4 Fe1 O5 31.2(12) 5_555 . 2_555 N
O4 Fe1 O4 90.0 6_555 . 7_555 N
O4 Fe1 O4 180.0 6_555 . 8_555 N
O4 Fe1 O5 31.2(12) 6_555 . 1_455 N
O4 Fe1 O5 148.8(12) 6_555 . 1_555 N
O4 Fe1 O5 58.8(12) 6_555 . 2_545 N
O4 Fe1 O5 121.2(12) 6_555 . 2_555 N
O4 Fe1 O4 90.0 7_555 . 8_555 N
O4 Fe1 O5 121.2(12) 7_555 . 1_455 N
O4 Fe1 O5 58.8(12) 7_555 . 1_555 N
O4 Fe1 O5 31.2(12) 7_555 . 2_545 N
O4 Fe1 O5 148.8(12) 7_555 . 2_555 N
O4 Fe1 O5 148.8(12) 8_555 . 1_455 N
O4 Fe1 O5 31.2(12) 8_555 . 1_555 N
O4 Fe1 O5 121.2(12) 8_555 . 2_545 N
O4 Fe1 O5 58.8(12) 8_555 . 2_555 N
O5 Fe1 O5 180.0 1_455 . 1_555 N
O5 Fe1 O5 90.0 1_455 . 2_545 N
O5 Fe1 O5 90.0 1_455 . 2_555 N
O5 Fe1 O5 90.0 1_555 . 2_545 N
O5 Fe1 O5 90.0 1_555 . 2_555 N
O5 Fe1 O5 180.0 2_545 . 2_555 N
Sr1 Fe2 Sr1 69.66(14) 101_444 . 101_454 N
Sr1 Fe2 Sr1 69.66(14) 101_444 . 101_544 N
Sr1 Fe2 Sr1 107.75(27) 101_444 . 101_554 N
Sr1 Fe2 Sr2 69.10(9) 101_444 . 101_444 N
Sr1 Fe2 Sr2 108.71(4) 101_444 . 101_454 N
Sr1 Fe2 Sr2 108.71(4) 101_444 . 101_544 N
Sr1 Fe2 Sr2 176.84(24) 101_444 . 101_554 N
Sr1 Fe2 O1 51.60(24) 101_444 . 1_545 N
Sr1 Fe2 O1 121.11(28) 101_444 . 1_555 N
Sr1 Fe2 O1 51.60(24) 101_444 . 2_555 N
Sr1 Fe2 O1 121.11(28) 101_444 . 2_655 N
Sr1 Fe2 O3 126.13(13) 101_444 . 1_555 N
Sr1 Fe2 Sr1 107.75(27) 101_454 . 101_544 N
Sr1 Fe2 Sr1 69.66(14) 101_454 . 101_554 N
Sr1 Fe2 Sr2 108.71(4) 101_454 . 101_444 N
Sr1 Fe2 Sr2 69.10(9) 101_454 . 101_454 N
Sr1 Fe2 Sr2 176.84(24) 101_454 . 101_544 N
Sr1 Fe2 Sr2 108.71(4) 101_454 . 101_554 N
Sr1 Fe2 O1 121.11(28) 101_454 . 1_545 N
Sr1 Fe2 O1 51.60(24) 101_454 . 1_555 N
Sr1 Fe2 O1 51.60(24) 101_454 . 2_555 N
Sr1 Fe2 O1 121.11(28) 101_454 . 2_655 N
Sr1 Fe2 O3 126.13(13) 101_454 . 1_555 N
Sr1 Fe2 Sr1 69.66(14) 101_544 . 101_554 N
Sr1 Fe2 Sr2 108.71(4) 101_544 . 101_444 N
Sr1 Fe2 Sr2 176.84(24) 101_544 . 101_454 N
Sr1 Fe2 Sr2 69.10(9) 101_544 . 101_544 N
Sr1 Fe2 Sr2 108.71(4) 101_544 . 101_554 N
Sr1 Fe2 O1 51.60(24) 101_544 . 1_545 N
Sr1 Fe2 O1 121.11(28) 101_544 . 1_555 N
Sr1 Fe2 O1 121.11(28) 101_544 . 2_555 N
Sr1 Fe2 O1 51.60(24) 101_544 . 2_655 N
Sr1 Fe2 O3 126.13(13) 101_544 . 1_555 N
Sr1 Fe2 Sr2 176.84(24) 101_554 . 101_444 N
Sr1 Fe2 Sr2 108.71(4) 101_554 . 101_454 N
Sr1 Fe2 Sr2 108.71(4) 101_554 . 101_544 N
Sr1 Fe2 Sr2 69.10(9) 101_554 . 101_554 N
Sr1 Fe2 O1 121.11(28) 101_554 . 1_545 N
Sr1 Fe2 O1 51.60(24) 101_554 . 1_555 N
Sr1 Fe2 O1 121.11(28) 101_554 . 2_555 N
Sr1 Fe2 O1 51.60(24) 101_554 . 2_655 N
Sr1 Fe2 O3 126.13(13) 101_554 . 1_555 N
Sr2 Fe2 Sr2 72.77(11) 101_444 . 101_454 N
Sr2 Fe2 Sr2 72.77(11) 101_444 . 101_544 N
Sr2 Fe2 Sr2 114.06(24) 101_444 . 101_554 N
Sr2 Fe2 O1 57.13(24) 101_444 . 1_545 N
Sr2 Fe2 O1 129.72(24) 101_444 . 1_555 N
Sr2 Fe2 O1 57.13(24) 101_444 . 2_555 N
Sr2 Fe2 O1 129.72(24) 101_444 . 2_655 N
Sr2 Fe2 O3 57.03(12) 101_444 . 1_555 N
Sr2 Fe2 Sr2 114.06(24) 101_454 . 101_544 N
Sr2 Fe2 Sr2 72.77(11) 101_454 . 101_554 N
Sr2 Fe2 O1 129.72(24) 101_454 . 1_545 N
Sr2 Fe2 O1 57.13(24) 101_454 . 1_555 N
Sr2 Fe2 O1 57.13(24) 101_454 . 2_555 N
Sr2 Fe2 O1 129.72(24) 101_454 . 2_655 N
Sr2 Fe2 O3 57.03(12) 101_454 . 1_555 N
Sr2 Fe2 Sr2 72.77(11) 101_544 . 101_554 N
Sr2 Fe2 O1 57.13(24) 101_544 . 1_545 N
Sr2 Fe2 O1 129.72(24) 101_544 . 1_555 N
Sr2 Fe2 O1 129.72(24) 101_544 . 2_555 N
Sr2 Fe2 O1 57.13(24) 101_544 . 2_655 N
Sr2 Fe2 O3 57.03(12) 101_544 . 1_555 N
Sr2 Fe2 O1 129.72(24) 101_554 . 1_545 N
Sr2 Fe2 O1 57.13(24) 101_554 . 1_555 N
Sr2 Fe2 O1 129.72(24) 101_554 . 2_555 N
Sr2 Fe2 O1 57.13(24) 101_554 . 2_655 N
Sr2 Fe2 O3 57.03(12) 101_554 . 1_555 N
O1 Fe2 O1 169.8(7) 1_545 . 1_555 N
O1 Fe2 O1 89.55(6) 1_545 . 2_555 N
O1 Fe2 O1 89.55(6) 1_545 . 2_655 N
O1 Fe2 O3 95.1(4) 1_545 . 1_555 N
O1 Fe2 O1 89.55(6) 1_555 . 2_555 N
O1 Fe2 O1 89.55(6) 1_555 . 2_655 N
O1 Fe2 O3 95.1(4) 1_555 . 1_555 N
O1 Fe2 O1 169.8(7) 2_555 . 2_655 N
O1 Fe2 O3 95.1(4) 2_555 . 1_555 N
O1 Fe2 O3 95.1(4) 2_655 . 1_555 N
Sr1 La1 Sr1 90.0 1_455 . 1_545 N
Sr1 La1 Sr1 90.0 1_455 . 1_565 N
Sr1 La1 Sr1 180.0 1_455 . 1_655 N
Sr1 La1 La2 90.0 1_455 . 1_555 N
Sr1 La1 Sr2 90.0 1_455 . 1_555 N
Sr1 La1 O1 43.33(24) 1_455 . 101_445 N
Sr1 La1 O1 136.67(24) 1_455 . 101_545 N
Sr1 La1 O1 90.0 1_455 . 102_545 N
Sr1 La1 O1 90.0 1_455 . 102_555 N
Sr1 La1 O2 45.723(34) 1_455 . 101_445 N
Sr1 La1 O2 45.723(34) 1_455 . 101_455 N
Sr1 La1 O2 134.277(34) 1_455 . 101_545 N
Sr1 La1 O2 134.277(34) 1_455 . 101_555 N
Sr1 La1 O4 68.0(8) 1_455 . 101_445 N
Sr1 La1 O4 95.8(11) 1_455 . 102_545 N
Sr1 La1 O4 112.0(8) 1_455 . 103_555 N
Sr1 La1 O4 84.2(11) 1_455 . 104_455 N
Sr1 La1 O4 112.0(8) 1_455 . 105_545 N
Sr1 La1 O4 95.8(11) 1_455 . 106_555 N
Sr1 La1 O4 68.0(8) 1_455 . 107_455 N
Sr1 La1 O4 84.2(11) 1_455 . 108_445 N
Sr1 La1 Sr1 180.0 1_545 . 1_565 N
Sr1 La1 Sr1 90.0 1_545 . 1_655 N
Sr1 La1 La2 90.0 1_545 . 1_555 N
Sr1 La1 Sr2 90.0 1_545 . 1_555 N
Sr1 La1 O1 90.0 1_545 . 101_445 N
Sr1 La1 O1 90.0 1_545 . 101_545 N
Sr1 La1 O1 43.33(24) 1_545 . 102_545 N
Sr1 La1 O1 136.67(24) 1_545 . 102_555 N
Sr1 La1 O2 45.723(34) 1_545 . 101_445 N
Sr1 La1 O2 134.277(34) 1_545 . 101_455 N
Sr1 La1 O2 45.723(34) 1_545 . 101_545 N
Sr1 La1 O2 134.277(34) 1_545 . 101_555 N
Sr1 La1 O4 84.2(11) 1_545 . 101_445 N
Sr1 La1 O4 68.0(8) 1_545 . 102_545 N
Sr1 La1 O4 95.8(11) 1_545 . 103_555 N
Sr1 La1 O4 112.0(8) 1_545 . 104_455 N
Sr1 La1 O4 84.2(11) 1_545 . 105_545 N
Sr1 La1 O4 112.0(8) 1_545 . 106_555 N
Sr1 La1 O4 95.8(11) 1_545 . 107_455 N
Sr1 La1 O4 68.0(8) 1_545 . 108_445 N
Sr1 La1 Sr1 90.0 1_565 . 1_655 N
Sr1 La1 La2 90.0 1_565 . 1_555 N
Sr1 La1 Sr2 90.0 1_565 . 1_555 N
Sr1 La1 O1 90.0 1_565 . 101_445 N
Sr1 La1 O1 90.0 1_565 . 101_545 N
Sr1 La1 O1 136.67(24) 1_565 . 102_545 N
Sr1 La1 O1 43.33(24) 1_565 . 102_555 N
Sr1 La1 O2 134.277(34) 1_565 . 101_445 N
Sr1 La1 O2 45.723(34) 1_565 . 101_455 N
Sr1 La1 O2 134.277(34) 1_565 . 101_545 N
Sr1 La1 O2 45.723(34) 1_565 . 101_555 N
Sr1 La1 O4 95.8(11) 1_565 . 101_445 N
Sr1 La1 O4 112.0(8) 1_565 . 102_545 N
Sr1 La1 O4 84.2(11) 1_565 . 103_555 N
Sr1 La1 O4 68.0(8) 1_565 . 104_455 N
Sr1 La1 O4 95.8(11) 1_565 . 105_545 N
Sr1 La1 O4 68.0(8) 1_565 . 106_555 N
Sr1 La1 O4 84.2(11) 1_565 . 107_455 N
Sr1 La1 O4 112.0(8) 1_565 . 108_445 N
Sr1 La1 La2 90.0 1_655 . 1_555 N
Sr1 La1 Sr2 90.0 1_655 . 1_555 N
Sr1 La1 O1 136.67(24) 1_655 . 101_445 N
Sr1 La1 O1 43.33(24) 1_655 . 101_545 N
Sr1 La1 O1 90.0 1_655 . 102_545 N
Sr1 La1 O1 90.0 1_655 . 102_555 N
Sr1 La1 O2 134.277(34) 1_655 . 101_445 N
Sr1 La1 O2 134.277(34) 1_655 . 101_455 N
Sr1 La1 O2 45.723(34) 1_655 . 101_545 N
Sr1 La1 O2 45.723(34) 1_655 . 101_555 N
Sr1 La1 O4 112.0(8) 1_655 . 101_445 N
Sr1 La1 O4 84.2(11) 1_655 . 102_545 N
Sr1 La1 O4 68.0(8) 1_655 . 103_555 N
Sr1 La1 O4 95.8(11) 1_655 . 104_455 N
Sr1 La1 O4 68.0(8) 1_655 . 105_545 N
Sr1 La1 O4 84.2(11) 1_655 . 106_555 N
Sr1 La1 O4 112.0(8) 1_655 . 107_455 N
Sr1 La1 O4 95.8(11) 1_655 . 108_445 N
La2 La1 Sr2 0.0 1_555 . 1_555 N
La2 La1 O1 46.67(24) 1_555 . 101_445 N
La2 La1 O1 46.67(24) 1_555 . 101_545 N
La2 La1 O1 46.67(24) 1_555 . 102_545 N
La2 La1 O1 46.67(24) 1_555 . 102_555 N
La2 La1 O2 99.14(22) 1_555 . 101_445 N
La2 La1 O2 99.14(22) 1_555 . 101_455 N
La2 La1 O2 99.14(22) 1_555 . 101_545 N
La2 La1 O2 99.14(22) 1_555 . 101_555 N
La2 La1 O4 157.2(8) 1_555 . 101_445 N
La2 La1 O4 157.2(8) 1_555 . 102_545 N
La2 La1 O4 157.2(8) 1_555 . 103_555 N
La2 La1 O4 157.2(8) 1_555 . 104_455 N
La2 La1 O4 157.2(8) 1_555 . 105_545 N
La2 La1 O4 157.2(8) 1_555 . 106_555 N
La2 La1 O4 157.2(8) 1_555 . 107_455 N
La2 La1 O4 157.2(8) 1_555 . 108_445 N
Sr2 La1 O1 46.67(24) 1_555 . 101_445 N
Sr2 La1 O1 46.67(24) 1_555 . 101_545 N
Sr2 La1 O1 46.67(24) 1_555 . 102_545 N
Sr2 La1 O1 46.67(24) 1_555 . 102_555 N
Sr2 La1 O2 99.14(22) 1_555 . 101_445 N
Sr2 La1 O2 99.14(22) 1_555 . 101_455 N
Sr2 La1 O2 99.14(22) 1_555 . 101_545 N
Sr2 La1 O2 99.14(22) 1_555 . 101_555 N
Sr2 La1 O4 157.2(8) 1_555 . 101_445 N
Sr2 La1 O4 157.2(8) 1_555 . 102_545 N
Sr2 La1 O4 157.2(8) 1_555 . 103_555 N
Sr2 La1 O4 157.2(8) 1_555 . 104_455 N
Sr2 La1 O4 157.2(8) 1_555 . 105_545 N
Sr2 La1 O4 157.2(8) 1_555 . 106_555 N
Sr2 La1 O4 157.2(8) 1_555 . 107_455 N
Sr2 La1 O4 157.2(8) 1_555 . 108_445 N
O1 La1 O1 93.3(5) 101_445 . 101_545 N
O1 La1 O1 61.91(27) 101_445 . 102_545 N
O1 La1 O1 61.91(27) 101_445 . 102_555 N
O1 La1 O2 66.50(16) 101_445 . 101_445 N
O1 La1 O2 66.50(16) 101_445 . 101_455 N
O1 La1 O2 128.08(24) 101_445 . 101_545 N
O1 La1 O2 128.08(24) 101_445 . 101_555 N
O1 La1 O4 111.1(8) 101_445 . 101_445 N
O1 La1 O4 134.9(10) 101_445 . 102_545 N
O1 La1 O4 154.8(9) 101_445 . 103_555 N
O1 La1 O4 124.0(11) 101_445 . 104_455 N
O1 La1 O4 154.8(9) 101_445 . 105_545 N
O1 La1 O4 134.9(10) 101_445 . 106_555 N
O1 La1 O4 111.1(8) 101_445 . 107_455 N
O1 La1 O4 124.0(11) 101_445 . 108_445 N
O1 La1 O1 61.91(27) 101_545 . 102_545 N
O1 La1 O1 61.91(27) 101_545 . 102_555 N
O1 La1 O2 128.08(24) 101_545 . 101_445 N
O1 La1 O2 128.08(24) 101_545 . 101_455 N
O1 La1 O2 66.50(16) 101_545 . 101_545 N
O1 La1 O2 66.50(16) 101_545 . 101_555 N
O1 La1 O4 154.8(9) 101_545 . 101_445 N
O1 La1 O4 124.0(11) 101_545 . 102_545 N
O1 La1 O4 111.1(8) 101_545 . 103_555 N
O1 La1 O4 134.9(10) 101_545 . 104_455 N
O1 La1 O4 111.1(8) 101_545 . 105_545 N
O1 La1 O4 124.0(11) 101_545 . 106_555 N
O1 La1 O4 154.8(9) 101_545 . 107_455 N
O1 La1 O4 134.9(10) 101_545 . 108_445 N
O1 La1 O1 93.3(5) 102_545 . 102_555 N
O1 La1 O2 66.50(16) 102_545 . 101_445 N
O1 La1 O2 128.08(24) 102_545 . 101_455 N
O1 La1 O2 66.50(16) 102_545 . 101_545 N
O1 La1 O2 128.08(24) 102_545 . 101_555 N
O1 La1 O4 124.0(11) 102_545 . 101_445 N
O1 La1 O4 111.1(8) 102_545 . 102_545 N
O1 La1 O4 134.9(10) 102_545 . 103_555 N
O1 La1 O4 154.8(9) 102_545 . 104_455 N
O1 La1 O4 124.0(11) 102_545 . 105_545 N
O1 La1 O4 154.8(9) 102_545 . 106_555 N
O1 La1 O4 134.9(10) 102_545 . 107_455 N
O1 La1 O4 111.1(8) 102_545 . 108_445 N
O1 La1 O2 128.08(24) 102_555 . 101_445 N
O1 La1 O2 66.50(16) 102_555 . 101_455 N
O1 La1 O2 128.08(24) 102_555 . 101_545 N
O1 La1 O2 66.50(16) 102_555 . 101_555 N
O1 La1 O4 134.9(10) 102_555 . 101_445 N
O1 La1 O4 154.8(9) 102_555 . 102_545 N
O1 La1 O4 124.0(11) 102_555 . 103_555 N
O1 La1 O4 111.1(8) 102_555 . 104_455 N
O1 La1 O4 134.9(10) 102_555 . 105_545 N
O1 La1 O4 111.1(8) 102_555 . 106_555 N
O1 La1 O4 124.0(11) 102_555 . 107_455 N
O1 La1 O4 154.8(9) 102_555 . 108_445 N
O2 La1 O2 88.55(7) 101_445 . 101_455 N
O2 La1 O2 88.55(7) 101_445 . 101_545 N
O2 La1 O2 161.7(4) 101_445 . 101_555 N
O2 La1 O4 61.4(9) 101_445 . 101_445 N
O2 La1 O4 70.3(10) 101_445 . 102_545 N
O2 La1 O4 100.7(10) 101_445 . 103_555 N
O2 La1 O4 92.5(10) 101_445 . 104_455 N
O2 La1 O4 92.5(10) 101_445 . 105_545 N
O2 La1 O4 100.7(10) 101_445 . 106_555 N
O2 La1 O4 70.3(10) 101_445 . 107_455 N
O2 La1 O4 61.4(9) 101_445 . 108_445 N
O2 La1 O2 161.7(4) 101_455 . 101_545 N
O2 La1 O2 88.55(7) 101_455 . 101_555 N
O2 La1 O4 70.3(10) 101_455 . 101_445 N
O2 La1 O4 100.7(10) 101_455 . 102_545 N
O2 La1 O4 92.5(10) 101_455 . 103_555 N
O2 La1 O4 61.4(9) 101_455 . 104_455 N
O2 La1 O4 100.7(10) 101_455 . 105_545 N
O2 La1 O4 70.3(10) 101_455 . 106_555 N
O2 La1 O4 61.4(9) 101_455 . 107_455 N
O2 La1 O4 92.5(10) 101_455 . 108_445 N
O2 La1 O2 88.55(7) 101_545 . 101_555 N
O2 La1 O4 92.5(10) 101_545 . 101_445 N
O2 La1 O4 61.4(9) 101_545 . 102_545 N
O2 La1 O4 70.3(10) 101_545 . 103_555 N
O2 La1 O4 100.7(10) 101_545 . 104_455 N
O2 La1 O4 61.4(9) 101_545 . 105_545 N
O2 La1 O4 92.5(10) 101_545 . 106_555 N
O2 La1 O4 100.7(10) 101_545 . 107_455 N
O2 La1 O4 70.3(10) 101_545 . 108_445 N
O2 La1 O4 100.7(10) 101_555 . 101_445 N
O2 La1 O4 92.5(10) 101_555 . 102_545 N
O2 La1 O4 61.4(9) 101_555 . 103_555 N
O2 La1 O4 70.3(10) 101_555 . 104_455 N
O2 La1 O4 70.3(10) 101_555 . 105_545 N
O2 La1 O4 61.4(9) 101_555 . 106_555 N
O2 La1 O4 92.5(10) 101_555 . 107_455 N
O2 La1 O4 100.7(10) 101_555 . 108_445 N
O4 La1 O4 31.8(11) 101_445 . 102_545 N
O4 La1 O4 45.6(16) 101_445 . 103_555 N
O4 La1 O4 31.8(11) 101_445 . 104_455 N
O4 La1 O4 44.0(16) 101_445 . 105_545 N
O4 La1 O4 39.3(18) 101_445 . 106_555 N
O4 La1 O4 11.6(21) 101_445 . 107_455 N
O4 La1 O4 22.3(20) 101_445 . 108_445 N
O4 La1 O4 31.8(11) 102_545 . 103_555 N
O4 La1 O4 45.6(16) 102_545 . 104_455 N
O4 La1 O4 22.3(20) 102_545 . 105_545 N
O4 La1 O4 44.0(16) 102_545 . 106_555 N
O4 La1 O4 39.3(18) 102_545 . 107_455 N
O4 La1 O4 11.6(21) 102_545 . 108_445 N
O4 La1 O4 31.8(11) 103_555 . 104_455 N
O4 La1 O4 11.6(21) 103_555 . 105_545 N
O4 La1 O4 22.3(20) 103_555 . 106_555 N
O4 La1 O4 44.0(16) 103_555 . 107_455 N
O4 La1 O4 39.3(18) 103_555 . 108_445 N
O4 La1 O4 39.3(18) 104_455 . 105_545 N
O4 La1 O4 11.6(21) 104_455 . 106_555 N
O4 La1 O4 22.3(20) 104_455 . 107_455 N
O4 La1 O4 44.0(16) 104_455 . 108_445 N
O4 La1 O4 31.8(11) 105_545 . 106_555 N
O4 La1 O4 45.6(16) 105_545 . 107_455 N
O4 La1 O4 31.8(11) 105_545 . 108_445 N
O4 La1 O4 31.8(11) 106_555 . 107_455 N
O4 La1 O4 45.6(16) 106_555 . 108_445 N
O4 La1 O4 31.8(11) 107_455 . 108_445 N
Fe2 Sr1 Fe2 69.66(14) 101_445 . 101_455 N
Fe2 Sr1 Fe2 69.66(14) 101_445 . 101_545 N
Fe2 Sr1 Fe2 107.74(27) 101_445 . 101_555 N
Fe2 Sr1 La1 55.17(7) 101_445 . 1_455 N
Fe2 Sr1 La1 55.17(7) 101_445 . 1_545 N
Fe2 Sr1 La1 124.83(7) 101_445 . 1_565 N
Fe2 Sr1 La1 124.83(7) 101_445 . 1_655 N
Fe2 Sr1 Sr1 55.17(7) 101_445 . 1_455 N
Fe2 Sr1 Sr1 55.17(7) 101_445 . 1_545 N
Fe2 Sr1 Sr1 124.83(7) 101_445 . 1_565 N
Fe2 Sr1 Sr1 124.83(7) 101_445 . 1_655 N
Fe2 Sr1 La2 53.87(13) 101_445 . 1_555 N
Fe2 Sr1 Sr2 53.87(13) 101_445 . 1_555 N
Fe2 Sr1 O1 34.91(7) 101_445 . 101_445 N
Fe2 Sr1 O1 90.62(28) 101_445 . 101_545 N
Fe2 Sr1 O1 34.91(7) 101_445 . 102_545 N
Fe2 Sr1 O1 90.62(28) 101_445 . 102_555 N
Fe2 Sr1 O2 45.27(21) 101_445 . 101_445 N
Fe2 Sr1 O2 95.37(12) 101_445 . 101_455 N
Fe2 Sr1 O2 95.37(12) 101_445 . 101_545 N
Fe2 Sr1 O2 153.01(29) 101_445 . 101_555 N
Fe2 Sr1 O4 105.8(9) 101_445 . 101_445 N
Fe2 Sr1 O4 112.8(9) 101_445 . 102_545 N
Fe2 Sr1 O4 144.6(10) 101_445 . 103_555 N
Fe2 Sr1 Fe2 107.74(27) 101_455 . 101_545 N
Fe2 Sr1 Fe2 69.66(14) 101_455 . 101_555 N
Fe2 Sr1 La1 55.17(7) 101_455 . 1_455 N
Fe2 Sr1 La1 124.83(7) 101_455 . 1_545 N
Fe2 Sr1 La1 55.17(7) 101_455 . 1_565 N
Fe2 Sr1 La1 124.83(7) 101_455 . 1_655 N
Fe2 Sr1 Sr1 55.17(7) 101_455 . 1_455 N
Fe2 Sr1 Sr1 124.83(7) 101_455 . 1_545 N
Fe2 Sr1 Sr1 55.17(7) 101_455 . 1_565 N
Fe2 Sr1 Sr1 124.83(7) 101_455 . 1_655 N
Fe2 Sr1 La2 53.87(13) 101_455 . 1_555 N
Fe2 Sr1 Sr2 53.87(13) 101_455 . 1_555 N
Fe2 Sr1 O1 34.91(7) 101_455 . 101_445 N
Fe2 Sr1 O1 90.62(28) 101_455 . 101_545 N
Fe2 Sr1 O1 90.62(28) 101_455 . 102_545 N
Fe2 Sr1 O1 34.91(7) 101_455 . 102_555 N
Fe2 Sr1 O2 95.37(12) 101_455 . 101_445 N
Fe2 Sr1 O2 45.27(21) 101_455 . 101_455 N
Fe2 Sr1 O2 153.01(29) 101_455 . 101_545 N
Fe2 Sr1 O2 95.37(12) 101_455 . 101_555 N
Fe2 Sr1 O4 112.8(9) 101_455 . 101_445 N
Fe2 Sr1 O4 144.6(10) 101_455 . 102_545 N
Fe2 Sr1 O4 134.4(11) 101_455 . 103_555 N
Fe2 Sr1 Fe2 69.66(14) 101_545 . 101_555 N
Fe2 Sr1 La1 124.83(7) 101_545 . 1_455 N
Fe2 Sr1 La1 55.17(7) 101_545 . 1_545 N
Fe2 Sr1 La1 124.83(7) 101_545 . 1_565 N
Fe2 Sr1 La1 55.17(7) 101_545 . 1_655 N
Fe2 Sr1 Sr1 124.83(7) 101_545 . 1_455 N
Fe2 Sr1 Sr1 55.17(7) 101_545 . 1_545 N
Fe2 Sr1 Sr1 124.83(7) 101_545 . 1_565 N
Fe2 Sr1 Sr1 55.17(7) 101_545 . 1_655 N
Fe2 Sr1 La2 53.87(13) 101_545 . 1_555 N
Fe2 Sr1 Sr2 53.87(13) 101_545 . 1_555 N
Fe2 Sr1 O1 90.62(28) 101_545 . 101_445 N
Fe2 Sr1 O1 34.91(7) 101_545 . 101_545 N
Fe2 Sr1 O1 34.91(7) 101_545 . 102_545 N
Fe2 Sr1 O1 90.62(28) 101_545 . 102_555 N
Fe2 Sr1 O2 95.37(12) 101_545 . 101_445 N
Fe2 Sr1 O2 153.01(29) 101_545 . 101_455 N
Fe2 Sr1 O2 45.27(21) 101_545 . 101_545 N
Fe2 Sr1 O2 95.37(12) 101_545 . 101_555 N
Fe2 Sr1 O4 134.4(11) 101_545 . 101_445 N
Fe2 Sr1 O4 105.8(9) 101_545 . 102_545 N
Fe2 Sr1 O4 112.8(9) 101_545 . 103_555 N
Fe2 Sr1 La1 124.83(7) 101_555 . 1_455 N
Fe2 Sr1 La1 124.83(7) 101_555 . 1_545 N
Fe2 Sr1 La1 55.17(7) 101_555 . 1_565 N
Fe2 Sr1 La1 55.17(7) 101_555 . 1_655 N
Fe2 Sr1 Sr1 124.83(7) 101_555 . 1_455 N
Fe2 Sr1 Sr1 124.83(7) 101_555 . 1_545 N
Fe2 Sr1 Sr1 55.17(7) 101_555 . 1_565 N
Fe2 Sr1 Sr1 55.17(7) 101_555 . 1_655 N
Fe2 Sr1 La2 53.87(13) 101_555 . 1_555 N
Fe2 Sr1 Sr2 53.87(13) 101_555 . 1_555 N
Fe2 Sr1 O1 90.62(28) 101_555 . 101_445 N
Fe2 Sr1 O1 34.91(7) 101_555 . 101_545 N
Fe2 Sr1 O1 90.62(28) 101_555 . 102_545 N
Fe2 Sr1 O1 34.91(7) 101_555 . 102_555 N
Fe2 Sr1 O2 153.01(29) 101_555 . 101_445 N
Fe2 Sr1 O2 95.37(12) 101_555 . 101_455 N
Fe2 Sr1 O2 95.37(12) 101_555 . 101_545 N
Fe2 Sr1 O2 45.27(21) 101_555 . 101_555 N
Fe2 Sr1 O4 144.6(10) 101_555 . 101_445 N
Fe2 Sr1 O4 134.4(11) 101_555 . 102_545 N
Fe2 Sr1 O4 105.8(9) 101_555 . 103_555 N
La1 Sr1 La1 90.0 1_455 . 1_545 N
La1 Sr1 La1 90.0 1_455 . 1_565 N
La1 Sr1 La1 180.0 1_455 . 1_655 N
La1 Sr1 Sr1 0.0 1_455 . 1_455 N
La1 Sr1 Sr1 90.0 1_455 . 1_545 N
La1 Sr1 Sr1 90.0 1_455 . 1_565 N
La1 Sr1 Sr1 180.0 1_455 . 1_655 N
La1 Sr1 La2 90.0 1_455 . 1_555 N
La1 Sr1 Sr2 90.0 1_455 . 1_555 N
La1 Sr1 O1 43.33(24) 1_455 . 101_445 N
La1 Sr1 O1 136.67(24) 1_455 . 101_545 N
La1 Sr1 O1 90.0 1_455 . 102_545 N
La1 Sr1 O1 90.0 1_455 . 102_555 N
La1 Sr1 O2 45.723(34) 1_455 . 101_445 N
La1 Sr1 O2 45.723(34) 1_455 . 101_455 N
La1 Sr1 O2 134.277(34) 1_455 . 101_545 N
La1 Sr1 O2 134.277(34) 1_455 . 101_555 N
La1 Sr1 O4 68.0(8) 1_455 . 101_445 N
La1 Sr1 O4 95.8(11) 1_455 . 102_545 N
La1 Sr1 O4 112.0(8) 1_455 . 103_555 N
La1 Sr1 La1 180.0 1_545 . 1_565 N
La1 Sr1 La1 90.0 1_545 . 1_655 N
La1 Sr1 Sr1 90.0 1_545 . 1_455 N
La1 Sr1 Sr1 0.0 1_545 . 1_545 N
La1 Sr1 Sr1 180.0 1_545 . 1_565 N
La1 Sr1 Sr1 90.0 1_545 . 1_655 N
La1 Sr1 La2 90.0 1_545 . 1_555 N
La1 Sr1 Sr2 90.0 1_545 . 1_555 N
La1 Sr1 O1 90.0 1_545 . 101_445 N
La1 Sr1 O1 90.0 1_545 . 101_545 N
La1 Sr1 O1 43.33(24) 1_545 . 102_545 N
La1 Sr1 O1 136.67(24) 1_545 . 102_555 N
La1 Sr1 O2 45.723(34) 1_545 . 101_445 N
La1 Sr1 O2 134.277(34) 1_545 . 101_455 N
La1 Sr1 O2 45.723(34) 1_545 . 101_545 N
La1 Sr1 O2 134.277(34) 1_545 . 101_555 N
La1 Sr1 O4 84.2(11) 1_545 . 101_445 N
La1 Sr1 O4 68.0(8) 1_545 . 102_545 N
La1 Sr1 O4 95.8(11) 1_545 . 103_555 N
La1 Sr1 La1 90.0 1_565 . 1_655 N
La1 Sr1 Sr1 90.0 1_565 . 1_455 N
La1 Sr1 Sr1 180.0 1_565 . 1_545 N
La1 Sr1 Sr1 0.0 1_565 . 1_565 N
La1 Sr1 Sr1 90.0 1_565 . 1_655 N
La1 Sr1 La2 90.0 1_565 . 1_555 N
La1 Sr1 Sr2 90.0 1_565 . 1_555 N
La1 Sr1 O1 90.0 1_565 . 101_445 N
La1 Sr1 O1 90.0 1_565 . 101_545 N
La1 Sr1 O1 136.67(24) 1_565 . 102_545 N
La1 Sr1 O1 43.33(24) 1_565 . 102_555 N
La1 Sr1 O2 134.277(34) 1_565 . 101_445 N
La1 Sr1 O2 45.723(34) 1_565 . 101_455 N
La1 Sr1 O2 134.277(34) 1_565 . 101_545 N
La1 Sr1 O2 45.723(34) 1_565 . 101_555 N
La1 Sr1 O4 95.8(11) 1_565 . 101_445 N
La1 Sr1 O4 112.0(8) 1_565 . 102_545 N
La1 Sr1 O4 84.2(11) 1_565 . 103_555 N
La1 Sr1 Sr1 180.0 1_655 . 1_455 N
La1 Sr1 Sr1 90.0 1_655 . 1_545 N
La1 Sr1 Sr1 90.0 1_655 . 1_565 N
La1 Sr1 Sr1 0.0 1_655 . 1_655 N
La1 Sr1 La2 90.0 1_655 . 1_555 N
La1 Sr1 Sr2 90.0 1_655 . 1_555 N
La1 Sr1 O1 136.67(24) 1_655 . 101_445 N
La1 Sr1 O1 43.33(24) 1_655 . 101_545 N
La1 Sr1 O1 90.0 1_655 . 102_545 N
La1 Sr1 O1 90.0 1_655 . 102_555 N
La1 Sr1 O2 134.277(34) 1_655 . 101_445 N
La1 Sr1 O2 134.277(34) 1_655 . 101_455 N
La1 Sr1 O2 45.723(34) 1_655 . 101_545 N
La1 Sr1 O2 45.723(34) 1_655 . 101_555 N
La1 Sr1 O4 112.0(8) 1_655 . 101_445 N
La1 Sr1 O4 84.2(11) 1_655 . 102_545 N
La1 Sr1 O4 68.0(8) 1_655 . 103_555 N
Sr1 Sr1 Sr1 90.0 1_455 . 1_545 N
Sr1 Sr1 Sr1 90.0 1_455 . 1_565 N
Sr1 Sr1 Sr1 180.0 1_455 . 1_655 N
Sr1 Sr1 La2 90.0 1_455 . 1_555 N
Sr1 Sr1 Sr2 90.0 1_455 . 1_555 N
Sr1 Sr1 O1 43.33(24) 1_455 . 101_445 N
Sr1 Sr1 O1 136.67(24) 1_455 . 101_545 N
Sr1 Sr1 O1 90.0 1_455 . 102_545 N
Sr1 Sr1 O1 90.0 1_455 . 102_555 N
Sr1 Sr1 O2 45.723(34) 1_455 . 101_445 N
Sr1 Sr1 O2 45.723(34) 1_455 . 101_455 N
Sr1 Sr1 O2 134.277(34) 1_455 . 101_545 N
Sr1 Sr1 O2 134.277(34) 1_455 . 101_555 N
Sr1 Sr1 O4 68.0(8) 1_455 . 101_445 N
Sr1 Sr1 O4 95.8(11) 1_455 . 102_545 N
Sr1 Sr1 O4 112.0(8) 1_455 . 103_555 N
Sr1 Sr1 Sr1 180.0 1_545 . 1_565 N
Sr1 Sr1 Sr1 90.0 1_545 . 1_655 N
Sr1 Sr1 La2 90.0 1_545 . 1_555 N
Sr1 Sr1 Sr2 90.0 1_545 . 1_555 N
Sr1 Sr1 O1 90.0 1_545 . 101_445 N
Sr1 Sr1 O1 90.0 1_545 . 101_545 N
Sr1 Sr1 O1 43.33(24) 1_545 . 102_545 N
Sr1 Sr1 O1 136.67(24) 1_545 . 102_555 N
Sr1 Sr1 O2 45.723(34) 1_545 . 101_445 N
Sr1 Sr1 O2 134.277(34) 1_545 . 101_455 N
Sr1 Sr1 O2 45.723(34) 1_545 . 101_545 N
Sr1 Sr1 O2 134.277(34) 1_545 . 101_555 N
Sr1 Sr1 O4 84.2(11) 1_545 . 101_445 N
Sr1 Sr1 O4 68.0(8) 1_545 . 102_545 N
Sr1 Sr1 O4 95.8(11) 1_545 . 103_555 N
Sr1 Sr1 Sr1 90.0 1_565 . 1_655 N
Sr1 Sr1 La2 90.0 1_565 . 1_555 N
Sr1 Sr1 Sr2 90.0 1_565 . 1_555 N
Sr1 Sr1 O1 90.0 1_565 . 101_445 N
Sr1 Sr1 O1 90.0 1_565 . 101_545 N
Sr1 Sr1 O1 136.67(24) 1_565 . 102_545 N
Sr1 Sr1 O1 43.33(24) 1_565 . 102_555 N
Sr1 Sr1 O2 134.277(34) 1_565 . 101_445 N
Sr1 Sr1 O2 45.723(34) 1_565 . 101_455 N
Sr1 Sr1 O2 134.277(34) 1_565 . 101_545 N
Sr1 Sr1 O2 45.723(34) 1_565 . 101_555 N
Sr1 Sr1 O4 95.8(11) 1_565 . 101_445 N
Sr1 Sr1 O4 112.0(8) 1_565 . 102_545 N
Sr1 Sr1 O4 84.2(11) 1_565 . 103_555 N
Sr1 Sr1 La2 90.0 1_655 . 1_555 N
Sr1 Sr1 Sr2 90.0 1_655 . 1_555 N
Sr1 Sr1 O1 136.67(24) 1_655 . 101_445 N
Sr1 Sr1 O1 43.33(24) 1_655 . 101_545 N
Sr1 Sr1 O1 90.0 1_655 . 102_545 N
Sr1 Sr1 O1 90.0 1_655 . 102_555 N
Sr1 Sr1 O2 134.277(34) 1_655 . 101_445 N
Sr1 Sr1 O2 134.277(34) 1_655 . 101_455 N
Sr1 Sr1 O2 45.723(34) 1_655 . 101_545 N
Sr1 Sr1 O2 45.723(34) 1_655 . 101_555 N
Sr1 Sr1 O4 112.0(8) 1_655 . 101_445 N
Sr1 Sr1 O4 84.2(11) 1_655 . 102_545 N
Sr1 Sr1 O4 68.0(8) 1_655 . 103_555 N
La2 Sr1 Sr2 0.0 1_555 . 1_555 N
La2 Sr1 O1 46.67(24) 1_555 . 101_445 N
La2 Sr1 O1 46.67(24) 1_555 . 101_545 N
La2 Sr1 O1 46.67(24) 1_555 . 102_545 N
La2 Sr1 O1 46.67(24) 1_555 . 102_555 N
La2 Sr1 O2 99.14(22) 1_555 . 101_445 N
La2 Sr1 O2 99.14(22) 1_555 . 101_455 N
La2 Sr1 O2 99.14(22) 1_555 . 101_545 N
La2 Sr1 O2 99.14(22) 1_555 . 101_555 N
La2 Sr1 O4 157.2(8) 1_555 . 101_445 N
La2 Sr1 O4 157.2(8) 1_555 . 102_545 N
La2 Sr1 O4 157.2(8) 1_555 . 103_555 N
Sr2 Sr1 O1 46.67(24) 1_555 . 101_445 N
Sr2 Sr1 O1 46.67(24) 1_555 . 101_545 N
Sr2 Sr1 O1 46.67(24) 1_555 . 102_545 N
Sr2 Sr1 O1 46.67(24) 1_555 . 102_555 N
Sr2 Sr1 O2 99.14(22) 1_555 . 101_445 N
Sr2 Sr1 O2 99.14(22) 1_555 . 101_455 N
Sr2 Sr1 O2 99.14(22) 1_555 . 101_545 N
Sr2 Sr1 O2 99.14(22) 1_555 . 101_555 N
Sr2 Sr1 O4 157.2(8) 1_555 . 101_445 N
Sr2 Sr1 O4 157.2(8) 1_555 . 102_545 N
Sr2 Sr1 O4 157.2(8) 1_555 . 103_555 N
O1 Sr1 O1 93.3(5) 101_445 . 101_545 N
O1 Sr1 O1 61.91(27) 101_445 . 102_545 N
O1 Sr1 O1 61.91(27) 101_445 . 102_555 N
O1 Sr1 O2 66.50(16) 101_445 . 101_445 N
O1 Sr1 O2 66.50(16) 101_445 . 101_455 N
O1 Sr1 O2 128.08(24) 101_445 . 101_545 N
O1 Sr1 O2 128.08(24) 101_445 . 101_555 N
O1 Sr1 O4 111.1(8) 101_445 . 101_445 N
O1 Sr1 O4 134.9(10) 101_445 . 102_545 N
O1 Sr1 O4 154.8(9) 101_445 . 103_555 N
O1 Sr1 O1 61.91(27) 101_545 . 102_545 N
O1 Sr1 O1 61.91(27) 101_545 . 102_555 N
O1 Sr1 O2 128.08(24) 101_545 . 101_445 N
O1 Sr1 O2 128.08(24) 101_545 . 101_455 N
O1 Sr1 O2 66.50(16) 101_545 . 101_545 N
O1 Sr1 O2 66.50(16) 101_545 . 101_555 N
O1 Sr1 O4 154.8(9) 101_545 . 101_445 N
O1 Sr1 O4 124.0(11) 101_545 . 102_545 N
O1 Sr1 O4 111.1(8) 101_545 . 103_555 N
O1 Sr1 O1 93.3(5) 102_545 . 102_555 N
O1 Sr1 O2 66.50(16) 102_545 . 101_445 N
O1 Sr1 O2 128.08(24) 102_545 . 101_455 N
O1 Sr1 O2 66.50(16) 102_545 . 101_545 N
O1 Sr1 O2 128.08(24) 102_545 . 101_555 N
O1 Sr1 O4 124.0(11) 102_545 . 101_445 N
O1 Sr1 O4 111.1(8) 102_545 . 102_545 N
O1 Sr1 O4 134.9(10) 102_545 . 103_555 N
O1 Sr1 O2 128.08(24) 102_555 . 101_445 N
O1 Sr1 O2 66.50(16) 102_555 . 101_455 N
O1 Sr1 O2 128.08(24) 102_555 . 101_545 N
O1 Sr1 O2 66.50(16) 102_555 . 101_555 N
O1 Sr1 O4 134.9(10) 102_555 . 101_445 N
O1 Sr1 O4 154.8(9) 102_555 . 102_545 N
O1 Sr1 O4 124.0(11) 102_555 . 103_555 N
O2 Sr1 O2 88.55(7) 101_445 . 101_455 N
O2 Sr1 O2 88.55(7) 101_445 . 101_545 N
O2 Sr1 O2 161.7(4) 101_445 . 101_555 N
O2 Sr1 O4 61.4(9) 101_445 . 101_445 N
O2 Sr1 O4 70.3(10) 101_445 . 102_545 N
O2 Sr1 O4 100.7(10) 101_445 . 103_555 N
O2 Sr1 O2 161.7(4) 101_455 . 101_545 N
O2 Sr1 O2 88.55(7) 101_455 . 101_555 N
O2 Sr1 O4 70.3(10) 101_455 . 101_445 N
O2 Sr1 O4 100.7(10) 101_455 . 102_545 N
O2 Sr1 O4 92.5(10) 101_455 . 103_555 N
O2 Sr1 O2 88.55(7) 101_545 . 101_555 N
O2 Sr1 O4 92.5(10) 101_545 . 101_445 N
O2 Sr1 O4 61.4(9) 101_545 . 102_545 N
O2 Sr1 O4 70.3(10) 101_545 . 103_555 N
O2 Sr1 O4 100.7(10) 101_555 . 101_445 N
O2 Sr1 O4 92.5(10) 101_555 . 102_545 N
O2 Sr1 O4 61.4(9) 101_555 . 103_555 N
O4 Sr1 O4 31.8(11) 101_445 . 102_545 N
O4 Sr1 O4 45.6(16) 101_445 . 103_555 N
O4 Sr1 O4 31.8(11) 102_545 . 103_555 N
La1 La2 Sr1 0.0 1_555 . 1_555 N
La1 La2 Sr2 90.0 1_555 . 1_455 N
La1 La2 Sr2 90.0 1_555 . 1_545 N
La1 La2 Sr2 90.0 1_555 . 1_565 N
La1 La2 Sr2 90.0 1_555 . 1_655 N
La1 La2 Sr2 135.62(12) 1_555 . -101_335 N
La1 La2 Sr2 135.62(12) 1_555 . -101_345 N
La1 La2 Sr2 135.62(12) 1_555 . -101_435 N
La1 La2 Sr2 135.62(12) 1_555 . -101_445 N
La1 La2 O1 44.82(19) 1_555 . 101_445 N
La1 La2 O1 44.82(19) 1_555 . 101_545 N
La1 La2 O1 44.82(19) 1_555 . 102_545 N
La1 La2 O1 44.82(19) 1_555 . 102_555 N
La1 La2 O3 179.944 1_555 . -1_556 N
La1 La2 O3 96.68(20) 1_555 . 101_445 N
La1 La2 O3 96.68(20) 1_555 . 101_455 N
La1 La2 O3 96.68(20) 1_555 . 101_545 N
La1 La2 O3 96.68(20) 1_555 . 101_555 N
Sr1 La2 Sr2 90.0 1_555 . 1_455 N
Sr1 La2 Sr2 90.0 1_555 . 1_545 N
Sr1 La2 Sr2 90.0 1_555 . 1_565 N
Sr1 La2 Sr2 90.0 1_555 . 1_655 N
Sr1 La2 Sr2 135.62(12) 1_555 . -101_335 N
Sr1 La2 Sr2 135.62(12) 1_555 . -101_345 N
Sr1 La2 Sr2 135.62(12) 1_555 . -101_435 N
Sr1 La2 Sr2 135.62(12) 1_555 . -101_445 N
Sr1 La2 O1 44.82(19) 1_555 . 101_445 N
Sr1 La2 O1 44.82(19) 1_555 . 101_545 N
Sr1 La2 O1 44.82(19) 1_555 . 102_545 N
Sr1 La2 O1 44.82(19) 1_555 . 102_555 N
Sr1 La2 O3 179.944 1_555 . -1_556 N
Sr1 La2 O3 96.68(20) 1_555 . 101_445 N
Sr1 La2 O3 96.68(20) 1_555 . 101_455 N
Sr1 La2 O3 96.68(20) 1_555 . 101_545 N
Sr1 La2 O3 96.68(20) 1_555 . 101_555 N
Sr2 La2 Sr2 90.0 1_455 . 1_545 N
Sr2 La2 Sr2 90.0 1_455 . 1_565 N
Sr2 La2 Sr2 180.0 1_455 . 1_655 N
Sr2 La2 Sr2 60.36(7) 1_455 . -101_335 N
Sr2 La2 Sr2 60.36(7) 1_455 . -101_345 N
Sr2 La2 Sr2 119.64(7) 1_455 . -101_435 N
Sr2 La2 Sr2 119.64(7) 1_455 . -101_445 N
Sr2 La2 O1 45.18(19) 1_455 . 101_445 N
Sr2 La2 O1 134.82(19) 1_455 . 101_545 N
Sr2 La2 O1 90.0 1_455 . 102_545 N
Sr2 La2 O1 90.0 1_455 . 102_555 N
Sr2 La2 O3 90.0 1_455 . -1_556 N
Sr2 La2 O3 45.388(23) 1_455 . 101_445 N
Sr2 La2 O3 45.388(23) 1_455 . 101_455 N
Sr2 La2 O3 134.612(23) 1_455 . 101_545 N
Sr2 La2 O3 134.612(23) 1_455 . 101_555 N
Sr2 La2 Sr2 180.0 1_545 . 1_565 N
Sr2 La2 Sr2 90.0 1_545 . 1_655 N
Sr2 La2 Sr2 60.36(7) 1_545 . -101_335 N
Sr2 La2 Sr2 119.64(7) 1_545 . -101_345 N
Sr2 La2 Sr2 60.36(7) 1_545 . -101_435 N
Sr2 La2 Sr2 119.64(7) 1_545 . -101_445 N
Sr2 La2 O1 90.0 1_545 . 101_445 N
Sr2 La2 O1 90.0 1_545 . 101_545 N
Sr2 La2 O1 45.18(19) 1_545 . 102_545 N
Sr2 La2 O1 134.82(19) 1_545 . 102_555 N
Sr2 La2 O3 90.0 1_545 . -1_556 N
Sr2 La2 O3 45.388(23) 1_545 . 101_445 N
Sr2 La2 O3 134.612(23) 1_545 . 101_455 N
Sr2 La2 O3 45.388(23) 1_545 . 101_545 N
Sr2 La2 O3 134.612(23) 1_545 . 101_555 N
Sr2 La2 Sr2 90.0 1_565 . 1_655 N
Sr2 La2 Sr2 119.64(7) 1_565 . -101_335 N
Sr2 La2 Sr2 60.36(7) 1_565 . -101_345 N
Sr2 La2 Sr2 119.64(7) 1_565 . -101_435 N
Sr2 La2 Sr2 60.36(7) 1_565 . -101_445 N
Sr2 La2 O1 90.0 1_565 . 101_445 N
Sr2 La2 O1 90.0 1_565 . 101_545 N
Sr2 La2 O1 134.82(19) 1_565 . 102_545 N
Sr2 La2 O1 45.18(19) 1_565 . 102_555 N
Sr2 La2 O3 90.0 1_565 . -1_556 N
Sr2 La2 O3 134.612(23) 1_565 . 101_445 N
Sr2 La2 O3 45.388(23) 1_565 . 101_455 N
Sr2 La2 O3 134.612(23) 1_565 . 101_545 N
Sr2 La2 O3 45.388(23) 1_565 . 101_555 N
Sr2 La2 Sr2 119.64(7) 1_655 . -101_335 N
Sr2 La2 Sr2 119.64(7) 1_655 . -101_345 N
Sr2 La2 Sr2 60.36(7) 1_655 . -101_435 N
Sr2 La2 Sr2 60.36(7) 1_655 . -101_445 N
Sr2 La2 O1 134.82(19) 1_655 . 101_445 N
Sr2 La2 O1 45.18(19) 1_655 . 101_545 N
Sr2 La2 O1 90.0 1_655 . 102_545 N
Sr2 La2 O1 90.0 1_655 . 102_555 N
Sr2 La2 O3 90.0 1_655 . -1_556 N
Sr2 La2 O3 134.612(23) 1_655 . 101_445 N
Sr2 La2 O3 134.612(23) 1_655 . 101_455 N
Sr2 La2 O3 45.388(23) 1_655 . 101_545 N
Sr2 La2 O3 45.388(23) 1_655 . 101_555 N
Sr2 La2 Sr2 59.28(14) -101_335 . -101_345 N
Sr2 La2 Sr2 59.28(14) -101_335 . -101_435 N
Sr2 La2 Sr2 88.75(25) -101_335 . -101_445 N
Sr2 La2 O1 99.11(11) -101_335 . 101_445 N
Sr2 La2 O1 148.82(4) -101_335 . 101_545 N
Sr2 La2 O1 99.11(11) -101_335 . 102_545 N
Sr2 La2 O1 148.82(4) -101_335 . 102_555 N
Sr2 La2 O3 44.38(12) -101_446 . -1_556 N
Sr2 La2 O3 38.94(17) -101_446 . 101_445 N
Sr2 La2 O3 85.23(14) -101_446 . 101_455 N
Sr2 La2 O3 85.23(14) -101_446 . 101_545 N
Sr2 La2 O3 127.70(28) -101_446 . 101_555 N
Sr2 La2 Sr2 88.75(25) -101_345 . -101_435 N
Sr2 La2 Sr2 59.28(14) -101_345 . -101_445 N
Sr2 La2 O1 99.11(11) -101_345 . 101_445 N
Sr2 La2 O1 148.82(4) -101_345 . 101_545 N
Sr2 La2 O1 148.82(4) -101_345 . 102_545 N
Sr2 La2 O1 99.11(11) -101_345 . 102_555 N
Sr2 La2 O3 44.38(12) -101_456 . -1_556 N
Sr2 La2 O3 85.23(14) -101_456 . 101_445 N
Sr2 La2 O3 38.94(17) -101_456 . 101_455 N
Sr2 La2 O3 127.70(28) -101_456 . 101_545 N
Sr2 La2 O3 85.23(14) -101_456 . 101_555 N
Sr2 La2 Sr2 59.28(14) -101_435 . -101_445 N
Sr2 La2 O1 148.82(4) -101_435 . 101_445 N
Sr2 La2 O1 99.11(11) -101_435 . 101_545 N
Sr2 La2 O1 99.11(11) -101_435 . 102_545 N
Sr2 La2 O1 148.82(4) -101_435 . 102_555 N
Sr2 La2 O3 44.38(12) -101_546 . -1_556 N
Sr2 La2 O3 85.23(14) -101_546 . 101_445 N
Sr2 La2 O3 127.70(28) -101_546 . 101_455 N
Sr2 La2 O3 38.94(17) -101_546 . 101_545 N
Sr2 La2 O3 85.23(14) -101_546 . 101_555 N
Sr2 La2 O1 148.82(4) -101_445 . 101_445 N
Sr2 La2 O1 99.11(11) -101_445 . 101_545 N
Sr2 La2 O1 148.82(4) -101_445 . 102_545 N
Sr2 La2 O1 99.11(11) -101_445 . 102_555 N
Sr2 La2 O3 44.38(12) -101_556 . -1_556 N
Sr2 La2 O3 127.70(28) -101_556 . 101_445 N
Sr2 La2 O3 85.23(14) -101_556 . 101_455 N
Sr2 La2 O3 85.23(14) -101_556 . 101_545 N
Sr2 La2 O3 38.94(17) -101_556 . 101_555 N
O1 La2 O1 89.6(4) 101_445 . 101_545 N
O1 La2 O1 59.79(21) 101_445 . 102_545 N
O1 La2 O1 59.79(21) 101_445 . 102_555 N
O1 La2 O3 135.18(19) 101_445 . -1_556 N
O1 La2 O3 65.64(18) 101_445 . 101_445 N
O1 La2 O3 65.64(18) 101_445 . 101_455 N
O1 La2 O3 125.28(20) 101_445 . 101_545 N
O1 La2 O3 125.28(20) 101_445 . 101_555 N
O1 La2 O1 59.79(21) 101_545 . 102_545 N
O1 La2 O1 59.79(21) 101_545 . 102_555 N
O1 La2 O3 135.18(19) 101_545 . -1_556 N
O1 La2 O3 125.28(20) 101_545 . 101_445 N
O1 La2 O3 125.28(20) 101_545 . 101_455 N
O1 La2 O3 65.64(18) 101_545 . 101_545 N
O1 La2 O3 65.64(18) 101_545 . 101_555 N
O1 La2 O1 89.6(4) 102_545 . 102_555 N
O1 La2 O3 135.18(19) 102_545 . -1_556 N
O1 La2 O3 65.64(18) 102_545 . 101_445 N
O1 La2 O3 125.28(20) 102_545 . 101_455 N
O1 La2 O3 65.64(18) 102_545 . 101_545 N
O1 La2 O3 125.28(20) 102_545 . 101_555 N
O1 La2 O3 135.18(19) 102_555 . -1_556 N
O1 La2 O3 125.28(20) 102_555 . 101_445 N
O1 La2 O3 65.64(18) 102_555 . 101_455 N
O1 La2 O3 125.28(20) 102_555 . 101_545 N
O1 La2 O3 65.64(18) 102_555 . 101_555 N
O3 La2 O3 83.32(20) -1_556 . 101_445 N
O3 La2 O3 83.32(20) -1_556 . 101_455 N
O3 La2 O3 83.32(20) -1_556 . 101_545 N
O3 La2 O3 83.32(20) -1_556 . 101_555 N
O3 La2 O3 89.22(5) 101_445 . 101_455 N
O3 La2 O3 89.22(5) 101_445 . 101_545 N
O3 La2 O3 166.6(4) 101_445 . 101_555 N
O3 La2 O3 166.6(4) 101_455 . 101_545 N
O3 La2 O3 89.22(5) 101_455 . 101_555 N
O3 La2 O3 89.22(5) 101_545 . 101_555 N
Fe2 Sr2 Fe2 72.77(11) 101_445 . 101_455 N
Fe2 Sr2 Fe2 72.77(11) 101_445 . 101_545 N
Fe2 Sr2 Fe2 114.06(24) 101_445 . 101_555 N
Fe2 Sr2 La1 57.03(12) 101_445 . 1_555 N
Fe2 Sr2 Sr1 57.03(12) 101_445 . 1_555 N
Fe2 Sr2 La2 53.61(6) 101_445 . 1_455 N
Fe2 Sr2 La2 53.61(6) 101_445 . 1_545 N
Fe2 Sr2 La2 126.39(6) 101_445 . 1_565 N
Fe2 Sr2 La2 126.39(6) 101_445 . 1_655 N
Fe2 Sr2 La2 78.59(13) 101_445 . -101_335 N
Fe2 Sr2 La2 112.89(7) 101_445 . -101_345 N
Fe2 Sr2 La2 112.89(7) 101_445 . -101_435 N
Fe2 Sr2 La2 167.35(20) 101_445 . -101_445 N
Fe2 Sr2 Sr2 53.61(6) 101_445 . 1_455 N
Fe2 Sr2 Sr2 53.61(6) 101_445 . 1_545 N
Fe2 Sr2 Sr2 126.39(6) 101_445 . 1_565 N
Fe2 Sr2 Sr2 126.39(6) 101_445 . 1_655 N
Fe2 Sr2 Sr2 78.59(13) 101_445 . -101_335 N
Fe2 Sr2 Sr2 112.89(7) 101_445 . -101_345 N
Fe2 Sr2 Sr2 112.89(7) 101_445 . -101_435 N
Fe2 Sr2 Sr2 167.35(20) 101_445 . -101_445 N
Fe2 Sr2 O1 36.47(6) 101_445 . 101_445 N
Fe2 Sr2 O1 91.84(21) 101_445 . 101_545 N
Fe2 Sr2 O1 36.47(6) 101_445 . 102_545 N
Fe2 Sr2 Fe2 114.06(24) 101_455 . 101_545 N
Fe2 Sr2 Fe2 72.77(11) 101_455 . 101_555 N
Fe2 Sr2 La1 57.03(12) 101_455 . 1_555 N
Fe2 Sr2 Sr1 57.03(12) 101_455 . 1_555 N
Fe2 Sr2 La2 53.61(6) 101_455 . 1_455 N
Fe2 Sr2 La2 126.39(6) 101_455 . 1_545 N
Fe2 Sr2 La2 53.61(6) 101_455 . 1_565 N
Fe2 Sr2 La2 126.39(6) 101_455 . 1_655 N
Fe2 Sr2 La2 112.89(7) 101_455 . -101_335 N
Fe2 Sr2 La2 78.59(13) 101_455 . -101_345 N
Fe2 Sr2 La2 167.35(20) 101_455 . -101_435 N
Fe2 Sr2 La2 112.89(7) 101_455 . -101_445 N
Fe2 Sr2 Sr2 53.61(6) 101_455 . 1_455 N
Fe2 Sr2 Sr2 126.39(6) 101_455 . 1_545 N
Fe2 Sr2 Sr2 53.61(6) 101_455 . 1_565 N
Fe2 Sr2 Sr2 126.39(6) 101_455 . 1_655 N
Fe2 Sr2 Sr2 112.89(7) 101_455 . -101_335 N
Fe2 Sr2 Sr2 78.59(13) 101_455 . -101_345 N
Fe2 Sr2 Sr2 167.35(20) 101_455 . -101_435 N
Fe2 Sr2 Sr2 112.89(7) 101_455 . -101_445 N
Fe2 Sr2 O1 36.47(6) 101_455 . 101_445 N
Fe2 Sr2 O1 91.84(21) 101_455 . 101_545 N
Fe2 Sr2 O1 91.84(21) 101_455 . 102_545 N
Fe2 Sr2 Fe2 72.77(11) 101_545 . 101_555 N
Fe2 Sr2 La1 57.03(12) 101_545 . 1_555 N
Fe2 Sr2 Sr1 57.03(12) 101_545 . 1_555 N
Fe2 Sr2 La2 126.39(6) 101_545 . 1_455 N
Fe2 Sr2 La2 53.61(6) 101_545 . 1_545 N
Fe2 Sr2 La2 126.39(6) 101_545 . 1_565 N
Fe2 Sr2 La2 53.61(6) 101_545 . 1_655 N
Fe2 Sr2 La2 112.89(7) 101_545 . -101_335 N
Fe2 Sr2 La2 167.35(20) 101_545 . -101_345 N
Fe2 Sr2 La2 78.59(13) 101_545 . -101_435 N
Fe2 Sr2 La2 112.89(7) 101_545 . -101_445 N
Fe2 Sr2 Sr2 126.39(6) 101_545 . 1_455 N
Fe2 Sr2 Sr2 53.61(6) 101_545 . 1_545 N
Fe2 Sr2 Sr2 126.39(6) 101_545 . 1_565 N
Fe2 Sr2 Sr2 53.61(6) 101_545 . 1_655 N
Fe2 Sr2 Sr2 112.89(7) 101_545 . -101_335 N
Fe2 Sr2 Sr2 167.35(20) 101_545 . -101_345 N
Fe2 Sr2 Sr2 78.59(13) 101_545 . -101_435 N
Fe2 Sr2 Sr2 112.89(7) 101_545 . -101_445 N
Fe2 Sr2 O1 91.84(21) 101_545 . 101_445 N
Fe2 Sr2 O1 36.47(6) 101_545 . 101_545 N
Fe2 Sr2 O1 36.47(6) 101_545 . 102_545 N
Fe2 Sr2 La1 57.03(12) 101_555 . 1_555 N
Fe2 Sr2 Sr1 57.03(12) 101_555 . 1_555 N
Fe2 Sr2 La2 126.39(6) 101_555 . 1_455 N
Fe2 Sr2 La2 126.39(6) 101_555 . 1_545 N
Fe2 Sr2 La2 53.61(6) 101_555 . 1_565 N
Fe2 Sr2 La2 53.61(6) 101_555 . 1_655 N
Fe2 Sr2 La2 167.35(20) 101_555 . -101_335 N
Fe2 Sr2 La2 112.89(7) 101_555 . -101_345 N
Fe2 Sr2 La2 112.89(7) 101_555 . -101_435 N
Fe2 Sr2 La2 78.59(13) 101_555 . -101_445 N
Fe2 Sr2 Sr2 126.39(6) 101_555 . 1_455 N
Fe2 Sr2 Sr2 126.39(6) 101_555 . 1_545 N
Fe2 Sr2 Sr2 53.61(6) 101_555 . 1_565 N
Fe2 Sr2 Sr2 53.61(6) 101_555 . 1_655 N
Fe2 Sr2 Sr2 167.35(20) 101_555 . -101_335 N
Fe2 Sr2 Sr2 112.89(7) 101_555 . -101_345 N
Fe2 Sr2 Sr2 112.89(7) 101_555 . -101_435 N
Fe2 Sr2 Sr2 78.59(13) 101_555 . -101_445 N
Fe2 Sr2 O1 91.84(21) 101_555 . 101_445 N
Fe2 Sr2 O1 36.47(6) 101_555 . 101_545 N
Fe2 Sr2 O1 91.84(21) 101_555 . 102_545 N
La1 Sr2 Sr1 0.0 1_555 . 1_555 N
La1 Sr2 La2 90.0 1_555 . 1_455 N
La1 Sr2 La2 90.0 1_555 . 1_545 N
La1 Sr2 La2 90.0 1_555 . 1_565 N
La1 Sr2 La2 90.0 1_555 . 1_655 N
La1 Sr2 La2 135.62(12) 1_555 . -101_335 N
La1 Sr2 La2 135.62(12) 1_555 . -101_345 N
La1 Sr2 La2 135.62(12) 1_555 . -101_435 N
La1 Sr2 La2 135.62(12) 1_555 . -101_445 N
La1 Sr2 Sr2 90.0 1_555 . 1_455 N
La1 Sr2 Sr2 90.0 1_555 . 1_545 N
La1 Sr2 Sr2 90.0 1_555 . 1_565 N
La1 Sr2 Sr2 90.0 1_555 . 1_655 N
La1 Sr2 Sr2 135.62(12) 1_555 . -101_335 N
La1 Sr2 Sr2 135.62(12) 1_555 . -101_345 N
La1 Sr2 Sr2 135.62(12) 1_555 . -101_435 N
La1 Sr2 Sr2 135.62(12) 1_555 . -101_445 N
La1 Sr2 O1 44.82(19) 1_555 . 101_445 N
La1 Sr2 O1 44.82(19) 1_555 . 101_545 N
La1 Sr2 O1 44.82(19) 1_555 . 102_545 N
Sr1 Sr2 La2 90.0 1_555 . 1_455 N
Sr1 Sr2 La2 90.0 1_555 . 1_545 N
Sr1 Sr2 La2 90.0 1_555 . 1_565 N
Sr1 Sr2 La2 90.0 1_555 . 1_655 N
Sr1 Sr2 La2 135.62(12) 1_555 . -101_335 N
Sr1 Sr2 La2 135.62(12) 1_555 . -101_345 N
Sr1 Sr2 La2 135.62(12) 1_555 . -101_435 N
Sr1 Sr2 La2 135.62(12) 1_555 . -101_445 N
Sr1 Sr2 Sr2 90.0 1_555 . 1_455 N
Sr1 Sr2 Sr2 90.0 1_555 . 1_545 N
Sr1 Sr2 Sr2 90.0 1_555 . 1_565 N
Sr1 Sr2 Sr2 90.0 1_555 . 1_655 N
Sr1 Sr2 Sr2 135.62(12) 1_555 . -101_335 N
Sr1 Sr2 Sr2 135.62(12) 1_555 . -101_345 N
Sr1 Sr2 Sr2 135.62(12) 1_555 . -101_435 N
Sr1 Sr2 Sr2 135.62(12) 1_555 . -101_445 N
Sr1 Sr2 O1 44.82(19) 1_555 . 101_445 N
Sr1 Sr2 O1 44.82(19) 1_555 . 101_545 N
Sr1 Sr2 O1 44.82(19) 1_555 . 102_545 N
La2 Sr2 La2 90.0 1_455 . 1_545 N
La2 Sr2 La2 90.0 1_455 . 1_565 N
La2 Sr2 La2 180.0 1_455 . 1_655 N
La2 Sr2 La2 60.36(7) 1_455 . -101_335 N
La2 Sr2 La2 60.36(7) 1_455 . -101_345 N
La2 Sr2 La2 119.64(7) 1_455 . -101_435 N
La2 Sr2 La2 119.64(7) 1_455 . -101_445 N
La2 Sr2 Sr2 0.0 1_455 . 1_455 N
La2 Sr2 Sr2 90.0 1_455 . 1_545 N
La2 Sr2 Sr2 90.0 1_455 . 1_565 N
La2 Sr2 Sr2 180.0 1_455 . 1_655 N
La2 Sr2 Sr2 60.36(7) 1_455 . -101_335 N
La2 Sr2 Sr2 60.36(7) 1_455 . -101_345 N
La2 Sr2 Sr2 119.64(7) 1_455 . -101_435 N
La2 Sr2 Sr2 119.64(7) 1_455 . -101_445 N
La2 Sr2 O1 45.18(19) 1_455 . 101_445 N
La2 Sr2 O1 134.82(19) 1_455 . 101_545 N
La2 Sr2 O1 90.0 1_455 . 102_545 N
La2 Sr2 La2 180.0 1_545 . 1_565 N
La2 Sr2 La2 90.0 1_545 . 1_655 N
La2 Sr2 La2 60.36(7) 1_545 . -101_335 N
La2 Sr2 La2 119.64(7) 1_545 . -101_345 N
La2 Sr2 La2 60.36(7) 1_545 . -101_435 N
La2 Sr2 La2 119.64(7) 1_545 . -101_445 N
La2 Sr2 Sr2 90.0 1_545 . 1_455 N
La2 Sr2 Sr2 0.0 1_545 . 1_545 N
La2 Sr2 Sr2 180.0 1_545 . 1_565 N
La2 Sr2 Sr2 90.0 1_545 . 1_655 N
La2 Sr2 Sr2 60.36(7) 1_545 . -101_335 N
La2 Sr2 Sr2 119.64(7) 1_545 . -101_345 N
La2 Sr2 Sr2 60.36(7) 1_545 . -101_435 N
La2 Sr2 Sr2 119.64(7) 1_545 . -101_445 N
La2 Sr2 O1 90.0 1_545 . 101_445 N
La2 Sr2 O1 90.0 1_545 . 101_545 N
La2 Sr2 O1 45.18(19) 1_545 . 102_545 N
La2 Sr2 La2 90.0 1_565 . 1_655 N
La2 Sr2 La2 119.64(7) 1_565 . -101_335 N
La2 Sr2 La2 60.36(7) 1_565 . -101_345 N
La2 Sr2 La2 119.64(7) 1_565 . -101_435 N
La2 Sr2 La2 60.36(7) 1_565 . -101_445 N
La2 Sr2 Sr2 90.0 1_565 . 1_455 N
La2 Sr2 Sr2 180.0 1_565 . 1_545 N
La2 Sr2 Sr2 0.0 1_565 . 1_565 N
La2 Sr2 Sr2 90.0 1_565 . 1_655 N
La2 Sr2 Sr2 119.64(7) 1_565 . -101_335 N
La2 Sr2 Sr2 60.36(7) 1_565 . -101_345 N
La2 Sr2 Sr2 119.64(7) 1_565 . -101_435 N
La2 Sr2 Sr2 60.36(7) 1_565 . -101_445 N
La2 Sr2 O1 90.0 1_565 . 101_445 N
La2 Sr2 O1 90.0 1_565 . 101_545 N
La2 Sr2 O1 134.82(19) 1_565 . 102_545 N
La2 Sr2 La2 119.64(7) 1_655 . -101_335 N
La2 Sr2 La2 119.64(7) 1_655 . -101_345 N
La2 Sr2 La2 60.36(7) 1_655 . -101_435 N
La2 Sr2 La2 60.36(7) 1_655 . -101_445 N
La2 Sr2 Sr2 180.0 1_655 . 1_455 N
La2 Sr2 Sr2 90.0 1_655 . 1_545 N
La2 Sr2 Sr2 90.0 1_655 . 1_565 N
La2 Sr2 Sr2 0.0 1_655 . 1_655 N
La2 Sr2 Sr2 119.64(7) 1_655 . -101_335 N
La2 Sr2 Sr2 119.64(7) 1_655 . -101_345 N
La2 Sr2 Sr2 60.36(7) 1_655 . -101_435 N
La2 Sr2 Sr2 60.36(7) 1_655 . -101_445 N
La2 Sr2 O1 134.82(19) 1_655 . 101_445 N
La2 Sr2 O1 45.18(19) 1_655 . 101_545 N
La2 Sr2 O1 90.0 1_655 . 102_545 N
La2 Sr2 La2 59.28(14) -101_335 . -101_345 N
La2 Sr2 La2 59.28(14) -101_335 . -101_435 N
La2 Sr2 La2 88.75(25) -101_335 . -101_445 N
La2 Sr2 Sr2 60.36(7) -101_335 . 1_455 N
La2 Sr2 Sr2 60.36(7) -101_335 . 1_545 N
La2 Sr2 Sr2 119.64(7) -101_335 . 1_565 N
La2 Sr2 Sr2 119.64(7) -101_335 . 1_655 N
La2 Sr2 Sr2 0.0 -101_335 . -101_335 N
La2 Sr2 Sr2 59.28(14) -101_335 . -101_345 N
La2 Sr2 Sr2 59.28(14) -101_335 . -101_435 N
La2 Sr2 Sr2 88.75(25) -101_335 . -101_445 N
La2 Sr2 O1 99.11(11) -101_335 . 101_445 N
La2 Sr2 O1 148.82(4) -101_335 . 101_545 N
La2 Sr2 O1 99.11(11) -101_335 . 102_545 N
La2 Sr2 La2 88.75(25) -101_345 . -101_435 N
La2 Sr2 La2 59.28(14) -101_345 . -101_445 N
La2 Sr2 Sr2 60.36(7) -101_345 . 1_455 N
La2 Sr2 Sr2 119.64(7) -101_345 . 1_545 N
La2 Sr2 Sr2 60.36(7) -101_345 . 1_565 N
La2 Sr2 Sr2 119.64(7) -101_345 . 1_655 N
La2 Sr2 Sr2 59.28(14) -101_345 . -101_335 N
La2 Sr2 Sr2 0.0 -101_345 . -101_345 N
La2 Sr2 Sr2 88.75(25) -101_345 . -101_435 N
La2 Sr2 Sr2 59.28(14) -101_345 . -101_445 N
La2 Sr2 O1 99.11(11) -101_345 . 101_445 N
La2 Sr2 O1 148.82(4) -101_345 . 101_545 N
La2 Sr2 O1 148.82(4) -101_345 . 102_545 N
La2 Sr2 La2 59.28(14) -101_435 . -101_445 N
La2 Sr2 Sr2 119.64(7) -101_435 . 1_455 N
La2 Sr2 Sr2 60.36(7) -101_435 . 1_545 N
La2 Sr2 Sr2 119.64(7) -101_435 . 1_565 N
La2 Sr2 Sr2 60.36(7) -101_435 . 1_655 N
La2 Sr2 Sr2 59.28(14) -101_435 . -101_335 N
La2 Sr2 Sr2 88.75(25) -101_435 . -101_345 N
La2 Sr2 Sr2 0.0 -101_435 . -101_435 N
La2 Sr2 Sr2 59.28(14) -101_435 . -101_445 N
La2 Sr2 O1 148.82(4) -101_435 . 101_445 N
La2 Sr2 O1 99.11(11) -101_435 . 101_545 N
La2 Sr2 O1 99.11(11) -101_435 . 102_545 N
La2 Sr2 Sr2 119.64(7) -101_445 . 1_455 N
La2 Sr2 Sr2 119.64(7) -101_445 . 1_545 N
La2 Sr2 Sr2 60.36(7) -101_445 . 1_565 N
La2 Sr2 Sr2 60.36(7) -101_445 . 1_655 N
La2 Sr2 Sr2 88.75(25) -101_445 . -101_335 N
La2 Sr2 Sr2 59.28(14) -101_445 . -101_345 N
La2 Sr2 Sr2 59.28(14) -101_445 . -101_435 N
La2 Sr2 Sr2 0.0 -101_445 . -101_445 N
La2 Sr2 O1 148.82(4) -101_445 . 101_445 N
La2 Sr2 O1 99.11(11) -101_445 . 101_545 N
La2 Sr2 O1 148.82(4) -101_445 . 102_545 N
Sr2 Sr2 Sr2 90.0 1_455 . 1_545 N
Sr2 Sr2 Sr2 90.0 1_455 . 1_565 N
Sr2 Sr2 Sr2 180.0 1_455 . 1_655 N
Sr2 Sr2 Sr2 60.36(7) 1_455 . -101_335 N
Sr2 Sr2 Sr2 60.36(7) 1_455 . -101_345 N
Sr2 Sr2 Sr2 119.64(7) 1_455 . -101_435 N
Sr2 Sr2 Sr2 119.64(7) 1_455 . -101_445 N
Sr2 Sr2 O1 45.18(19) 1_455 . 101_445 N
Sr2 Sr2 O1 134.82(19) 1_455 . 101_545 N
Sr2 Sr2 O1 90.0 1_455 . 102_545 N
Sr2 Sr2 Sr2 180.0 1_545 . 1_565 N
Sr2 Sr2 Sr2 90.0 1_545 . 1_655 N
Sr2 Sr2 Sr2 60.36(7) 1_545 . -101_335 N
Sr2 Sr2 Sr2 119.64(7) 1_545 . -101_345 N
Sr2 Sr2 Sr2 60.36(7) 1_545 . -101_435 N
Sr2 Sr2 Sr2 119.64(7) 1_545 . -101_445 N
Sr2 Sr2 O1 90.0 1_545 . 101_445 N
Sr2 Sr2 O1 90.0 1_545 . 101_545 N
Sr2 Sr2 O1 45.18(19) 1_545 . 102_545 N
Sr2 Sr2 Sr2 90.0 1_565 . 1_655 N
Sr2 Sr2 Sr2 119.64(7) 1_565 . -101_335 N
Sr2 Sr2 Sr2 60.36(7) 1_565 . -101_345 N
Sr2 Sr2 Sr2 119.64(7) 1_565 . -101_435 N
Sr2 Sr2 Sr2 60.36(7) 1_565 . -101_445 N
Sr2 Sr2 O1 90.0 1_565 . 101_445 N
Sr2 Sr2 O1 90.0 1_565 . 101_545 N
Sr2 Sr2 O1 134.82(19) 1_565 . 102_545 N
Sr2 Sr2 Sr2 119.64(7) 1_655 . -101_335 N
Sr2 Sr2 Sr2 119.64(7) 1_655 . -101_345 N
Sr2 Sr2 Sr2 60.36(7) 1_655 . -101_435 N
Sr2 Sr2 Sr2 60.36(7) 1_655 . -101_445 N
Sr2 Sr2 O1 134.82(19) 1_655 . 101_445 N
Sr2 Sr2 O1 45.18(19) 1_655 . 101_545 N
Sr2 Sr2 O1 90.0 1_655 . 102_545 N
Sr2 Sr2 Sr2 59.28(14) -101_335 . -101_345 N
Sr2 Sr2 Sr2 59.28(14) -101_335 . -101_435 N
Sr2 Sr2 Sr2 88.75(25) -101_335 . -101_445 N
Sr2 Sr2 O1 99.11(11) -101_335 . 101_445 N
Sr2 Sr2 O1 148.82(4) -101_335 . 101_545 N
Sr2 Sr2 O1 99.11(11) -101_335 . 102_545 N
Sr2 Sr2 Sr2 88.75(25) -101_345 . -101_435 N
Sr2 Sr2 Sr2 59.28(14) -101_345 . -101_445 N
Sr2 Sr2 O1 99.11(11) -101_345 . 101_445 N
Sr2 Sr2 O1 148.82(4) -101_345 . 101_545 N
Sr2 Sr2 O1 148.82(4) -101_345 . 102_545 N
Sr2 Sr2 Sr2 59.28(14) -101_435 . -101_445 N
Sr2 Sr2 O1 148.82(4) -101_435 . 101_445 N
Sr2 Sr2 O1 99.11(11) -101_435 . 101_545 N
Sr2 Sr2 O1 99.11(11) -101_435 . 102_545 N
Sr2 Sr2 O1 148.82(4) -101_445 . 101_445 N
Sr2 Sr2 O1 99.11(11) -101_445 . 101_545 N
Sr2 Sr2 O1 148.82(4) -101_445 . 102_545 N
O1 Sr2 O1 89.6(4) 101_445 . 101_545 N
O1 Sr2 O1 59.79(21) 101_445 . 102_545 N
O1 Sr2 O1 59.79(21) 101_545 . 102_545 N
Fe2 O1 Fe2 169.8(7) 1_555 . 1_565 N
Fe2 O1 La1 93.48(23) 1_555 . 101_454 N
Fe2 O1 La1 93.48(23) 1_555 . 101_554 N
Fe2 O1 Sr1 93.48(23) 1_555 . 101_454 N
Fe2 O1 Sr1 93.48(23) 1_555 . 101_554 N
Fe2 O1 La2 86.40(26) 1_555 . 101_454 N
Fe2 O1 La2 86.40(26) 1_555 . 101_554 N
Fe2 O1 Sr2 86.40(26) 1_555 . 101_454 N
Fe2 O1 Sr2 86.40(26) 1_555 . 101_554 N
Fe2 O1 Co2 0.0 1_555 . 1_555 N
Fe2 O1 Co2 169.8(7) 1_555 . 1_565 N
Fe2 O1 La1 93.48(23) 1_565 . 101_454 N
Fe2 O1 La1 93.48(23) 1_565 . 101_554 N
Fe2 O1 Sr1 93.48(23) 1_565 . 101_454 N
Fe2 O1 Sr1 93.48(23) 1_565 . 101_554 N
Fe2 O1 La2 86.40(26) 1_565 . 101_454 N
Fe2 O1 La2 86.40(26) 1_565 . 101_554 N
Fe2 O1 Sr2 86.40(26) 1_565 . 101_454 N
Fe2 O1 Sr2 86.40(26) 1_565 . 101_554 N
Fe2 O1 Co2 169.8(7) 1_565 . 1_555 N
Fe2 O1 Co2 0.0 1_565 . 1_565 N
La1 O1 La1 93.3(5) 101_454 . 101_554 N
La1 O1 Sr1 0.0 101_454 . 101_454 N
La1 O1 Sr1 93.3(5) 101_454 . 101_554 N
La1 O1 La2 88.51(10) 101_454 . 101_454 N
La1 O1 La2 178.2(4) 101_454 . 101_554 N
La1 O1 Sr2 88.51(10) 101_454 . 101_454 N
La1 O1 Sr2 178.2(4) 101_454 . 101_554 N
La1 O1 Co2 93.48(23) 101_454 . 1_555 N
La1 O1 Co2 93.48(23) 101_454 . 1_565 N
La1 O1 Sr1 93.3(5) 101_554 . 101_454 N
La1 O1 Sr1 0.0 101_554 . 101_554 N
La1 O1 La2 178.2(4) 101_554 . 101_454 N
La1 O1 La2 88.51(10) 101_554 . 101_554 N
La1 O1 Sr2 178.2(4) 101_554 . 101_454 N
La1 O1 Sr2 88.51(10) 101_554 . 101_554 N
La1 O1 Co2 93.48(23) 101_554 . 1_555 N
La1 O1 Co2 93.48(23) 101_554 . 1_565 N
Sr1 O1 Sr1 93.3(5) 101_454 . 101_554 N
Sr1 O1 La2 88.51(10) 101_454 . 101_454 N
Sr1 O1 La2 178.2(4) 101_454 . 101_554 N
Sr1 O1 Sr2 88.51(10) 101_454 . 101_454 N
Sr1 O1 Sr2 178.2(4) 101_454 . 101_554 N
Sr1 O1 Co2 93.48(23) 101_454 . 1_555 N
Sr1 O1 Co2 93.48(23) 101_454 . 1_565 N
Sr1 O1 La2 178.2(4) 101_554 . 101_454 N
Sr1 O1 La2 88.51(10) 101_554 . 101_554 N
Sr1 O1 Sr2 178.2(4) 101_554 . 101_454 N
Sr1 O1 Sr2 88.51(10) 101_554 . 101_554 N
Sr1 O1 Co2 93.48(23) 101_554 . 1_555 N
Sr1 O1 Co2 93.48(23) 101_554 . 1_565 N
La2 O1 La2 89.6(4) 101_454 . 101_554 N
La2 O1 Sr2 0.0 101_454 . 101_454 N
La2 O1 Sr2 89.6(4) 101_454 . 101_554 N
La2 O1 Co2 86.40(26) 101_454 . 1_555 N
La2 O1 Co2 86.40(26) 101_454 . 1_565 N
La2 O1 Sr2 89.6(4) 101_554 . 101_454 N
La2 O1 Sr2 0.0 101_554 . 101_554 N
La2 O1 Co2 86.40(26) 101_554 . 1_555 N
La2 O1 Co2 86.40(26) 101_554 . 1_565 N
Sr2 O1 Sr2 89.6(4) 101_454 . 101_554 N
Sr2 O1 Co2 86.40(26) 101_454 . 1_555 N
Sr2 O1 Co2 86.40(26) 101_454 . 1_565 N
Sr2 O1 Co2 86.40(26) 101_554 . 1_555 N
Sr2 O1 Co2 86.40(26) 101_554 . 1_565 N
Co2 O1 Co2 169.8(7) 1_555 . 1_565 N
Fe1 O2 La1 99.14(22) 1_555 . 101_444 N
Fe1 O2 La1 99.14(22) 1_555 . 101_454 N
Fe1 O2 La1 99.14(22) 1_555 . 101_544 N
Fe1 O2 La1 99.14(22) 1_555 . 101_554 N
Fe1 O2 Sr1 99.14(22) 1_555 . 101_444 N
Fe1 O2 Sr1 99.14(22) 1_555 . 101_454 N
Fe1 O2 Sr1 99.14(22) 1_555 . 101_544 N
Fe1 O2 Sr1 99.14(22) 1_555 . 101_554 N
Fe1 O2 Co1 0.0 1_555 . 1_555 N
La1 O2 La1 88.55(7) 101_444 . 101_454 N
La1 O2 La1 88.55(7) 101_444 . 101_544 N
La1 O2 La1 161.7(4) 101_444 . 101_554 N
La1 O2 Sr1 0.0 101_444 . 101_444 N
La1 O2 Sr1 88.55(7) 101_444 . 101_454 N
La1 O2 Sr1 88.55(7) 101_444 . 101_544 N
La1 O2 Sr1 161.7(4) 101_444 . 101_554 N
La1 O2 Co1 99.14(22) 101_444 . 1_555 N
La1 O2 La1 161.7(4) 101_454 . 101_544 N
La1 O2 La1 88.55(7) 101_454 . 101_554 N
La1 O2 Sr1 88.55(7) 101_454 . 101_444 N
La1 O2 Sr1 0.0 101_454 . 101_454 N
La1 O2 Sr1 161.7(4) 101_454 . 101_544 N
La1 O2 Sr1 88.55(7) 101_454 . 101_554 N
La1 O2 Co1 99.14(22) 101_454 . 1_555 N
La1 O2 La1 88.55(7) 101_544 . 101_554 N
La1 O2 Sr1 88.55(7) 101_544 . 101_444 N
La1 O2 Sr1 161.7(4) 101_544 . 101_454 N
La1 O2 Sr1 0.0 101_544 . 101_544 N
La1 O2 Sr1 88.55(7) 101_544 . 101_554 N
La1 O2 Co1 99.14(22) 101_544 . 1_555 N
La1 O2 Sr1 161.7(4) 101_554 . 101_444 N
La1 O2 Sr1 88.55(7) 101_554 . 101_454 N
La1 O2 Sr1 88.55(7) 101_554 . 101_544 N
La1 O2 Sr1 0.0 101_554 . 101_554 N
La1 O2 Co1 99.14(22) 101_554 . 1_555 N
Sr1 O2 Sr1 88.55(7) 101_444 . 101_454 N
Sr1 O2 Sr1 88.55(7) 101_444 . 101_544 N
Sr1 O2 Sr1 161.7(4) 101_444 . 101_554 N
Sr1 O2 Co1 99.14(22) 101_444 . 1_555 N
Sr1 O2 Sr1 161.7(4) 101_454 . 101_544 N
Sr1 O2 Sr1 88.55(7) 101_454 . 101_554 N
Sr1 O2 Co1 99.14(22) 101_454 . 1_555 N
Sr1 O2 Sr1 88.55(7) 101_544 . 101_554 N
Sr1 O2 Co1 99.14(22) 101_544 . 1_555 N
Sr1 O2 Co1 99.14(22) 101_554 . 1_555 N
Fe2 O3 La2 180.0 1_555 . -1_556 N
Fe2 O3 La2 83.32(20) 1_555 . 101_444 N
Fe2 O3 La2 83.32(20) 1_555 . 101_454 N
Fe2 O3 La2 83.32(20) 1_555 . 101_544 N
Fe2 O3 La2 83.32(20) 1_555 . 101_554 N
Fe2 O3 Sr2 180.0 1_555 . -1_556 N
Fe2 O3 Sr2 83.32(20) 1_555 . 101_444 N
Fe2 O3 Sr2 83.32(20) 1_555 . 101_454 N
Fe2 O3 Sr2 83.32(20) 1_555 . 101_544 N
Fe2 O3 Sr2 83.32(20) 1_555 . 101_554 N
Fe2 O3 Co2 0.0 1_555 . 1_555 N
La2 O3 La2 96.68(20) -1_556 . 101_444 N
La2 O3 La2 96.68(20) -1_556 . 101_454 N
La2 O3 La2 96.68(20) -1_556 . 101_544 N
La2 O3 La2 96.68(20) -1_556 . 101_554 N
La2 O3 Sr2 0.0 -1_556 . -1_556 N
La2 O3 Sr2 96.68(20) -1_556 . 101_444 N
La2 O3 Sr2 96.68(20) -1_556 . 101_454 N
La2 O3 Sr2 96.68(20) -1_556 . 101_544 N
La2 O3 Sr2 96.68(20) -1_556 . 101_554 N
La2 O3 Co2 180.0 -1_556 . 1_555 N
La2 O3 La2 89.22(5) 101_444 . 101_454 N
La2 O3 La2 89.22(5) 101_444 . 101_544 N
La2 O3 La2 166.6(4) 101_444 . 101_554 N
La2 O3 Sr2 96.68(20) 101_444 . -1_556 N
La2 O3 Sr2 0.0 101_444 . 101_444 N
La2 O3 Sr2 89.22(5) 101_444 . 101_454 N
La2 O3 Sr2 89.22(5) 101_444 . 101_544 N
La2 O3 Sr2 166.6(4) 101_444 . 101_554 N
La2 O3 Co2 83.32(20) 101_444 . 1_555 N
La2 O3 La2 166.6(4) 101_454 . 101_544 N
La2 O3 La2 89.22(5) 101_454 . 101_554 N
La2 O3 Sr2 96.68(20) 101_454 . -1_556 N
La2 O3 Sr2 89.22(5) 101_454 . 101_444 N
La2 O3 Sr2 0.0 101_454 . 101_454 N
La2 O3 Sr2 166.6(4) 101_454 . 101_544 N
La2 O3 Sr2 89.22(5) 101_454 . 101_554 N
La2 O3 Co2 83.32(20) 101_454 . 1_555 N
La2 O3 La2 89.22(5) 101_544 . 101_554 N
La2 O3 Sr2 96.68(20) 101_544 . -1_556 N
La2 O3 Sr2 89.22(5) 101_544 . 101_444 N
La2 O3 Sr2 166.6(4) 101_544 . 101_454 N
La2 O3 Sr2 0.0 101_544 . 101_544 N
La2 O3 Sr2 89.22(5) 101_544 . 101_554 N
La2 O3 Co2 83.32(20) 101_544 . 1_555 N
La2 O3 Sr2 96.68(20) 101_554 . -1_556 N
La2 O3 Sr2 166.6(4) 101_554 . 101_444 N
La2 O3 Sr2 89.22(5) 101_554 . 101_454 N
La2 O3 Sr2 89.22(5) 101_554 . 101_544 N
La2 O3 Sr2 0.0 101_554 . 101_554 N
La2 O3 Co2 83.32(20) 101_554 . 1_555 N
Sr2 O3 Sr2 96.68(20) -1_556 . 101_444 N
Sr2 O3 Sr2 96.68(20) -1_556 . 101_454 N
Sr2 O3 Sr2 96.68(20) -1_556 . 101_544 N
Sr2 O3 Sr2 96.68(20) -1_556 . 101_554 N
Sr2 O3 Co2 180.0 -1_556 . 1_555 N
Sr2 O3 Sr2 89.22(5) 101_444 . 101_454 N
Sr2 O3 Sr2 89.22(5) 101_444 . 101_544 N
Sr2 O3 Sr2 166.6(4) 101_444 . 101_554 N
Sr2 O3 Co2 83.32(20) 101_444 . 1_555 N
Sr2 O3 Sr2 166.6(4) 101_454 . 101_544 N
Sr2 O3 Sr2 89.22(5) 101_454 . 101_554 N
Sr2 O3 Co2 83.32(20) 101_454 . 1_555 N
Sr2 O3 Sr2 89.22(5) 101_544 . 101_554 N
Sr2 O3 Co2 83.32(20) 101_544 . 1_555 N
Sr2 O3 Co2 83.32(20) 101_554 . 1_555 N
Fe1 O4 La1 106.3(11) 1_555 . 101_554 N
Fe1 O4 La1 106.3(11) 1_555 . -101_444 N
Fe1 O4 Sr1 106.3(11) 1_555 . 101_554 N
Fe1 O4 Sr1 106.3(11) 1_555 . -101_444 N
Fe1 O4 O4 91(4) 1_555 . 2_655 N
Fe1 O4 O4 179(4) 1_555 . 4_565 N
Fe1 O4 O4 166.2(12) 1_555 . 6_665 N
Fe1 O4 O4 148.8(12) 1_555 . 7_565 N
Fe1 O4 O4 76.2(12) 1_555 . 8_555 N
Fe1 O4 Co1 0.0 1_555 . 1_555 N
Fe1 O4 O5 72.4(22) 1_555 . 2_555 N
La1 O4 La1 134.4(16) 101_554 . -101_444 N
La1 O4 Sr1 0.0 101_554 . 101_554 N
La1 O4 Sr1 134.4(16) 101_554 . -101_444 N
La1 O4 O4 74.1(6) 101_554 . 2_655 N
La1 O4 O4 74.1(6) 101_554 . 4_565 N
La1 O4 O4 70.3(9) 101_554 . 6_665 N
La1 O4 O4 84.2(11) 101_554 . 7_565 N
La1 O4 O4 78.9(10) 101_554 . 8_555 N
La1 O4 Co1 106.3(11) 101_554 . 1_555 N
La1 O4 O5 109.9(11) 101_554 . 2_555 N
La1 O4 Sr1 134.4(16) -101_444 . 101_554 N
La1 O4 Sr1 0.0 -101_444 . -101_444 N
La1 O4 O4 74.1(6) -101_555 . 2_655 N
La1 O4 O4 74.1(6) -101_555 . 4_565 N
La1 O4 O4 70.3(9) -101_555 . 6_665 N
La1 O4 O4 84.2(11) -101_555 . 7_565 N
La1 O4 O4 78.9(10) -101_555 . 8_555 N
La1 O4 Co1 106.3(11) -101_555 . 1_555 N
La1 O4 O5 109.9(11) -101_555 . 2_555 N
Sr1 O4 Sr1 134.4(16) 101_554 . -101_444 N
Sr1 O4 O4 74.1(6) 101_554 . 2_655 N
Sr1 O4 O4 74.1(6) 101_554 . 4_565 N
Sr1 O4 O4 70.3(9) 101_554 . 6_665 N
Sr1 O4 O4 84.2(11) 101_554 . 7_565 N
Sr1 O4 O4 78.9(10) 101_554 . 8_555 N
Sr1 O4 Co1 106.3(11) 101_554 . 1_555 N
Sr1 O4 O5 109.9(11) 101_554 . 2_555 N
Sr1 O4 O4 74.1(6) -101_555 . 2_655 N
Sr1 O4 O4 74.1(6) -101_555 . 4_565 N
Sr1 O4 O4 70.3(9) -101_555 . 6_665 N
Sr1 O4 O4 84.2(11) -101_555 . 7_565 N
Sr1 O4 O4 78.9(10) -101_555 . 8_555 N
Sr1 O4 Co1 106.3(11) -101_555 . 1_555 N
Sr1 O4 O5 109.9(11) -101_555 . 2_555 N
O4 O4 O4 90.0000(4) 2_655 . 4_565 N
O4 O4 O4 74.8(27) 2_655 . 6_665 N
O4 O4 O4 119.8(27) 2_655 . 7_565 N
O4 O4 O4 15.2(27) 2_655 . 8_555 N
O4 O4 Co1 91(4) 2_655 . 1_555 N
O4 O4 O5 164(5) 2_655 . 2_555 N
O4 O4 O4 15.2(27) 4_565 . 6_665 N
O4 O4 O4 29.8(27) 4_565 . 7_565 N
O4 O4 O4 105.2(27) 4_565 . 8_555 N
O4 O4 Co1 179(4) 4_565 . 1_555 N
O4 O4 O5 106(5) 4_565 . 2_555 N
O4 O4 O4 45.0000(8) 6_665 . 7_565 N
O4 O4 O4 90.0 6_665 . 8_555 N
O4 O4 Co1 166.2(12) 6_665 . 1_555 N
O4 O4 O5 121.4(24) 6_665 . 2_555 N
O4 O4 O4 135.0000(13) 7_565 . 8_555 N
O4 O4 Co1 148.8(12) 7_565 . 1_555 N
O4 O4 O5 76.4(24) 7_565 . 2_555 N
O4 O4 Co1 76.2(12) 8_555 . 1_555 N
O4 O4 O5 148.6(24) 8_555 . 2_555 N
Co1 O4 O5 72.4(22) 1_555 . 2_555 N
O2 Co1 O2 180.0 1_555 . -1_555 N
O2 Co1 O4 90.0 1_555 . 1_555 N
O2 Co1 O4 90.0 1_555 . 2_555 N
O2 Co1 O4 90.0 1_555 . 3_555 N
O2 Co1 O4 90.0 1_555 . 4_555 N
O2 Co1 O4 90.0 1_555 . 5_555 N
O2 Co1 O4 90.0 1_555 . 6_555 N
O2 Co1 O4 90.0 1_555 . 7_555 N
O2 Co1 O4 90.0 1_555 . 8_555 N
O2 Co1 O5 90.0 1_555 . 1_455 N
O2 Co1 O5 90.0 1_555 . 1_555 N
O2 Co1 O5 90.0 1_555 . 2_545 N
O2 Co1 O5 90.0 1_555 . 2_555 N
O2 Co1 O4 90.0 -1_555 . 1_555 N
O2 Co1 O4 90.0 -1_555 . 2_555 N
O2 Co1 O4 90.0 -1_555 . 3_555 N
O2 Co1 O4 90.0 -1_555 . 4_555 N
O2 Co1 O4 90.0 -1_555 . 5_555 N
O2 Co1 O4 90.0 -1_555 . 6_555 N
O2 Co1 O4 90.0 -1_555 . 7_555 N
O2 Co1 O4 90.0 -1_555 . 8_555 N
O2 Co1 O5 90.0 -1_555 . 1_455 N
O2 Co1 O5 90.0 -1_555 . 1_555 N
O2 Co1 O5 90.0 -1_555 . 2_545 N
O2 Co1 O5 90.0 -1_555 . 2_555 N
O4 Co1 O4 90.0 1_555 . 2_555 N
O4 Co1 O4 180.0 1_555 . 3_555 N
O4 Co1 O4 90.0 1_555 . 4_555 N
O4 Co1 O4 62.4(23) 1_555 . 5_555 N
O4 Co1 O4 152.4(23) 1_555 . 6_555 N
O4 Co1 O4 117.6(23) 1_555 . 7_555 N
O4 Co1 O4 27.6(23) 1_555 . 8_555 N
O4 Co1 O5 121.2(12) 1_555 . 1_455 N
O4 Co1 O5 58.8(12) 1_555 . 1_555 N
O4 Co1 O5 148.8(12) 1_555 . 2_545 N
O4 Co1 O5 31.2(12) 1_555 . 2_555 N
O4 Co1 O4 90.0 2_555 . 3_555 N
O4 Co1 O4 180.0 2_555 . 4_555 N
O4 Co1 O4 27.6(23) 2_555 . 5_555 N
O4 Co1 O4 62.4(23) 2_555 . 6_555 N
O4 Co1 O4 152.4(23) 2_555 . 7_555 N
O4 Co1 O4 117.6(23) 2_555 . 8_555 N
O4 Co1 O5 31.2(12) 2_555 . 1_455 N
O4 Co1 O5 148.8(12) 2_555 . 1_555 N
O4 Co1 O5 121.2(12) 2_555 . 2_545 N
O4 Co1 O5 58.8(12) 2_555 . 2_555 N
O4 Co1 O4 90.0 3_555 . 4_555 N
O4 Co1 O4 117.6(23) 3_555 . 5_555 N
O4 Co1 O4 27.6(23) 3_555 . 6_555 N
O4 Co1 O4 62.4(23) 3_555 . 7_555 N
O4 Co1 O4 152.4(23) 3_555 . 8_555 N
O4 Co1 O5 58.8(12) 3_555 . 1_455 N
O4 Co1 O5 121.2(12) 3_555 . 1_555 N
O4 Co1 O5 31.2(12) 3_555 . 2_545 N
O4 Co1 O5 148.8(12) 3_555 . 2_555 N
O4 Co1 O4 152.4(23) 4_555 . 5_555 N
O4 Co1 O4 117.6(23) 4_555 . 6_555 N
O4 Co1 O4 27.6(23) 4_555 . 7_555 N
O4 Co1 O4 62.4(23) 4_555 . 8_555 N
O4 Co1 O5 148.8(12) 4_555 . 1_455 N
O4 Co1 O5 31.2(12) 4_555 . 1_555 N
O4 Co1 O5 58.8(12) 4_555 . 2_545 N
O4 Co1 O5 121.2(12) 4_555 . 2_555 N
O4 Co1 O4 90.0 5_555 . 6_555 N
O4 Co1 O4 179.9802 5_555 . 7_555 N
O4 Co1 O4 90.0 5_555 . 8_555 N
O4 Co1 O5 58.8(12) 5_555 . 1_455 N
O4 Co1 O5 121.2(12) 5_555 . 1_555 N
O4 Co1 O5 148.8(12) 5_555 . 2_545 N
O4 Co1 O5 31.2(12) 5_555 . 2_555 N
O4 Co1 O4 90.0 6_555 . 7_555 N
O4 Co1 O4 180.0 6_555 . 8_555 N
O4 Co1 O5 31.2(12) 6_555 . 1_455 N
O4 Co1 O5 148.8(12) 6_555 . 1_555 N
O4 Co1 O5 58.8(12) 6_555 . 2_545 N
O4 Co1 O5 121.2(12) 6_555 . 2_555 N
O4 Co1 O4 90.0 7_555 . 8_555 N
O4 Co1 O5 121.2(12) 7_555 . 1_455 N
O4 Co1 O5 58.8(12) 7_555 . 1_555 N
O4 Co1 O5 31.2(12) 7_555 . 2_545 N
O4 Co1 O5 148.8(12) 7_555 . 2_555 N
O4 Co1 O5 148.8(12) 8_555 . 1_455 N
O4 Co1 O5 31.2(12) 8_555 . 1_555 N
O4 Co1 O5 121.2(12) 8_555 . 2_545 N
O4 Co1 O5 58.8(12) 8_555 . 2_555 N
O5 Co1 O5 180.0 1_455 . 1_555 N
O5 Co1 O5 90.0 1_455 . 2_545 N
O5 Co1 O5 90.0 1_455 . 2_555 N
O5 Co1 O5 90.0 1_555 . 2_545 N
O5 Co1 O5 90.0 1_555 . 2_555 N
O5 Co1 O5 180.0 2_545 . 2_555 N
Sr1 Co2 Sr1 69.66(14) 101_444 . 101_454 N
Sr1 Co2 Sr1 69.66(14) 101_444 . 101_544 N
Sr1 Co2 Sr1 107.75(27) 101_444 . 101_554 N
Sr1 Co2 Sr2 69.10(9) 101_444 . 101_444 N
Sr1 Co2 Sr2 108.71(4) 101_444 . 101_454 N
Sr1 Co2 Sr2 108.71(4) 101_444 . 101_544 N
Sr1 Co2 Sr2 176.84(24) 101_444 . 101_554 N
Sr1 Co2 O1 51.60(24) 101_444 . 1_545 N
Sr1 Co2 O1 121.11(28) 101_444 . 1_555 N
Sr1 Co2 O1 51.60(24) 101_444 . 2_555 N
Sr1 Co2 O1 121.11(28) 101_444 . 2_655 N
Sr1 Co2 O3 126.13(13) 101_444 . 1_555 N
Sr1 Co2 Sr1 107.75(27) 101_454 . 101_544 N
Sr1 Co2 Sr1 69.66(14) 101_454 . 101_554 N
Sr1 Co2 Sr2 108.71(4) 101_454 . 101_444 N
Sr1 Co2 Sr2 69.10(9) 101_454 . 101_454 N
Sr1 Co2 Sr2 176.84(24) 101_454 . 101_544 N
Sr1 Co2 Sr2 108.71(4) 101_454 . 101_554 N
Sr1 Co2 O1 121.11(28) 101_454 . 1_545 N
Sr1 Co2 O1 51.60(24) 101_454 . 1_555 N
Sr1 Co2 O1 51.60(24) 101_454 . 2_555 N
Sr1 Co2 O1 121.11(28) 101_454 . 2_655 N
Sr1 Co2 O3 126.13(13) 101_454 . 1_555 N
Sr1 Co2 Sr1 69.66(14) 101_544 . 101_554 N
Sr1 Co2 Sr2 108.71(4) 101_544 . 101_444 N
Sr1 Co2 Sr2 176.84(24) 101_544 . 101_454 N
Sr1 Co2 Sr2 69.10(9) 101_544 . 101_544 N
Sr1 Co2 Sr2 108.71(4) 101_544 . 101_554 N
Sr1 Co2 O1 51.60(24) 101_544 . 1_545 N
Sr1 Co2 O1 121.11(28) 101_544 . 1_555 N
Sr1 Co2 O1 121.11(28) 101_544 . 2_555 N
Sr1 Co2 O1 51.60(24) 101_544 . 2_655 N
Sr1 Co2 O3 126.13(13) 101_544 . 1_555 N
Sr1 Co2 Sr2 176.84(24) 101_554 . 101_444 N
Sr1 Co2 Sr2 108.71(4) 101_554 . 101_454 N
Sr1 Co2 Sr2 108.71(4) 101_554 . 101_544 N
Sr1 Co2 Sr2 69.10(9) 101_554 . 101_554 N
Sr1 Co2 O1 121.11(28) 101_554 . 1_545 N
Sr1 Co2 O1 51.60(24) 101_554 . 1_555 N
Sr1 Co2 O1 121.11(28) 101_554 . 2_555 N
Sr1 Co2 O1 51.60(24) 101_554 . 2_655 N
Sr1 Co2 O3 126.13(13) 101_554 . 1_555 N
Sr2 Co2 Sr2 72.77(11) 101_444 . 101_454 N
Sr2 Co2 Sr2 72.77(11) 101_444 . 101_544 N
Sr2 Co2 Sr2 114.06(24) 101_444 . 101_554 N
Sr2 Co2 O1 57.13(24) 101_444 . 1_545 N
Sr2 Co2 O1 129.72(24) 101_444 . 1_555 N
Sr2 Co2 O1 57.13(24) 101_444 . 2_555 N
Sr2 Co2 O1 129.72(24) 101_444 . 2_655 N
Sr2 Co2 O3 57.03(12) 101_444 . 1_555 N
Sr2 Co2 Sr2 114.06(24) 101_454 . 101_544 N
Sr2 Co2 Sr2 72.77(11) 101_454 . 101_554 N
Sr2 Co2 O1 129.72(24) 101_454 . 1_545 N
Sr2 Co2 O1 57.13(24) 101_454 . 1_555 N
Sr2 Co2 O1 57.13(24) 101_454 . 2_555 N
Sr2 Co2 O1 129.72(24) 101_454 . 2_655 N
Sr2 Co2 O3 57.03(12) 101_454 . 1_555 N
Sr2 Co2 Sr2 72.77(11) 101_544 . 101_554 N
Sr2 Co2 O1 57.13(24) 101_544 . 1_545 N
Sr2 Co2 O1 129.72(24) 101_544 . 1_555 N
Sr2 Co2 O1 129.72(24) 101_544 . 2_555 N
Sr2 Co2 O1 57.13(24) 101_544 . 2_655 N
Sr2 Co2 O3 57.03(12) 101_544 . 1_555 N
Sr2 Co2 O1 129.72(24) 101_554 . 1_545 N
Sr2 Co2 O1 57.13(24) 101_554 . 1_555 N
Sr2 Co2 O1 129.72(24) 101_554 . 2_555 N
Sr2 Co2 O1 57.13(24) 101_554 . 2_655 N
Sr2 Co2 O3 57.03(12) 101_554 . 1_555 N
O1 Co2 O1 169.8(7) 1_545 . 1_555 N
O1 Co2 O1 89.55(6) 1_545 . 2_555 N
O1 Co2 O1 89.55(6) 1_545 . 2_655 N
O1 Co2 O3 95.1(4) 1_545 . 1_555 N
O1 Co2 O1 89.55(6) 1_555 . 2_555 N
O1 Co2 O1 89.55(6) 1_555 . 2_655 N
O1 Co2 O3 95.1(4) 1_555 . 1_555 N
O1 Co2 O1 169.8(7) 2_555 . 2_655 N
O1 Co2 O3 95.1(4) 2_555 . 1_555 N
O1 Co2 O3 95.1(4) 2_655 . 1_555 N
Fe1 O5 Fe1 180.0 1_555 . 1_655 N
Fe1 O5 Sr1 90.0 1_555 . 101_544 N
Fe1 O5 Sr1 90.0 1_555 . 101_554 N
Fe1 O5 Sr1 90.0 1_555 . -101_434 N
Fe1 O5 Sr1 90.0 1_555 . -101_444 N
Fe1 O5 O4 103.6(24) 1_555 . 2_655 N
Fe1 O5 O4 76.4(24) 1_555 . 4_555 N
Fe1 O5 O4 103.6(24) 1_555 . 6_655 N
Fe1 O5 O4 76.4(24) 1_555 . 8_555 N
Fe1 O5 Co1 0.0 1_555 . 1_555 N
Fe1 O5 Co1 180.0 1_555 . 1_655 N
Fe1 O5 Sr1 90.0 1_655 . 101_544 N
Fe1 O5 Sr1 90.0 1_655 . 101_554 N
Fe1 O5 Sr1 90.0 1_655 . -101_434 N
Fe1 O5 Sr1 90.0 1_655 . -101_444 N
Fe1 O5 O4 76.4(24) 1_655 . 2_655 N
Fe1 O5 O4 103.6(24) 1_655 . 4_555 N
Fe1 O5 O4 76.4(24) 1_655 . 6_655 N
Fe1 O5 O4 103.6(24) 1_655 . 8_555 N
Fe1 O5 Co1 180.0 1_655 . 1_555 N
Fe1 O5 Co1 0.0 1_655 . 1_655 N
Sr1 O5 Sr1 81.43(20) 101_544 . 101_554 N
Sr1 O5 Sr1 98.57(20) 101_544 . -101_434 N
Sr1 O5 Sr1 179.972 101_544 . -101_444 N
Sr1 O5 O4 129.3(5) 101_544 . 2_655 N
Sr1 O5 O4 50.7(5) 101_544 . 4_555 N
Sr1 O5 O4 50.7(5) 101_544 . 6_655 N
Sr1 O5 O4 129.3(5) 101_544 . 8_555 N
Sr1 O5 Co1 90.0 101_544 . 1_555 N
Sr1 O5 Co1 90.0 101_544 . 1_655 N
Sr1 O5 Sr1 179.9802 101_554 . -101_434 N
Sr1 O5 Sr1 98.57(20) 101_554 . -101_444 N
Sr1 O5 O4 50.7(5) 101_554 . 2_655 N
Sr1 O5 O4 129.3(5) 101_554 . 4_555 N
Sr1 O5 O4 129.3(5) 101_554 . 6_655 N
Sr1 O5 O4 50.7(5) 101_554 . 8_555 N
Sr1 O5 Co1 90.0 101_554 . 1_555 N
Sr1 O5 Co1 90.0 101_554 . 1_655 N
Sr1 O5 Sr1 81.43(20) -101_434 . -101_444 N
Sr1 O5 O4 129.3(5) -101_545 . 2_655 N
Sr1 O5 O4 50.7(5) -101_545 . 4_555 N
Sr1 O5 O4 50.7(5) -101_545 . 6_655 N
Sr1 O5 O4 129.3(5) -101_545 . 8_555 N
Sr1 O5 Co1 90.0 -101_545 . 1_555 N
Sr1 O5 Co1 90.0 -101_545 . 1_655 N
Sr1 O5 O4 50.7(5) -101_555 . 2_655 N
Sr1 O5 O4 129.3(5) -101_555 . 4_555 N
Sr1 O5 O4 129.3(5) -101_555 . 6_655 N
Sr1 O5 O4 50.7(5) -101_555 . 8_555 N
Sr1 O5 Co1 90.0 -101_555 . 1_555 N
Sr1 O5 Co1 90.0 -101_555 . 1_655 N
O4 O5 O4 180.0 2_655 . 4_555 N
O4 O5 O4 153(5) 2_655 . 6_655 N
O4 O5 O4 27(5) 2_655 . 8_555 N
O4 O5 Co1 103.6(24) 2_655 . 1_555 N
O4 O5 Co1 76.4(24) 2_655 . 1_655 N
O4 O5 O4 27(5) 4_555 . 6_655 N
O4 O5 O4 153(5) 4_555 . 8_555 N
O4 O5 Co1 76.4(24) 4_555 . 1_555 N
O4 O5 Co1 103.6(24) 4_555 . 1_655 N
O4 O5 O4 180.0 6_655 . 8_555 N
O4 O5 Co1 103.6(24) 6_655 . 1_555 N
O4 O5 Co1 76.4(24) 6_655 . 1_655 N
O4 O5 Co1 76.4(24) 8_555 . 1_555 N
O4 O5 Co1 103.6(24) 8_555 . 1_655 N
Co1 O5 Co1 180.0 1_555 . 1_655 N
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_1
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Fe1 La1 3.500(5) . 101_444 N
Fe1 La1 3.500(5) . 101_454 N
Fe1 La1 3.500(5) . 101_544 N
Fe1 La1 3.500(5) . 101_554 N
Fe1 La1 3.500(5) . -101_334 N
Fe1 La1 3.500(5) . -101_344 N
Fe1 La1 3.500(5) . -101_434 N
Fe1 La1 3.500(5) . -101_444 N
Fe1 Sr1 3.500(5) . 101_444 N
Fe1 Sr1 3.500(5) . 101_454 N
Fe1 Sr1 3.500(5) . 101_544 N
Fe1 Sr1 3.500(5) . 101_554 N
Fe1 Sr1 3.500(5) . -101_334 N
Fe1 Sr1 3.500(5) . -101_344 N
Fe1 Sr1 3.500(5) . -101_434 N
Fe1 Sr1 3.500(5) . -101_444 N
Fe1 O2 1.787(7) . 1_555 N
Fe1 O2 1.787(7) . -1_555 N
Fe1 O4 2.38(4) . 1_545 N
Fe1 O4 1.95(4) . 1_555 N
Fe1 O4 1.95(4) . 2_555 N
Fe1 O4 2.38(4) . 2_655 N
Fe1 O4 1.95(4) . 3_555 N
Fe1 O4 2.38(4) . 3_565 N
Fe1 O4 2.38(4) . 4_455 N
Fe1 O4 1.95(4) . 4_555 N
Fe1 O4 2.38(4) . 5_545 N
Fe1 O4 1.95(4) . 5_555 N
Fe1 O4 1.95(4) . 6_555 N
Fe1 O4 2.38(4) . 6_655 N
Fe1 O4 1.95(4) . 7_555 N
Fe1 O4 2.38(4) . 7_565 N
Fe1 O4 2.38(4) . 8_455 N
Fe1 O4 1.95(4) . 8_555 N
Fe1 O5 1.91208(6) . 1_455 N
Fe1 O5 1.91208(6) . 1_555 N
Fe1 O5 1.91208(6) . 2_545 N
Fe1 O5 1.91208(6) . 2_555 N
Fe2 La1 3.348(6) . 101_444 N
Fe2 La1 3.348(6) . 101_454 N
Fe2 La1 3.348(6) . 101_544 N
Fe2 La1 3.348(6) . 101_554 N
Fe2 Sr1 3.348(6) . 101_444 N
Fe2 Sr1 3.348(6) . 101_454 N
Fe2 Sr1 3.348(6) . 101_544 N
Fe2 Sr1 3.348(6) . 101_554 N
Fe2 La2 3.223(4) . 101_444 N
Fe2 La2 3.223(4) . 101_454 N
Fe2 La2 3.223(4) . 101_544 N
Fe2 La2 3.223(4) . 101_554 N
Fe2 Sr2 3.223(4) . 101_444 N
Fe2 Sr2 3.223(4) . 101_454 N
Fe2 Sr2 3.223(4) . 101_544 N
Fe2 Sr2 3.223(4) . 101_554 N
Fe2 O1 1.9196(10) . 1_545 N
Fe2 O1 1.9196(10) . 1_555 N
Fe2 O1 1.9196(10) . 2_555 N
Fe2 O1 1.9196(10) . 2_655 N
Fe2 O2 2.409(11) . 1_555 N
Fe2 O3 2.071(9) . 1_555 N
La1 Fe1 3.500(5) . 101_445 N
La1 Fe1 3.500(5) . 101_455 N
La1 Fe1 3.500(5) . 101_545 N
La1 Fe1 3.500(5) . 101_555 N
La1 Fe2 3.348(6) . 101_445 N
La1 Fe2 3.348(6) . 101_455 N
La1 Fe2 3.348(6) . 101_545 N
La1 Fe2 3.348(6) . 101_555 N
La1 La1 3.82416(12) . 1_455 N
La1 La1 3.82416(12) . 1_545 N
La1 La1 3.82416(12) . 1_565 N
La1 La1 3.82416(12) . 1_655 N
La1 Sr1 3.82416(12) . 1_455 N
La1 Sr1 3.82416(12) . 1_545 N
La1 Sr1 3.82416(12) . 1_565 N
La1 Sr1 3.82416(12) . 1_655 N
La1 La2 3.728(6) . 1_555 N
La1 Sr2 3.728(6) . 1_555 N
La1 O1 2.629(10) . 101_445 N
La1 O1 2.629(10) . 101_545 N
La1 O1 2.629(10) . 102_545 N
La1 O1 2.629(10) . 102_555 N
La1 O2 2.7389(17) . 101_445 N
La1 O2 2.7389(17) . 101_455 N
La1 O2 2.7389(17) . 101_545 N
La1 O2 2.7389(17) . 101_555 N
La1 O4 2.411(16) . 101_445 N
La1 O4 2.411(16) . 102_545 N
La1 O4 2.411(16) . 103_555 N
La1 O4 2.411(16) . 104_455 N
La1 O4 2.411(16) . 105_545 N
La1 O4 2.411(16) . 106_555 N
La1 O4 2.411(16) . 107_455 N
La1 O4 2.411(16) . 108_445 N
La1 Co1 3.500(5) . 101_445 N
La1 Co1 3.500(5) . 101_455 N
La1 Co1 3.500(5) . 101_545 N
La1 Co1 3.500(5) . 101_555 N
La1 Co2 3.348(6) . 101_445 N
La1 Co2 3.348(6) . 101_455 N
La1 Co2 3.348(6) . 101_545 N
La1 Co2 3.348(6) . 101_555 N
La1 O5 2.931(6) . 101_445 N
La1 O5 2.931(6) . 101_455 N
La1 O5 2.931(6) . 102_445 N
La1 O5 2.931(6) . 102_545 N
Sr1 Fe1 3.500(5) . 101_445 N
Sr1 Fe1 3.500(5) . 101_455 N
Sr1 Fe1 3.500(5) . 101_545 N
Sr1 Fe1 3.500(5) . 101_555 N
Sr1 Fe2 3.348(6) . 101_445 N
Sr1 Fe2 3.348(6) . 101_455 N
Sr1 Fe2 3.348(6) . 101_545 N
Sr1 Fe2 3.348(6) . 101_555 N
Sr1 La1 3.82416(12) . 1_455 N
Sr1 La1 3.82416(12) . 1_545 N
Sr1 La1 3.82416(12) . 1_565 N
Sr1 La1 3.82416(12) . 1_655 N
Sr1 Sr1 3.82416(12) . 1_455 N
Sr1 Sr1 3.82416(12) . 1_545 N
Sr1 Sr1 3.82416(12) . 1_565 N
Sr1 Sr1 3.82416(12) . 1_655 N
Sr1 Sr1 4.444(15) . -1_556 N
Sr1 La2 3.728(6) . 1_555 N
Sr1 Sr2 3.728(6) . 1_555 N
Sr1 O1 2.629(10) . 101_445 N
Sr1 O1 2.629(10) . 101_545 N
Sr1 O1 2.629(10) . 102_545 N
Sr1 O1 2.629(10) . 102_555 N
Sr1 O2 2.7389(17) . 101_445 N
Sr1 O2 2.7389(17) . 101_455 N
Sr1 O2 2.7389(17) . 101_545 N
Sr1 O2 2.7389(17) . 101_555 N
Sr1 O4 2.411(16) . 101_445 N
Sr1 O4 2.411(16) . 102_545 N
Sr1 O4 2.411(16) . 103_555 N
Sr1 O4 2.411(16) . 104_455 N
Sr1 O4 2.411(16) . 105_545 N
Sr1 O4 2.411(16) . 106_555 N
Sr1 O4 2.411(16) . 107_455 N
Sr1 O4 2.411(16) . 108_445 N
Sr1 Co1 3.500(5) . 101_445 N
Sr1 Co1 3.500(5) . 101_455 N
Sr1 Co1 3.500(5) . 101_545 N
Sr1 Co1 3.500(5) . 101_555 N
Sr1 Co2 3.348(6) . 101_445 N
Sr1 Co2 3.348(6) . 101_455 N
Sr1 Co2 3.348(6) . 101_545 N
Sr1 Co2 3.348(6) . 101_555 N
Sr1 O5 2.931(6) . 101_445 N
Sr1 O5 2.931(6) . 101_455 N
Sr1 O5 2.931(6) . 102_445 N
Sr1 O5 2.931(6) . 102_545 N
La2 Fe2 3.223(4) . 101_445 N
La2 Fe2 3.223(4) . 101_455 N
La2 Fe2 3.223(4) . 101_545 N
La2 Fe2 3.223(4) . 101_555 N
La2 La1 3.728(6) . 1_555 N
La2 Sr1 3.728(6) . 1_555 N
La2 La2 3.82416(12) . 1_455 N
La2 La2 3.82416(12) . 1_545 N
La2 La2 3.82416(12) . 1_565 N
La2 La2 3.82416(12) . 1_655 N
La2 La2 3.866(9) . -101_335 N
La2 La2 3.866(9) . -101_345 N
La2 La2 3.866(9) . -101_435 N
La2 La2 3.866(9) . -101_445 N
La2 Sr2 3.82416(12) . 1_455 N
La2 Sr2 3.82416(12) . 1_545 N
La2 Sr2 3.82416(12) . 1_565 N
La2 Sr2 3.82416(12) . 1_655 N
La2 Sr2 3.866(9) . -101_335 N
La2 Sr2 3.866(9) . -101_345 N
La2 Sr2 3.866(9) . -101_435 N
La2 Sr2 3.866(9) . -101_445 N
La2 O1 2.713(9) . 101_445 N
La2 O1 2.713(9) . 101_545 N
La2 O1 2.713(9) . 102_545 N
La2 O1 2.713(9) . 102_555 N
La2 O3 2.447(11) . -1_556 N
La2 O3 2.7226(11) . 101_445 N
La2 O3 2.7226(11) . 101_455 N
La2 O3 2.7226(11) . 101_545 N
La2 O3 2.7226(11) . 101_555 N
La2 Co2 3.223(4) . 101_445 N
La2 Co2 3.223(4) . 101_455 N
La2 Co2 3.223(4) . 101_545 N
La2 Co2 3.223(4) . 101_555 N
Sr2 Fe2 3.223(4) . 101_445 N
Sr2 Fe2 3.223(4) . 101_455 N
Sr2 Fe2 3.223(4) . 101_545 N
Sr2 Fe2 3.223(4) . 101_555 N
Sr2 La1 3.728(6) . 1_555 N
Sr2 Sr1 3.728(6) . 1_555 N
Sr2 La2 3.82416(12) . 1_455 N
Sr2 La2 3.82416(12) . 1_545 N
Sr2 La2 3.82416(12) . 1_565 N
Sr2 La2 3.82416(12) . 1_655 N
Sr2 La2 3.866(9) . -101_335 N
Sr2 La2 3.866(9) . -101_345 N
Sr2 La2 3.866(9) . -101_435 N
Sr2 La2 3.866(9) . -101_445 N
Sr2 Sr2 3.82416(12) . 1_455 N
Sr2 Sr2 3.82416(12) . 1_545 N
Sr2 Sr2 3.82416(12) . 1_565 N
Sr2 Sr2 3.82416(12) . 1_655 N
Sr2 Sr2 3.866(9) . -101_335 N
Sr2 Sr2 3.866(9) . -101_345 N
Sr2 Sr2 3.866(9) . -101_435 N
Sr2 Sr2 3.866(9) . -101_445 N
Sr2 O1 2.713(9) . 101_445 N
Sr2 O1 2.713(9) . 101_545 N
Sr2 O1 2.713(9) . 102_545 N
Sr2 O1 2.713(9) . 102_555 N
Sr2 O3 2.447(11) . -1_556 N
Sr2 O3 2.7226(11) . 101_445 N
Sr2 O3 2.7226(11) . 101_455 N
Sr2 O3 2.7226(11) . 101_545 N
Sr2 O3 2.7226(11) . 101_555 N
Sr2 Co2 3.223(4) . 101_445 N
Sr2 Co2 3.223(4) . 101_455 N
Sr2 Co2 3.223(4) . 101_545 N
Sr2 Co2 3.223(4) . 101_555 N
O1 Fe2 1.9196(10) . 1_555 N
O1 Fe2 1.9196(10) . 1_565 N
O1 La1 2.629(10) . 101_454 N
O1 La1 2.629(10) . 101_554 N
O1 Sr1 2.629(10) . 101_454 N
O1 Sr1 2.629(10) . 101_554 N
O1 La2 2.713(9) . 101_454 N
O1 La2 2.713(9) . 101_554 N
O1 Sr2 2.713(9) . 101_454 N
O1 Sr2 2.713(9) . 101_554 N
O1 Co2 1.9196(10) . 1_555 N
O1 Co2 1.9196(10) . 1_565 N
O2 Fe1 1.787(7) . 1_555 N
O2 Fe2 2.409(11) . 1_555 N
O2 La1 2.7389(17) . 101_444 N
O2 La1 2.7389(17) . 101_454 N
O2 La1 2.7389(17) . 101_544 N
O2 La1 2.7389(17) . 101_554 N
O2 Sr1 2.7389(17) . 101_444 N
O2 Sr1 2.7389(17) . 101_454 N
O2 Sr1 2.7389(17) . 101_544 N
O2 Sr1 2.7389(17) . 101_554 N
O2 Co1 1.787(7) . 1_555 N
O2 Co2 2.409(11) . 1_555 N
O3 Fe2 2.071(9) . 1_555 N
O3 La2 2.447(11) . -1_556 N
O3 La2 2.7226(11) . 101_444 N
O3 La2 2.7226(11) . 101_454 N
O3 La2 2.7226(11) . 101_544 N
O3 La2 2.7226(11) . 101_554 N
O3 Sr2 2.447(11) . -1_556 N
O3 Sr2 2.7226(11) . 101_444 N
O3 Sr2 2.7226(11) . 101_454 N
O3 Sr2 2.7226(11) . 101_544 N
O3 Sr2 2.7226(11) . 101_554 N
O3 Co2 2.071(9) . 1_555 N
O4 Fe1 1.95(4) . 1_555 N
O4 Fe1 2.38(4) . 1_565 N
O4 La1 2.411(16) . 101_554 N
O4 La1 2.411(16) . -101_444 N
O4 Sr1 2.411(16) . 101_554 N
O4 Sr1 2.411(16) . -101_444 N
O4 O4 1.32(5) . 2_655 N
O4 O4 2.08(8) . 3_565 N
O4 O4 1.87(7) . 3_665 N
O4 O4 1.32(5) . 4_565 N
O4 O4 2.02(7) . 5_555 N
O4 O4 1.80(7) . 5_655 N
O4 O4 1.62(8) . 6_665 N
O4 O4 0.49(9) . 7_565 N
O4 O4 0.93(8) . 8_555 N
O4 Co1 1.95(4) . 1_555 N
O4 Co1 2.38(4) . 1_565 N
O4 O5 1.90(4) . 1_555 N
O4 O5 1.04(4) . 2_555 N
Co1 La1 3.500(5) . 101_444 N
Co1 La1 3.500(5) . 101_454 N
Co1 La1 3.500(5) . 101_544 N
Co1 La1 3.500(5) . 101_554 N
Co1 La1 3.500(5) . -101_334 N
Co1 La1 3.500(5) . -101_344 N
Co1 La1 3.500(5) . -101_434 N
Co1 La1 3.500(5) . -101_444 N
Co1 Sr1 3.500(5) . 101_444 N
Co1 Sr1 3.500(5) . 101_454 N
Co1 Sr1 3.500(5) . 101_544 N
Co1 Sr1 3.500(5) . 101_554 N
Co1 Sr1 3.500(5) . -101_334 N
Co1 Sr1 3.500(5) . -101_344 N
Co1 Sr1 3.500(5) . -101_434 N
Co1 Sr1 3.500(5) . -101_444 N
Co1 O2 1.787(7) . 1_555 N
Co1 O2 1.787(7) . -1_555 N
Co1 O4 2.38(4) . 1_545 N
Co1 O4 1.95(4) . 1_555 N
Co1 O4 1.95(4) . 2_555 N
Co1 O4 2.38(4) . 2_655 N
Co1 O4 1.95(4) . 3_555 N
Co1 O4 2.38(4) . 3_565 N
Co1 O4 2.38(4) . 4_455 N
Co1 O4 1.95(4) . 4_555 N
Co1 O4 2.38(4) . 5_545 N
Co1 O4 1.95(4) . 5_555 N
Co1 O4 1.95(4) . 6_555 N
Co1 O4 2.38(4) . 6_655 N
Co1 O4 1.95(4) . 7_555 N
Co1 O4 2.38(4) . 7_565 N
Co1 O4 2.38(4) . 8_455 N
Co1 O4 1.95(4) . 8_555 N
Co1 O5 1.91208(6) . 1_455 N
Co1 O5 1.91208(6) . 1_555 N
Co1 O5 1.91208(6) . 2_545 N
Co1 O5 1.91208(6) . 2_555 N
Co2 La1 3.348(6) . 101_444 N
Co2 La1 3.348(6) . 101_454 N
Co2 La1 3.348(6) . 101_544 N
Co2 La1 3.348(6) . 101_554 N
Co2 Sr1 3.348(6) . 101_444 N
Co2 Sr1 3.348(6) . 101_454 N
Co2 Sr1 3.348(6) . 101_544 N
Co2 Sr1 3.348(6) . 101_554 N
Co2 La2 3.223(4) . 101_444 N
Co2 La2 3.223(4) . 101_454 N
Co2 La2 3.223(4) . 101_544 N
Co2 La2 3.223(4) . 101_554 N
Co2 Sr2 3.223(4) . 101_444 N
Co2 Sr2 3.223(4) . 101_454 N
Co2 Sr2 3.223(4) . 101_544 N
Co2 Sr2 3.223(4) . 101_554 N
Co2 O1 1.9196(10) . 1_545 N
Co2 O1 1.9196(10) . 1_555 N
Co2 O1 1.9196(10) . 2_555 N
Co2 O1 1.9196(10) . 2_655 N
Co2 O2 2.409(11) . 1_555 N
Co2 O3 2.071(9) . 1_555 N
O5 Fe1 1.91208(6) . 1_555 N
O5 Fe1 1.91208(6) . 1_655 N
O5 La1 2.931(6) . 101_544 N
O5 La1 2.931(6) . 101_554 N
O5 La1 2.931(6) . -101_434 N
O5 La1 2.931(6) . -101_444 N
O5 Sr1 2.931(6) . 101_544 N
O5 Sr1 2.931(6) . 101_554 N
O5 Sr1 2.931(6) . -101_434 N
O5 Sr1 2.931(6) . -101_444 N
O5 O4 1.90(4) . 1_555 N
O5 O4 1.04(4) . 2_655 N
O5 O4 1.90(4) . 3_655 N
O5 O4 1.04(4) . 4_555 N
O5 O4 1.90(4) . 5_655 N
O5 O4 1.04(4) . 6_655 N
O5 O4 1.90(4) . 7_555 N
O5 O4 1.04(4) . 8_555 N
O5 Co1 1.91208(6) . 1_555 N
O5 Co1 1.91208(6) . 1_655 N
loop_
_pd_meas_intensity_total
_pd_proc_ls_weight
_pd_proc_intensity_bkg_calc
_pd_calc_intensity_total
971(31) 0.0 717.0 .
1187(35) 0.0 716.3 .
1353(37) 0.0 716. .
1531(39) 0.0 715. .
1660(41) 0.0 715. .
1805(43) 0.0 714. .
1867(43) 0.0 713. .
1904(44) 0.0 713. .
1590(40) 0.0 712. .
1346(37) 0.0 712. .
1058(33) 0.0 711.1 .
733(27) 0.0 710.5 .
365(19) 0.0 709.9 .
224(15) 0.0 709.4 .
170(13) 0.0 708.8 .
162(13) 0.0 708.2 .
171(13) 0.0 707.7 .
153(12) 0.0 707.1 .
174(13) 0.0 706.6 .
188(14) 0.0 706.1 .
179(13) 0.0 705.5 .
251(16) 0.0 705.0 .
475(22) 0.0 704.5 .
760(27) 0.0 703.9 .
793(28) 0.0 703.4 .
591(24) 0.0 702.9 .
430(21) 0.0 702.4 .
384(20) 0.0 701.9 .
320(18) 0.0 701.3 .
364(19) 0.0 700.8 .
340(18) 0.0 700.3 .
401(20) 0.0 699.8 .
414(20) 0.0 699.3 .
451(21) 0.0 698.8 .
451(21) 0.0 698.3 .
421(20) 0.0 697.9 .
407(20) 0.0 697.4 .
439(21) 0.0 696.9 .
410(20) 0.0 696.4 .
414(20) 0.0 695.9 .
417(20) 0.0 695.5 .
386(20) 0.0 695.0 .
402(20) 0.0 694.5 .
393(20) 0.0 694.1 .
358(19) 0.0 693.6 .
328(18) 0.0 693.2 .
358(19) 0.0 692.7 .
359(19) 0.0 692.2 .
329(18) 0.0 691.8 .
336(18) 0.0 691.4 .
323(18) 0.0 690.9 .
369(19) 0.0 690.5 .
459(21) 0.0 690.0 .
479(22) 0.0 689.6 .
503(22) 0.0 689.2 .
535(23) 0.0 688.8 .
582(24) 0.0 688.3 .
615(25) 0.0 687.9 .
619(25) 0.0 687.5 .
655(25) 0.0 687.1 .
684(26) 0.0 686.7 .
728(27) 0.0 686.2 .
700(26) 0.0 685.8 .
722(27) 0.0 685.4 .
708(27) 0.0 685.0 .
668(26) 0.0 684.6 .
678(26) 0.0 684.2 .
697(26) 0.0 683.8 .
739(27) 0.0 683.5 .
760(27) 0.0 683.1 .
690(26) 0.0 682.7 .
700(26) 0.0 682.3 .
703(26) 0.0 681.9 .
735(27) 0.0 681.5 .
738(27) 0.0 681.2 .
702(26) 0.0 680.8 .
734(27) 0.0 680.4 .
703(27) 0.0 680.1 .
749(28) 0.0 679.7 .
743(27) 0.0 679.3 .
725(27) 0.0 679.0 .
751(27) 0.0 678.6 .
723(27) 0.0 678.3 .
651(25) 0.0 677.9 .
674(26) 0.0 677.6 .
658(26) 0.0 677.2 .
611(25) 0.0 676.9 .
637(25) 0.0 676.5 .
650(25) 0.0 676.2 .
696(26) 0.0 675.9 .
677(26) 0.0 675.5 .
674(26) 0.001479 675.2 675.3
670(26) 0.001479 674.9 675.0
610(24) 0.001736 674.5 674.6
652(25) 0.001600 674.2 674.3
673(26) 0.001479 673.9 673.9
695(26) 0.001479 673.6 673.6
640(25) 0.001600 673.2 673.3
644(25) 0.001600 672.9 673.0
650(25) 0.001600 672.6 672.7
653(25) 0.001600 672.3 672.3
627(25) 0.001600 672.0 672.0
680(26) 0.001479 671.7 671.7
661(26) 0.001479 671.4 671.4
662(26) 0.001479 671.1 671.1
664(26) 0.001479 670.8 670.8
681(26) 0.001479 670.5 670.5
661(26) 0.001479 670.2 670.2
670(26) 0.001479 669.9 669.9
664(26) 0.001479 669.6 669.6
716(27) 0.001372 669.3 669.3
621(25) 0.001600 669.0 669.0
656(26) 0.001479 668.7 668.7
643(25) 0.001600 668.5 668.5
648(25) 0.001600 668.2 668.2
628(25) 0.001600 667.9 667.9
659(26) 0.001479 667.6 667.6
695(26) 0.001479 667.3 667.3
694(26) 0.001479 667.1 667.1
656(25) 0.001600 666.8 666.8
661(26) 0.001479 666.5 666.5
602(24) 0.001736 666.3 666.3
675(26) 0.001479 666.0 666.0
649(25) 0.001600 665.7 665.7
646(25) 0.001600 665.5 665.5
669(26) 0.001479 665.2 665.5
671(26) 0.001479 665.0 665.2
670(26) 0.001479 664.7 665.0
668(26) 0.001479 664.5 664.8
691(26) 0.001479 664.2 664.6
661(25) 0.001600 664.0 664.3
659(26) 0.001479 663.7 664.1
627(25) 0.001600 663.5 663.9
636(25) 0.001600 663.2 663.7
664(26) 0.001479 663.0 663.6
681(26) 0.001479 662.7 663.4
659(26) 0.001479 662.5 663.2
667(26) 0.001479 662.3 663.1
667(26) 0.001479 662.0 663.0
693(26) 0.001479 661.8 662.9
687(26) 0.001479 661.6 662.8
661(26) 0.001479 661.3 662.8
644(26) 0.001479 661.1 662.9
659(26) 0.001479 660.9 663.1
726(27) 0.001372 660.7 663.6
706(26) 0.001479 660.4 665.1
705(27) 0.001372 660.2 669.8
692(26) 0.001479 660.0 682.6
777(28) 0.001276 659.8 711.9
743(27) 0.001372 659.6 765.0
817(28) 0.001276 659.4 838.3
827(28) 0.001276 659.1 909.2
930(30) 0.001111 658.9 942.3
915(30) 0.001111 658.7 916.5
907(30) 0.001111 658.5 848.2
833(29) 0.001189 658.3 773.0
779(28) 0.001276 658.1 716.1
716(27) 0.001372 657.9 683.4
697(26) 0.001479 657.7 668.4
692(26) 0.001479 657.5 662.6
643(25) 0.001600 657.3 660.4
638(25) 0.001600 657.1 659.4
670(26) 0.001479 656.9 658.8
690(26) 0.001479 656.7 658.3
675(26) 0.001479 656.5 657.8
654(25) 0.001600 656.3 657.5
662(26) 0.001479 656.2 657.1
664(26) 0.001479 656.0 656.8
655(25) 0.001600 655.8 656.5
659(26) 0.001479 655.6 656.3
700(26) 0.001479 655.4 656.0
652(25) 0.001600 655.2 655.8
607(25) 0.001600 655.1 655.5
638(26) 0.001479 654.9 655.3
690(27) 0.001372 654.7 655.1
643(26) 0.001479 654.5 654.9
624(25) 0.001600 654.4 654.7
654(26) 0.001479 654.2 654.5
706(26) 0.001479 654.0 654.3
651(26) 0.001479 653.8 653.8
658(25) 0.001600 653.7 653.7
697(26) 0.001479 653.5 653.5
703(26) 0.001479 653.4 653.4
642(25) 0.001600 653.2 653.2
663(26) 0.001479 653.0 653.0
706(26) 0.001479 652.9 652.9
687(26) 0.001479 652.7 652.7
640(25) 0.001600 652.5 652.5
624(25) 0.001600 652.4 652.4
663(26) 0.001479 652.2 652.2
648(25) 0.001600 652.1 652.1
629(25) 0.001600 651.9 651.9
630(25) 0.001600 651.8 651.8
662(26) 0.001479 651.6 651.6
666(26) 0.001479 651.5 651.5
702(26) 0.001479 651.3 651.3
705(26) 0.001479 651.2 651.2
705(26) 0.001479 651.0 651.0
667(26) 0.001479 650.9 650.9
655(26) 0.001479 650.7 650.8
693(26) 0.001479 650.6 650.6
689(26) 0.001479 650.5 650.5
690(26) 0.001479 650.3 650.3
663(26) 0.001479 650.2 650.2
736(27) 0.001372 650.0 650.1
642(26) 0.001479 649.9 649.9
674(26) 0.001479 649.8 649.8
701(27) 0.001372 649.6 649.7
686(26) 0.001479 649.5 649.5
666(26) 0.001479 649.4 649.4
631(25) 0.001600 649.2 649.3
672(26) 0.001479 649.1 649.2
667(26) 0.001479 649.0 649.0
610(24) 0.001736 648.9 648.9
698(27) 0.001372 648.7 648.8
647(25) 0.001600 648.6 648.7
640(24) 0.001736 648.5 648.6
680(27) 0.001372 648.4 648.5
658(25) 0.001600 648.2 648.4
676(26) 0.001479 648.1 648.3
654(26) 0.001479 648.0 648.3
656(25) 0.001600 647.9 648.4
654(25) 0.001600 647.8 649.0
697(26) 0.001479 647.6 650.4
706(26) 0.001479 647.5 653.2
667(26) 0.001479 647.4 656.9
669(26) 0.001479 647.3 660.2
655(25) 0.001600 647.2 661.2
619(25) 0.001600 647.1 659.1
646(25) 0.001600 647.0 655.3
660(26) 0.001479 646.8 651.5
659(26) 0.001479 646.7 648.9
645(25) 0.001600 646.6 647.6
656(26) 0.001479 646.5 646.9
627(25) 0.001600 646.4 646.6
632(25) 0.001600 646.3 646.5
653(26) 0.001479 646.2 646.3
650(26) 0.001479 646.1 646.2
645(26) 0.001479 646.0 646.1
640(25) 0.001600 645.9 646.0
677(26) 0.001479 645.8 645.8
676(26) 0.001479 645.7 645.7
622(25) 0.001600 645.6 645.6
639(25) 0.001600 645.5 645.5
650(25) 0.001600 645.4 645.4
653(26) 0.001479 645.3 645.3
625(25) 0.001600 645.2 645.2
657(25) 0.001600 645.1 645.1
661(26) 0.001479 645.0 645.0
643(25) 0.001600 644.9 644.9
615(25) 0.001600 644.8 644.8
604(24) 0.001736 644.7 644.7
642(25) 0.001600 644.6 644.6
633(25) 0.001600 644.5 644.6
659(25) 0.001600 644.4 644.5
641(25) 0.001600 644.4 644.4
639(25) 0.001600 644.3 644.3
648(25) 0.001600 644.2 644.2
669(26) 0.001479 644.1 644.1
656(25) 0.001600 644.0 644.0
702(26) 0.001479 643.9 643.9
639(25) 0.001600 643.8 643.8
635(25) 0.001600 643.8 643.9
682(26) 0.001479 643.7 643.8
641(25) 0.001600 643.6 643.8
627(25) 0.001600 643.5 643.7
668(26) 0.001479 643.4 643.6
679(26) 0.001479 643.3 643.6
631(25) 0.001600 643.3 643.5
640(26) 0.001479 643.2 643.4
643(26) 0.001479 643.1 643.4
610(25) 0.001600 643.0 643.3
663(26) 0.001479 642.9 643.3
655(25) 0.001600 642.9 643.3
643(25) 0.001600 642.8 643.2
634(25) 0.001600 642.7 643.2
679(26) 0.001479 642.6 643.2
625(25) 0.001600 642.6 643.2
650(25) 0.001600 642.5 643.2
650(25) 0.001600 642.4 643.2
630(25) 0.001600 642.3 643.3
637(25) 0.001600 642.3 643.4
636(25) 0.001600 642.2 643.5
648(25) 0.001600 642.1 643.7
640(25) 0.001600 642.1 644.1
663(26) 0.001479 642.0 644.7
603(24) 0.001736 641.9 646.1
628(25) 0.001600 641.8 650.4
636(25) 0.001600 641.8 661.7
670(26) 0.001479 641.7 686.4
729(27) 0.001372 641.6 727.9
793(28) 0.001276 641.6 778.2
802(28) 0.001276 641.5 814.4
842(29) 0.001189 641.4 812.3
826(29) 0.001189 641.4 773.4
763(27) 0.001372 641.3 723.1
736(27) 0.001372 641.3 683.1
672(26) 0.001479 641.2 660.1
605(24) 0.001736 641.1 650.4
647(25) 0.001600 641.1 648.4
626(25) 0.001600 641.0 650.3
597(25) 0.001600 640.9 654.0
623(25) 0.001600 640.9 657.1
634(25) 0.001600 640.8 657.2
648(25) 0.001600 640.8 653.9
610(25) 0.001600 640.7 649.3
648(25) 0.001600 640.6 645.4
663(26) 0.001479 640.6 643.1
596(24) 0.001736 640.5 642.0
626(25) 0.001600 640.5 641.5
602(24) 0.001736 640.4 641.4
648(25) 0.001600 640.3 641.3
653(25) 0.001600 640.3 641.2
626(25) 0.001600 640.2 641.0
613(25) 0.001600 640.2 640.8
627(25) 0.001600 640.1 640.6
649(25) 0.001600 640.1 640.5
598(24) 0.001736 640.0 640.4
611(25) 0.001600 639.9 640.3
643(25) 0.001600 639.9 640.2
639(25) 0.001600 639.8 640.1
620(25) 0.001600 639.8 640.1
635(25) 0.001600 639.7 640.0
596(24) 0.001736 639.7 639.8
636(25) 0.001600 639.6 639.7
645(25) 0.001600 639.6 639.7
657(26) 0.001479 639.5 639.6
628(25) 0.001600 639.5 639.6
643(25) 0.001600 639.4 639.5
643(25) 0.001600 639.4 639.5
643(25) 0.001600 639.3 639.5
617(25) 0.001600 639.3 639.4
623(25) 0.001600 639.2 639.4
614(25) 0.001600 639.2 639.3
591(25) 0.001600 639.1 639.3
659(26) 0.001479 639.1 639.3
609(24) 0.001736 639.0 639.3
624(25) 0.001600 639.0 639.3
608(25) 0.001600 638.9 639.3
598(24) 0.001736 638.9 639.4
623(25) 0.001600 638.8 639.5
595(24) 0.001736 638.8 640.0
627(25) 0.001600 638.7 641.4
624(25) 0.001600 638.7 644.9
633(25) 0.001600 638.6 651.9
659(26) 0.001479 638.6 662.3
623(25) 0.001600 638.5 672.7
640(26) 0.001479 638.5 676.9
642(25) 0.001600 638.4 671.6
664(26) 0.001479 638.4 660.8
647(25) 0.001600 638.4 650.6
640(25) 0.001600 638.3 643.9
656(25) 0.001600 638.3 640.7
587(24) 0.001736 638.2 639.4
623(25) 0.001600 638.2 638.9
592(24) 0.001736 638.1 638.6
600(24) 0.001736 638.1 638.5
618(25) 0.001600 638.0 638.4
595(24) 0.001736 638.0 638.3
647(25) 0.001600 638.0 638.2
644(25) 0.001600 637.9 638.8
620(25) 0.001600 637.9 638.8
596(24) 0.001736 637.8 638.7
616(25) 0.001600 637.8 638.7
611(25) 0.001600 637.7 638.7
647(26) 0.001479 637.7 638.7
616(25) 0.001600 637.7 638.7
621(25) 0.001600 637.6 638.8
661(26) 0.001479 637.6 638.8
668(26) 0.001479 637.5 638.8
652(25) 0.001600 637.5 638.9
607(25) 0.001600 637.5 638.9
634(25) 0.001600 637.4 639.0
624(25) 0.001600 637.4 639.1
620(25) 0.001600 637.3 639.3
628(25) 0.001600 637.3 639.4
629(25) 0.001600 637.2 639.7
629(25) 0.001600 637.2 640.0
586(24) 0.001736 637.2 642.5
591(24) 0.001736 637.1 643.1
591(24) 0.001736 637.1 643.7
619(25) 0.001600 637.0 644.2
629(25) 0.001600 637.0 644.8
643(25) 0.001600 637.0 645.6
615(25) 0.001600 636.9 646.7
597(24) 0.001736 636.9 648.2
623(25) 0.001600 636.8 650.3
621(25) 0.001600 636.8 653.3
680(26) 0.001479 636.8 658.7
689(26) 0.001479 636.7 672.2
742(27) 0.001372 636.7 709.2
778(28) 0.001276 636.6 799.8
913(30) 0.001111 636.6 973.6
1177(34) 0.000865 636.6 1217.0
1428(38) 0.000693 637. 1433.
1458(38) 0.000693 636. 1478.
1348(37) 0.000730 636. 1313.
1158(34) 0.000865 636.4 1065.5
894(30) 0.001111 636.4 861.1
755(28) 0.001276 636.3 742.9
676(26) 0.001479 636.3 691.9
664(25) 0.001600 636.3 674.7
683(26) 0.001479 636.2 670.6
653(25) 0.001600 636.2 671.2
670(26) 0.001479 636.1 674.5
679(26) 0.001479 636.1 680.8
714(27) 0.001372 636.1 693.4
727(27) 0.001372 636.0 725.8
761(27) 0.001372 636.0 816.8
1005(32) 0.000977 635.9 1050.3
1443(38) 0.000693 636. 1524.
2158(46) 0.000473 636. 2230.
2858(53) 0.000356 636. 2920.
3181(56) 0.0003189 636. 3148.
2784(52) 0.000370 636. 2721.
2136(46) 0.000473 636. 1982.
1438(38) 0.000693 636. 1338.
950(30) 0.001111 635.6 951.8
730(27) 0.001372 635.6 778.5
712(27) 0.001372 635.6 715.7
696(26) 0.001479 635.5 693.0
676(26) 0.001479 635.5 680.6
682(26) 0.001479 635.4 671.0
655(26) 0.001479 635.4 663.5
680(26) 0.001479 635.4 658.3
640(25) 0.001600 635.3 654.7
620(25) 0.001600 635.3 652.3
687(26) 0.001479 635.3 650.6
650(26) 0.001479 635.2 649.4
650(26) 0.001479 635.2 647.8
672(27) 0.001372 635.1 647.3
667(26) 0.001479 635.1 647.2
647(25) 0.001600 635.1 647.4
663(26) 0.001479 635.0 648.1
657(26) 0.001479 635.0 649.8
687(26) 0.001479 634.9 654.1
694(26) 0.001479 634.9 666.6
650(25) 0.001600 634.9 701.0
796(28) 0.001276 634.8 777.4
947(31) 0.001041 634.8 903.7
1067(33) 0.000918 634.8 1046.0
1099(33) 0.000918 634.7 1121.2
1051(32) 0.000977 634.7 1066.3
989(31) 0.001041 634.6 928.6
808(28) 0.001276 634.6 795.1
687(26) 0.001479 634.6 709.3
652(25) 0.001600 634.5 668.6
642(25) 0.001600 634.5 650.9
641(25) 0.001600 634.4 645.4
631(25) 0.001600 634.4 643.0
606(24) 0.001736 634.4 641.7
599(24) 0.001736 634.3 641.0
640(25) 0.001600 634.3 640.7
642(25) 0.001600 634.2 641.3
628(25) 0.001600 634.2 644.1
660(26) 0.001479 634.2 651.9
668(26) 0.001479 634.1 668.0
693(26) 0.001479 634.1 691.2
708(27) 0.001372 634.0 712.0
733(27) 0.001372 634.0 715.4
735(27) 0.001372 634.0 698.3
700(27) 0.001372 633.9 674.3
653(26) 0.001479 633.9 655.5
596(25) 0.001600 633.8 645.4
654(26) 0.001479 633.8 641.3
698(26) 0.001479 633.8 640.2
631(25) 0.001600 633.7 640.3
641(25) 0.001600 633.7 641.2
617(25) 0.001600 633.6 643.1
648(25) 0.001600 633.6 648.4
691(26) 0.001479 633.6 663.5
727(27) 0.001372 633.5 701.1
824(29) 0.001189 633.5 772.8
889(30) 0.001111 633.4 869.9
960(31) 0.001041 633.4 947.3
992(31) 0.001041 633.4 945.0
878(29) 0.001189 633.3 864.5
785(28) 0.001276 633.3 767.7
697(26) 0.001479 633.2 697.5
680(26) 0.001479 633.2 661.0
673(26) 0.001479 633.1 646.4
661(25) 0.001600 633.1 641.7
675(26) 0.001479 633.1 639.5
668(26) 0.001479 633.0 638.3
668(26) 0.001479 633.0 638.8
668(26) 0.001479 632.9 638.3
679(26) 0.001479 632.9 637.9
663(26) 0.001479 632.8 637.6
681(26) 0.001479 632.8 637.5
674(26) 0.001479 632.8 637.4
648(25) 0.001600 632.7 637.4
658(26) 0.001479 632.7 637.4
693(26) 0.001479 632.6 637.5
680(26) 0.001479 632.6 637.6
667(26) 0.001479 632.5 637.8
654(26) 0.001479 632.5 638.1
614(25) 0.001600 632.5 638.4
655(26) 0.001479 632.4 638.8
639(25) 0.001600 632.4 639.4
648(25) 0.001600 632.3 640.0
607(25) 0.001600 632.3 640.7
670(26) 0.001479 632.2 641.6
676(26) 0.001479 632.2 642.8
664(26) 0.001479 632.1 644.1
643(25) 0.001600 632.1 645.8
618(25) 0.001600 632.0 649.1
658(26) 0.001479 632.0 651.9
684(26) 0.001479 632.0 655.6
706(26) 0.001479 631.9 660.6
735(27) 0.001372 631.9 667.9
699(26) 0.001479 631.8 682.2
741(27) 0.001372 631.8 715.9
744(27) 0.001372 631.7 798.1
991(31) 0.001041 631.7 970.4
1283(36) 0.000772 632. 1258.
1630(40) 0.000625 632. 1632.
2052(45) 0.000494 632. 1999.
2331(48) 0.000434 631. 2285.
2438(49) 0.000416 631. 2406.
2190(47) 0.000453 631. 2192.
1678(41) 0.000595 631. 1710.
1204(35) 0.000816 631.3 1233.6
952(31) 0.001041 631.3 918.3
828(29) 0.001189 631.2 764.1
776(28) 0.001276 631.2 703.6
768(28) 0.001276 631.1 681.0
749(28) 0.001276 631.1 670.9
757(28) 0.001276 631.0 665.2
748(27) 0.001372 631.0 661.6
719(27) 0.001372 630.9 659.6
730(27) 0.001372 630.9 658.9
681(26) 0.001479 630.8 659.4
727(27) 0.001372 630.8 661.5
690(26) 0.001479 630.7 666.1
725(27) 0.001372 630.7 676.8
758(27) 0.001372 630.6 707.0
781(28) 0.001276 630.6 790.7
967(31) 0.001041 630.5 980.4
1224(35) 0.000816 630.5 1296.2
1512(39) 0.000657 630. 1643.
1684(41) 0.000595 630. 1791.
1556(39) 0.000657 630. 1600.
1278(35) 0.000816 630.3 1245.0
988(31) 0.001041 630.2 943.4
791(28) 0.001276 630.2 770.4
697(26) 0.001479 630.1 695.9
679(26) 0.001479 630.1 668.6
668(26) 0.001479 630.0 657.8
680(26) 0.001479 630.0 652.0
650(25) 0.001600 629.9 648.1
661(26) 0.001479 629.9 644.6
677(26) 0.001479 629.8 642.5
664(26) 0.001479 629.7 640.9
662(26) 0.001479 629.7 638.3
650(25) 0.001600 629.6 637.4
678(26) 0.001479 629.6 636.7
680(26) 0.001479 629.5 636.2
663(26) 0.001479 629.5 638.6
635(26) 0.001479 629.4 638.5
635(25) 0.001600 629.4 638.6
661(26) 0.001479 629.3 638.8
680(26) 0.001479 629.3 639.2
653(25) 0.001600 629.2 639.9
676(26) 0.001479 629.2 640.9
650(25) 0.001600 629.1 642.4
633(25) 0.001600 629.0 645.1
674(26) 0.001479 629.0 651.5
678(26) 0.001479 628.9 668.7
711(26) 0.001479 628.9 710.8
862(29) 0.001189 628.8 789.6
936(30) 0.001111 628.8 891.4
981(31) 0.001041 628.7 959.8
940(30) 0.001111 628.7 933.1
807(28) 0.001276 628.6 838.6
713(26) 0.001479 628.5 744.8
689(26) 0.001479 628.5 687.2
697(26) 0.001479 628.4 661.7
650(25) 0.001600 628.4 653.1
648(25) 0.001600 628.3 650.9
669(26) 0.001479 628.3 651.3
675(26) 0.001479 628.2 653.3
665(26) 0.001479 628.1 658.1
654(25) 0.001600 628.1 669.5
687(26) 0.001479 628.0 692.0
702(26) 0.001479 628.0 725.5
757(27) 0.001372 627.9 757.8
766(28) 0.001276 627.9 767.5
760(27) 0.001372 627.8 752.0
732(27) 0.001372 627.7 733.7
733(27) 0.001372 627.7 730.7
765(28) 0.001276 627.6 755.0
856(29) 0.001189 627.6 839.1
1103(33) 0.000918 627.5 1078.0
1649(40) 0.000625 627. 1635.
2672(52) 0.000370 627. 2593.
3729(61) 0.0002687 627. 3679.
4125(64) 0.0002441 627. 4158.
3500(59) 0.0002873 627. 3554.
2390(48) 0.000434 627. 2456.
1522(38) 0.000693 627. 1556.
985(31) 0.001041 627.0 1065.5
751(27) 0.001372 627.0 866.7
733(27) 0.001372 626.9 788.3
720(27) 0.001372 626.8 742.2
689(26) 0.001479 626.8 708.7
638(25) 0.001600 626.7 686.3
625(25) 0.001600 626.7 672.3
640(25) 0.001600 626.6 664.0
662(26) 0.001479 626.5 658.5
650(25) 0.001600 626.5 654.5
655(25) 0.001600 626.4 651.7
629(25) 0.001600 626.3 649.9
647(25) 0.001600 626.3 649.6
656(25) 0.001600 626.2 652.5
661(26) 0.001479 626.2 664.0
685(26) 0.001479 626.1 692.4
740(27) 0.001372 626.0 741.0
817(28) 0.001276 626.0 793.6
790(28) 0.001276 625.9 811.4
756(27) 0.001372 625.8 775.6
722(27) 0.001372 625.8 721.2
715(27) 0.001372 625.7 682.5
669(26) 0.001479 625.6 668.8
672(26) 0.001479 625.6 671.9
629(25) 0.001600 625.5 676.8
645(25) 0.001600 625.5 671.4
608(25) 0.001600 625.4 657.9
640(25) 0.001600 625.3 645.2
614(25) 0.001600 625.3 637.3
614(25) 0.001600 625.2 633.6
624(25) 0.001600 625.1 632.0
604(24) 0.001736 625.1 631.1
600(24) 0.001736 625.0 630.5
623(25) 0.001600 624.9 629.9
640(25) 0.001600 624.9 629.3
632(25) 0.001600 624.8 626.1
621(25) 0.001600 624.7 625.9
606(24) 0.001736 624.7 625.8
633(25) 0.001600 624.6 625.6
617(25) 0.001600 624.5 625.5
648(25) 0.001600 624.5 625.4
618(25) 0.001600 624.4 625.4
623(25) 0.001600 624.3 625.7
625(25) 0.001600 624.3 626.2
610(24) 0.001736 624.2 626.6
618(25) 0.001600 624.1 626.5
597(24) 0.001736 624.1 625.9
597(24) 0.001736 624.0 625.3
596(24) 0.001736 623.9 624.8
597(24) 0.001736 623.9 624.6
626(25) 0.001600 623.8 624.4
616(25) 0.001600 623.7 624.3
620(25) 0.001600 623.7 624.3
619(25) 0.001600 623.6 624.2
600(25) 0.001600 623.5 624.2
620(25) 0.001600 623.5 624.1
616(25) 0.001600 623.4 624.1
604(24) 0.001736 623.3 623.9
617(25) 0.001600 623.2 623.9
635(25) 0.001600 623.2 623.9
626(25) 0.001600 623.1 623.9
605(25) 0.001600 623.0 624.7
611(25) 0.001600 623.0 624.8
613(25) 0.001600 622.9 624.9
634(25) 0.001600 622.8 625.0
651(25) 0.001600 622.8 625.2
618(25) 0.001600 622.7 625.5
608(25) 0.001600 622.6 625.9
649(25) 0.001600 622.6 626.5
624(25) 0.001600 622.5 627.3
580(24) 0.001736 622.4 628.8
626(25) 0.001600 622.3 632.4
661(26) 0.001479 622.3 642.0
660(25) 0.001600 622.2 663.0
701(26) 0.001479 622.1 696.7
721(27) 0.001372 622.1 729.7
715(27) 0.001372 622.0 735.2
689(26) 0.001479 621.9 708.9
624(25) 0.001600 621.8 678.7
597(24) 0.001736 621.8 663.3
655(25) 0.001600 621.7 662.3
676(26) 0.001479 621.6 663.7
650(26) 0.001479 621.6 657.4
652(25) 0.001600 621.5 647.4
661(26) 0.001479 621.4 640.2
630(25) 0.001600 621.3 637.5
646(26) 0.001479 621.3 636.8
656(26) 0.001479 621.2 635.9
599(24) 0.001736 621.1 635.0
635(25) 0.001600 621.1 635.1
643(25) 0.001600 621.0 636.5
625(25) 0.001600 620.9 639.2
620(25) 0.001600 620.8 643.5
660(26) 0.001479 620.8 650.5
637(25) 0.001600 620.7 664.8
706(26) 0.001479 620.6 702.0
772(28) 0.001276 620.5 798.1
1008(31) 0.001041 620.5 996.3
1355(36) 0.000772 620. 1285.
1599(40) 0.000625 620. 1515.
1498(38) 0.000693 620. 1470.
1221(35) 0.000816 620.2 1199.6
895(29) 0.001189 620.1 932.0
733(27) 0.001372 620.0 772.0
684(26) 0.001479 620.0 709.2
685(26) 0.001479 619.9 696.9
721(27) 0.001372 619.8 696.8
667(26) 0.001479 619.7 687.0
631(25) 0.001600 619.7 670.3
600(24) 0.001736 619.6 659.7
627(25) 0.001600 619.5 662.0
651(25) 0.001600 619.4 675.8
663(26) 0.001479 619.4 690.0
668(26) 0.001479 619.3 687.7
653(25) 0.001600 619.2 669.2
637(25) 0.001600 619.1 650.0
657(26) 0.001479 619.1 637.7
629(25) 0.001600 619.0 632.0
642(26) 0.001479 618.9 629.8
648(26) 0.001479 618.8 629.0
642(25) 0.001600 618.8 628.7
644(25) 0.001600 618.7 628.8
625(25) 0.001600 618.6 629.2
648(25) 0.001600 618.5 630.2
603(24) 0.001736 618.5 631.9
623(25) 0.001600 618.4 634.6
642(25) 0.001600 618.3 637.6
637(25) 0.001600 618.2 640.2
653(25) 0.001600 618.2 642.4
641(25) 0.001600 618.1 646.1
645(25) 0.001600 618.0 653.3
692(26) 0.001479 617.9 669.3
744(27) 0.001372 617.8 711.5
854(29) 0.001189 617.8 819.2
1080(32) 0.000977 617.7 1037.4
1419(37) 0.000730 618. 1346.
1577(39) 0.000657 618. 1573.
1464(38) 0.000693 617. 1493.
1161(34) 0.000865 617.4 1196.9
915(30) 0.001111 617.3 929.8
759(27) 0.001372 617.2 784.7
692(26) 0.001479 617.2 736.5
681(26) 0.001479 617.1 724.1
679(26) 0.001479 617.0 704.4
683(26) 0.001479 616.9 676.4
661(26) 0.001479 616.9 653.3
662(26) 0.001479 616.8 639.6
663(26) 0.001479 616.7 632.8
645(26) 0.001479 616.6 629.2
633(25) 0.001600 616.5 627.0
639(26) 0.001479 616.5 625.4
604(25) 0.001600 616.4 624.1
617(25) 0.001600 616.3 623.1
652(25) 0.001600 616.2 622.3
627(25) 0.001600 616.2 621.6
619(25) 0.001600 616.1 621.0
597(24) 0.001736 616.0 620.5
595(24) 0.001736 615.9 620.1
609(24) 0.001736 615.9 619.8
613(25) 0.001600 615.8 619.5
616(25) 0.001600 615.7 619.2
609(24) 0.001736 615.6 619.0
614(25) 0.001600 615.5 618.9
645(25) 0.001600 615.5 618.8
658(26) 0.001479 615.4 618.7
626(25) 0.001600 615.3 618.7
586(24) 0.001736 615.2 618.7
613(24) 0.001736 615.2 618.8
615(25) 0.001600 615.1 619.0
628(25) 0.001600 615.0 619.3
646(25) 0.001600 614.9 619.9
625(25) 0.001600 614.8 621.0
602(24) 0.001736 614.8 623.4
625(25) 0.001600 614.7 628.1
652(25) 0.001600 614.6 635.3
662(26) 0.001479 614.5 642.4
675(26) 0.001479 614.5 648.8
655(25) 0.001600 614.4 659.3
657(26) 0.001479 614.3 689.3
738(27) 0.001372 614.2 746.3
822(29) 0.001189 614.1 809.3
848(30) 0.001111 614.1 823.4
800(29) 0.001189 614.0 770.0
712(27) 0.001372 613.9 702.8
636(25) 0.001600 613.8 656.8
658(26) 0.001479 613.8 634.5
643(25) 0.001600 613.7 625.9
618(25) 0.001600 613.6 622.3
673(26) 0.001479 613.5 620.4
614(25) 0.001600 613.4 619.2
636(25) 0.001600 613.4 618.3
646(25) 0.001600 613.3 617.7
647(25) 0.001600 613.2 617.2
636(25) 0.001600 613.1 616.9
662(26) 0.001479 613.1 616.7
676(26) 0.001479 613.0 616.5
651(25) 0.001600 612.9 616.4
628(25) 0.001600 612.8 616.4
644(25) 0.001600 612.7 616.4
642(25) 0.001600 612.7 616.6
642(25) 0.001600 612.6 618.8
625(25) 0.001600 612.5 619.5
613(25) 0.001600 612.4 621.3
629(25) 0.001600 612.4 625.3
655(26) 0.001479 612.3 632.3
658(25) 0.001600 612.2 640.3
684(26) 0.001479 612.1 643.5
679(26) 0.001479 612.0 638.6
649(25) 0.001600 612.0 631.3
624(25) 0.001600 611.9 626.4
622(25) 0.001600 611.8 624.5
649(26) 0.001479 611.7 624.5
642(25) 0.001600 611.7 625.4
649(26) 0.001479 611.6 626.8
625(26) 0.001479 611.5 628.9
633(25) 0.001600 611.4 631.7
633(25) 0.001600 611.3 635.5
667(26) 0.001479 611.3 641.0
675(26) 0.001479 611.2 649.8
681(26) 0.001479 611.1 667.8
705(26) 0.001479 611.0 712.3
826(29) 0.001189 611.0 816.4
1041(32) 0.000977 610.9 1006.4
1298(36) 0.000772 611. 1239.
1357(37) 0.000730 611. 1349.
1196(34) 0.000865 610.7 1215.2
967(31) 0.001041 610.6 1000.1
860(29) 0.001189 610.5 861.2
824(29) 0.001189 610.4 829.2
805(28) 0.001276 610.3 852.5
834(29) 0.001189 610.3 848.7
819(29) 0.001189 610.2 792.7
760(27) 0.001372 610.1 731.3
689(26) 0.001479 610.0 693.0
651(25) 0.001600 610.0 678.3
651(25) 0.001600 609.9 678.3
683(26) 0.001479 609.8 687.0
720(27) 0.001372 609.7 704.9
754(27) 0.001372 609.6 742.1
879(30) 0.001111 609.6 833.8
1126(33) 0.000918 609.5 1063.2
1558(39) 0.000657 609. 1533.
2281(48) 0.000434 609. 2219.
2833(53) 0.000356 609. 2760.
2624(51) 0.000384 609. 2599.
1883(44) 0.000517 609. 1927.
1219(35) 0.000816 609.0 1307.2
866(30) 0.001111 609.0 943.4
730(27) 0.001372 608.9 781.3
669(26) 0.001479 608.8 716.8
635(25) 0.001600 608.7 687.5
657(26) 0.001479 608.6 670.8
667(25) 0.001600 608.6 660.6
684(27) 0.001372 608.5 655.5
665(26) 0.001479 608.4 654.8
684(26) 0.001479 608.3 656.0
647(25) 0.001600 608.3 653.6
671(26) 0.001479 608.2 645.6
642(25) 0.001600 608.1 637.1
629(25) 0.001600 608.0 630.9
644(25) 0.001600 608.0 627.3
636(25) 0.001600 607.9 625.3
637(25) 0.001600 607.8 623.9
653(25) 0.001600 607.7 622.9
630(25) 0.001600 607.7 622.2
643(25) 0.001600 607.6 621.7
666(26) 0.001479 607.5 621.5
623(25) 0.001600 607.4 620.7
603(24) 0.001736 607.4 620.8
621(25) 0.001600 607.3 621.0
610(24) 0.001736 607.2 621.4
595(24) 0.001736 607.1 622.1
615(25) 0.001600 607.1 623.1
633(25) 0.001600 607.0 624.2
661(26) 0.001479 606.9 626.1
661(26) 0.001479 606.8 628.8
640(25) 0.001600 606.8 633.3
650(26) 0.001479 606.7 642.5
696(27) 0.001372 606.6 662.4
746(28) 0.001276 606.5 699.7
764(28) 0.001276 606.5 751.4
848(29) 0.001189 606.4 790.6
804(28) 0.001276 606.3 781.9
728(27) 0.001372 606.2 745.9
714(27) 0.001372 606.2 722.8
727(27) 0.001372 606.1 734.9
845(29) 0.001189 606.0 810.1
1052(32) 0.000977 605.9 1003.3
1361(37) 0.000730 606. 1372.
1783(42) 0.000567 606. 1849.
2016(45) 0.000494 606. 2119.
1863(43) 0.000541 606. 1880.
1484(38) 0.000693 606. 1411.
1099(33) 0.000918 605.5 1045.1
832(29) 0.001189 605.4 853.0
717(27) 0.001372 605.3 767.8
703(26) 0.001479 605.3 718.2
672(26) 0.001479 605.2 682.9
645(25) 0.001600 605.1 659.6
629(25) 0.001600 605.0 645.7
607(25) 0.001600 605.0 637.6
621(25) 0.001600 604.9 632.7
624(25) 0.001600 604.8 629.6
606(25) 0.001600 604.7 628.1
612(25) 0.001600 604.7 628.6
630(25) 0.001600 604.6 633.2
647(25) 0.001600 604.5 645.6
671(26) 0.001479 604.4 669.0
722(27) 0.001372 604.4 699.6
718(27) 0.001372 604.3 717.1
712(27) 0.001372 604.2 701.3
640(26) 0.001479 604.2 671.4
625(25) 0.001600 604.1 651.2
659(26) 0.001479 604.0 646.6
642(25) 0.001600 603.9 650.7
640(25) 0.001600 603.9 650.3
602(24) 0.001736 603.8 640.0
602(24) 0.001736 603.7 628.2
614(25) 0.001600 603.6 620.3
609(25) 0.001600 603.6 616.7
585(24) 0.001736 603.5 616.5
575(24) 0.001736 603.4 620.3
593(24) 0.001736 603.4 630.5
630(25) 0.001600 603.3 649.0
666(26) 0.001479 603.2 670.9
674(26) 0.001479 603.1 679.8
626(25) 0.001600 603.1 664.7
616(25) 0.001600 603.0 641.6
637(25) 0.001600 602.9 624.3
605(24) 0.001736 602.8 614.9
611(25) 0.001600 602.8 610.7
604(24) 0.001736 602.7 608.9
603(24) 0.001736 602.6 607.9
590(24) 0.001736 602.6 605.8
567(24) 0.001736 602.5 605.4
592(24) 0.001736 602.4 605.1
604(25) 0.001600 602.3 604.9
590(24) 0.001736 602.3 604.8
600(24) 0.001736 602.2 604.8
591(24) 0.001736 602.1 604.9
588(24) 0.001736 602.1 605.4
586(25) 0.001600 602.0 606.4
593(25) 0.001600 601.9 609.1
588(25) 0.001600 601.8 615.1
602(25) 0.001600 601.8 626.1
648(26) 0.001479 601.7 640.5
667(26) 0.001479 601.6 649.6
653(26) 0.001479 601.6 644.1
674(26) 0.001479 601.5 630.8
650(26) 0.001479 601.4 618.4
603(25) 0.001600 601.3 610.6
568(24) 0.001736 601.3 606.7
574(24) 0.001736 601.2 604.8
592(24) 0.001736 601.1 603.9
550(23) 0.001890 601.1 603.4
546(23) 0.001890 601.0 603.1
582(24) 0.001736 600.9 602.9
590(24) 0.001736 600.9 602.8
564(24) 0.001736 600.8 602.8
571(24) 0.001736 600.7 603.0
587(24) 0.001736 600.6 603.4
582(24) 0.001736 600.6 604.0
595(24) 0.001736 600.5 605.1
595(24) 0.001736 600.4 607.5
590(24) 0.001736 600.4 612.2
607(25) 0.001600 600.3 618.7
618(25) 0.001600 600.2 623.3
619(25) 0.001600 600.1 620.8
628(25) 0.001600 600.1 614.3
629(25) 0.001600 600.0 608.4
588(24) 0.001736 599.9 604.9
575(24) 0.001736 599.9 603.2
580(24) 0.001736 599.8 602.5
570(24) 0.001736 599.7 602.1
585(25) 0.001600 599.7 601.9
581(25) 0.001600 599.6 601.8
595(25) 0.001600 599.5 601.8
612(25) 0.001600 599.4 601.8
593(25) 0.001600 599.4 602.5
582(24) 0.001736 599.3 602.7
597(25) 0.001600 599.2 602.9
610(25) 0.001600 599.2 603.2
602(25) 0.001600 599.1 603.6
591(24) 0.001736 599.0 604.1
621(25) 0.001600 599.0 604.9
631(25) 0.001600 598.9 606.1
606(25) 0.001600 598.8 608.3
597(24) 0.001736 598.8 612.4
636(25) 0.001600 598.7 618.9
631(25) 0.001600 598.6 626.8
607(25) 0.001600 598.5 633.1
606(25) 0.001600 598.5 637.0
636(25) 0.001600 598.4 647.8
654(26) 0.001479 598.3 677.1
744(27) 0.001372 598.3 730.0
826(29) 0.001189 598.2 791.2
830(29) 0.001189 598.1 815.2
792(28) 0.001276 598.1 774.6
748(27) 0.001372 598.0 711.1
718(27) 0.001372 597.9 661.4
673(26) 0.001479 597.8 633.1
629(25) 0.001600 597.8 620.0
621(25) 0.001600 597.7 614.2
655(26) 0.001479 597.6 611.5
629(25) 0.001600 597.6 610.0
610(25) 0.001600 597.5 609.2
632(26) 0.001479 597.4 609.1
633(26) 0.001479 597.4 609.5
591(24) 0.001736 597.3 610.4
594(24) 0.001736 597.2 611.6
592(24) 0.001736 597.2 612.6
603(25) 0.001600 597.1 613.3
611(25) 0.001600 597.0 614.7
628(25) 0.001600 596.9 617.8
623(25) 0.001600 596.9 624.5
618(25) 0.001600 596.8 638.4
667(26) 0.001479 596.7 664.6
723(27) 0.001372 596.7 705.2
732(27) 0.001372 596.6 750.4
742(27) 0.001372 596.5 770.5
738(27) 0.001372 596.5 747.7
731(27) 0.001372 596.4 711.9
728(27) 0.001372 596.3 691.1
705(26) 0.001479 596.2 691.8
724(27) 0.001372 596.2 706.0
751(27) 0.001372 596.1 720.2
742(27) 0.001372 596.0 738.6
769(28) 0.001276 596.0 793.4
886(30) 0.001111 595.9 919.0
1112(33) 0.000918 595.8 1122.9
1276(36) 0.000772 596. 1341.
1327(37) 0.000730 596. 1409.
1260(35) 0.000816 595.6 1254.2
1086(33) 0.000918 595.5 1029.9
930(31) 0.001041 595.5 858.8
807(28) 0.001276 595.4 762.7
718(27) 0.001372 595.3 713.5
667(26) 0.001479 595.3 682.6
653(26) 0.001479 595.2 661.1
646(26) 0.001479 595.1 647.7
633(25) 0.001600 595.1 641.0
633(25) 0.001600 595.0 640.1
684(26) 0.001479 594.9 646.0
665(26) 0.001479 594.8 663.7
705(27) 0.001372 594.8 702.7
787(28) 0.001276 594.7 771.4
883(30) 0.001111 594.6 863.6
950(31) 0.001041 594.6 940.8
964(31) 0.001041 594.5 947.7
903(30) 0.001111 594.4 901.0
810(28) 0.001276 594.3 845.7
788(28) 0.001276 594.3 784.7
761(28) 0.001276 594.2 724.0
697(26) 0.001479 594.1 677.5
668(26) 0.001479 594.1 648.6
653(26) 0.001479 594.0 633.5
631(25) 0.001600 593.9 627.4
619(25) 0.001600 593.8 626.1
636(25) 0.001600 593.8 628.5
632(25) 0.001600 593.7 636.1
648(26) 0.001479 593.6 653.3
701(26) 0.001479 593.6 682.9
723(27) 0.001372 593.5 719.1
722(27) 0.001372 593.4 740.8
716(27) 0.001372 593.3 726.3
703(27) 0.001372 593.3 689.6
678(26) 0.001479 593.2 655.3
649(26) 0.001479 593.1 632.7
655(26) 0.001479 593.0 621.1
647(26) 0.001479 593.0 617.1
647(26) 0.001479 592.9 619.4
646(26) 0.001479 592.8 626.7
647(25) 0.001600 592.8 642.6
659(26) 0.001479 592.7 668.1
688(26) 0.001479 592.6 697.4
689(26) 0.001479 592.5 712.9
682(26) 0.001479 592.5 699.3
664(26) 0.001479 592.4 669.6
641(25) 0.001600 592.3 642.2
639(25) 0.001600 592.2 624.0
619(25) 0.001600 592.2 614.3
605(25) 0.001600 592.1 609.7
621(25) 0.001600 592.0 607.8
629(25) 0.001600 591.9 607.3
618(25) 0.001600 591.9 607.4
630(25) 0.001600 591.8 610.2
661(26) 0.001479 591.7 615.7
643(25) 0.001600 591.6 624.4
650(26) 0.001479 591.6 633.4
674(26) 0.001479 591.5 637.6
657(26) 0.001479 591.4 633.2
677(26) 0.001479 591.3 624.7
665(26) 0.001479 591.2 617.3
614(25) 0.001600 591.2 612.9
648(25) 0.001600 591.1 611.1
662(26) 0.001479 591.0 611.1
642(25) 0.001600 590.9 612.1
639(25) 0.001600 590.9 613.8
641(25) 0.001600 590.8 616.2
685(26) 0.001479 590.7 619.5
674(26) 0.001479 590.6 623.6
657(26) 0.001479 590.5 629.7
695(27) 0.001372 590.5 639.0
701(27) 0.001372 590.4 654.3
703(27) 0.001372 590.3 682.0
725(27) 0.001372 590.2 732.1
800(28) 0.001276 590.1 817.0
959(31) 0.001041 590.1 943.2
1088(33) 0.000918 590.0 1097.0
1198(35) 0.000816 589.9 1243.8
1266(36) 0.000772 590. 1328.
1268(36) 0.000772 590. 1291.
1217(35) 0.000816 589.7 1180.5
1100(33) 0.000918 589.6 1075.4
1010(32) 0.000977 589.5 985.9
937(31) 0.001041 589.4 892.9
832(29) 0.001189 589.3 806.3
758(28) 0.001276 589.2 742.0
704(27) 0.001372 589.2 701.9
665(26) 0.001479 589.1 681.8
673(26) 0.001479 589.0 675.7
678(26) 0.001479 588.9 679.8
688(26) 0.001479 588.8 695.5
738(27) 0.001372 588.7 731.8
782(28) 0.001276 588.7 807.2
885(30) 0.001111 588.6 946.9
1161(34) 0.000865 588.5 1166.0
1460(38) 0.000693 588. 1440.
1684(41) 0.000595 588. 1667.
1731(42) 0.000567 588. 1685.
1525(39) 0.000657 588. 1475.
1196(35) 0.000816 588.0 1197.5
922(31) 0.001041 588.0 966.1
778(28) 0.001276 587.9 813.8
691(27) 0.001372 587.8 728.5
692(27) 0.001372 587.7 685.2
696(26) 0.001479 587.6 663.5
705(27) 0.001372 587.5 652.4
687(26) 0.001479 587.4 647.1
660(26) 0.001479 587.3 645.6
700(26) 0.001479 587.2 645.9
682(26) 0.001479 587.2 645.4
657(26) 0.001479 587.1 643.0
660(26) 0.001479 587.0 640.8
662(26) 0.001479 586.9 642.1
648(25) 0.001600 586.8 650.4
662(26) 0.001479 586.7 671.3
739(27) 0.001372 586.6 712.4
815(28) 0.001276 586.5 780.1
856(29) 0.001189 586.4 872.0
916(30) 0.001111 586.3 966.5
964(31) 0.001041 586.2 1016.1
970(31) 0.001041 586.1 988.1
912(30) 0.001111 586.0 918.9
848(29) 0.001189 585.9 860.3
846(29) 0.001189 585.8 831.7
828(29) 0.001189 585.7 822.7
791(28) 0.001276 585.6 804.6
754(27) 0.001372 585.5 765.0
707(27) 0.001372 585.4 718.7
663(26) 0.001479 585.3 680.8
633(25) 0.001600 585.2 656.7
642(25) 0.001600 585.1 645.2
668(26) 0.001479 585.0 641.2
635(25) 0.001600 584.9 638.1
615(25) 0.001600 584.8 632.5
637(26) 0.001479 584.7 625.9
639(26) 0.001479 584.6 621.5
631(25) 0.001600 584.5 619.8
615(25) 0.001600 584.4 620.8
612(25) 0.001600 584.3 620.7
619(25) 0.001600 584.2 617.0
606(25) 0.001600 584.1 610.5
598(24) 0.001736 584.0 604.0
595(24) 0.001736 583.9 598.9
595(24) 0.001736 583.8 595.3
594(24) 0.001736 583.7 593.0
569(24) 0.001736 583.6 591.5
568(24) 0.001736 583.5 590.5
588(24) 0.001736 583.3 589.8
573(24) 0.001736 583.2 589.2
581(24) 0.001736 583.1 588.6
593(24) 0.001736 583.0 588.2
577(24) 0.001736 582.9 587.8
596(24) 0.001736 582.8 587.4
628(25) 0.001600 582.7 587.1
609(25) 0.001600 582.6 586.7
580(24) 0.001736 582.4 585.4
573(24) 0.001736 582.3 585.2
554(23) 0.001890 582.2 585.0
559(24) 0.001736 582.1 584.8
599(25) 0.001600 582.0 584.6
587(24) 0.001736 581.9 584.5
562(24) 0.001736 581.7 584.4
574(24) 0.001736 581.6 584.3
572(24) 0.001736 581.5 584.3
574(24) 0.001736 581.4 584.3
576(24) 0.001736 581.3 584.4
568(24) 0.001736 581.1 584.4
570(24) 0.001736 581.0 584.4
586(24) 0.001736 580.9 584.3
581(24) 0.001736 580.8 584.4
557(24) 0.001736 580.6 584.5
562(24) 0.001736 580.5 584.9
576(24) 0.001736 580.4 585.7
572(24) 0.001736 580.3 586.8
567(24) 0.001736 580.1 588.3
569(24) 0.001736 580.0 589.8
595(24) 0.001736 579.9 591.0
579(24) 0.001736 579.8 591.4
575(24) 0.001736 579.6 591.8
579(24) 0.001736 579.5 592.1
596(24) 0.001736 579.4 593.4
600(25) 0.001600 579.2 596.7
572(24) 0.001736 579.1 602.9
579(24) 0.001736 579.0 613.1
615(25) 0.001600 578.8 629.0
654(25) 0.001600 578.7 650.6
670(26) 0.001479 578.5 676.2
706(27) 0.001372 578.4 700.1
710(27) 0.001372 578.3 711.3
701(26) 0.001479 578.1 702.2
695(26) 0.001479 578.0 678.2
662(26) 0.001479 577.8 650.7
643(25) 0.001600 577.7 627.0
620(25) 0.001600 577.6 609.7
581(24) 0.001736 577.4 598.5
568(24) 0.001736 577.3 591.8
576(24) 0.001736 577.1 587.9
579(24) 0.001736 577.0 585.6
585(25) 0.001600 576.8 584.1
585(25) 0.001600 576.7 583.0
587(24) 0.001736 576.5 582.2
570(24) 0.001736 576.4 581.5
570(24) 0.001736 576.2 580.9
569(24) 0.001736 576.1 580.5
550(24) 0.001736 575.9 580.1
569(24) 0.001736 575.8 579.8
592(24) 0.001736 575.6 579.6
578(24) 0.001736 575.5 579.4
596(24) 0.001736 575.3 579.3
599(25) 0.001600 575.1 579.4
563(24) 0.001736 575.0 579.8
549(23) 0.001890 574.8 580.6
569(24) 0.001736 574.7 581.6
602(25) 0.001600 574.5 582.9
611(25) 0.001600 574.3 584.1
588(24) 0.001736 574.2 584.8
599(25) 0.001600 574.0 584.6
598(24) 0.001736 573.8 583.4
562(24) 0.001736 573.7 581.9
564(24) 0.001736 573.5 580.5
566(24) 0.001736 573.3 579.3
580(24) 0.001736 573.2 578.5
562(24) 0.001736 573.0 578.0
547(23) 0.001890 572.8 577.7
555(24) 0.001736 572.7 577.6
569(24) 0.001736 572.5 577.6
584(24) 0.001736 572.3 577.7
580(24) 0.001736 572.1 578.0
577(24) 0.001736 572.0 578.3
563(24) 0.001736 571.8 578.8
584(25) 0.001600 571.6 579.3
573(24) 0.001736 571.4 579.7
548(24) 0.001736 571.2 580.0
555(24) 0.001736 571.0 580.0
569(24) 0.001736 570.9 579.8
577(24) 0.001736 570.7 579.8
576(24) 0.001736 570.5 579.8
579(24) 0.001736 570.3 580.1
565(24) 0.001736 570.1 580.6
576(24) 0.001736 569.9 581.4
591(24) 0.001736 569.7 582.4
585(24) 0.001736 569.5 583.6
582(24) 0.001736 569.3 585.0
565(24) 0.001736 569.1 586.5
581(24) 0.001736 568.9 588.0
601(24) 0.001736 568.7 589.7
597(24) 0.001736 568.5 591.7
617(25) 0.001600 568.3 594.3
620(25) 0.001600 568.1 597.9
614(25) 0.001600 567.9 603.2
638(25) 0.001600 567.7 611.3
632(25) 0.001600 567.5 624.4
626(25) 0.001600 567.3 645.6
673(26) 0.001479 567.1 679.3
704(27) 0.001372 566.9 729.9
756(28) 0.001276 566.7 800.5
852(29) 0.001189 566.5 890.0
952(31) 0.001041 566.3 990.4
1034(32) 0.000977 566.0 1083.5
1143(34) 0.000865 565.8 1140.8
1214(35) 0.000816 565.6 1137.3
1171(35) 0.000816 565.4 1076.0
1041(33) 0.000918 565.2 984.3
962(32) 0.000977 564.9 889.8
839(29) 0.001189 564.7 808.7
731(27) 0.001372 564.5 747.2
677(26) 0.001479 564.3 705.2
642(25) 0.001600 564.0 679.3
607(25) 0.001600 563.8 665.2
617(25) 0.001600 563.6 659.9
634(25) 0.001600 563.3 662.1
636(25) 0.001600 563.1 671.3
645(25) 0.001600 562.9 686.3
682(26) 0.001479 562.6 704.4
718(27) 0.001372 562.4 720.6
719(27) 0.001372 562.1 728.2
735(27) 0.001372 561.9 722.4
743(27) 0.001372 561.6 704.1
723(27) 0.001372 561.4 679.1
666(26) 0.001479 561.2 653.5
611(25) 0.001600 560.9 630.9
614(25) 0.001600 560.7 612.9
596(24) 0.001736 560.4 599.8
587(24) 0.001736 560.1 590.7
608(25) 0.001600 559.9 584.7
592(24) 0.001736 559.6 580.8
551(24) 0.001736 559.4 578.3
553(24) 0.001736 559.1 576.6
570(24) 0.001736 558.8 575.5
596(25) 0.001600 558.6 574.7
570(24) 0.001736 558.3 574.2
541(23) 0.001890 558.0 574.1
571(24) 0.001736 557.8 574.2
572(24) 0.001736 557.5 574.8
585(25) 0.001600 557.2 576.0
604(25) 0.001600 557.0 578.0
601(25) 0.001600 556.7 581.5
616(25) 0.001600 556.4 587.1
621(25) 0.001600 556.1 595.9
626(25) 0.001600 555.8 609.0
630(25) 0.001600 555.6 627.3
656(26) 0.001479 555.3 651.1
677(26) 0.001479 555.0 679.7
684(26) 0.001479 554.7 711.0
734(27) 0.001372 554.4 740.4
757(28) 0.001276 554.1 761.3
765(28) 0.001276 553.8 767.1
763(28) 0.001276 553.5 755.6
727(27) 0.001372 553.2 731.3
694(26) 0.001479 552.9 701.7
677(26) 0.001479 552.6 672.6
674(26) 0.001479 552.3 647.7
655(25) 0.001600 552.0 628.5
642(25) 0.001600 551.7 614.8
641(25) 0.001600 551.4 606.1
651(26) 0.001479 551.1 601.4
624(25) 0.001600 550.8 600.0
596(24) 0.001736 550.4 601.4
612(25) 0.001600 550.1 605.0
617(25) 0.001600 549.8 609.8
614(25) 0.001600 549.5 614.2
611(25) 0.001600 549.1 616.5
610(25) 0.001600 548.8 615.0
615(25) 0.001600 548.5 609.5
591(25) 0.001600 548.2 601.3
570(24) 0.001736 547.8 592.0
576(25) 0.001600 547.5 583.0
590(25) 0.001600 547.2 575.0
604(25) 0.001600 546.8 568.4
621(25) 0.001600 546.5 563.3
593(24) 0.001736 546.1 559.5
578(24) 0.001736 545.8 556.7
585(24) 0.001736 545.4 554.7
572(24) 0.001736 545.1 553.2
530(23) 0.001890 544.7 552.0
525(23) 0.001890 544.4 551.0
532(23) 0.001890 544.0 550.2
545(23) 0.001890 543.7 549.4
570(24) 0.001736 543.3 548.7
569(24) 0.001736 542.9 548.1
575(24) 0.001736 542.6 547.5
563(24) 0.001736 542.2 546.4
568(24) 0.001736 541.8 545.9
567(24) 0.001736 541.5 545.5
547(23) 0.001890 541.1 545.1
565(24) 0.001736 540.7 544.7
567(24) 0.001736 540.3 544.5
561(24) 0.001736 539.9 544.3
545(23) 0.001890 539.5 544.2
549(23) 0.001890 539.2 544.4
556(24) 0.001736 538.8 544.8
534(23) 0.001890 538.4 545.5
542(23) 0.001890 538.0 546.6
532(23) 0.001890 537.6 548.1
537(23) 0.001890 537.2 550.0
552(24) 0.001736 536.8 552.0
575(24) 0.001736 536.4 554.1
567(24) 0.001736 536.0 556.0
559(24) 0.001736 535.6 557.2
558(24) 0.001736 535.1 557.5
533(23) 0.001890 534.7 556.7
537(23) 0.001890 534.3 555.0
560(24) 0.001736 533.9 552.5
529(23) 0.001890 533.5 549.6
529(23) 0.001890 533.0 546.5
558(24) 0.001736 532.6 543.6
548(23) 0.001890 532.2 541.1
537(23) 0.001890 531.8 539.0
550(23) 0.001890 531.3 537.2
547(23) 0.001890 530.9 535.7
545(23) 0.001890 530.4 534.5
545(23) 0.001890 530.0 533.6
534(23) 0.001890 529.5 532.8
551(23) 0.001890 529.1 532.1
565(24) 0.001736 528.6 531.4
558(24) 0.001736 528.2 530.8
550(23) 0.001890 527.7 530.3
547(23) 0.001890 527.3 529.8
537(23) 0.001890 526.8 529.3
524(23) 0.001890 526.3 528.8
528(23) 0.001890 525.9 528.3
530(23) 0.001890 525.4 527.8
543(23) 0.001890 524.9 527.3
540(23) 0.001890 524.4 526.9
489(22) 0.002066 524.0 526.4
497(22) 0.002066 523.5 526.0
500(22) 0.002066 523.0 525.5
511(23) 0.001890 522.5 525.1
497(22) 0.002066 522.0 524.6
491(23) 0.001890 521.5 524.2
497(23) 0.001890 521.0 523.8
493(23) 0.001890 520.5 523.4
510(23) 0.001890 520.0 523.0
521(23) 0.001890 519.5 522.7
518(23) 0.001890 519.0 522.3
502(22) 0.002066 518.5 522.1
507(22) 0.002066 518.0 521.9
531(23) 0.001890 517.4 521.9
527(23) . . .
524(23) . . .
500(22) . . .
469(22) . . .
429(21) . . .
378(20) . . .
312(17) . . .
265(16) . . .
237(15) . . .
168(13) . . .
115(11) . . .
91(9) . . .
74(9) . . .
77(9) . . .
85(9) . . .
77(9) . . .
77(9) . . .
85(9) . . .
88(9) . . .
82(9) . . .
77(9) . . .
73(9) . . .
67(8) . . .
54(7) . . .
64(8) . . .
66(8) . . .
59(8) . . .
59(8) . . .
45(7) . . .
39(6) . . .
43(7) . . .
42(6) . . .
40(6) . . .
41(6) . . .
38(6) . . .
24(5) . . .
24(5) . . .
25(5) . . .
19(4) . . .
30(5) . . .
32(6) . . .
26(5) . . .
24(5) . . .
26(5) . . .
27(5) . . .
25(5) . . .
23(5) . . .
26(5) . . .
26(5) . . .
23(5) . . .
30(5) . . .
30(5) . . .
26(5) . . .
29(5) . . .
24(5) . . .
29(5) . . .
29(5) . . .
32(6) . . .
30(5) . . .
33(6) . . .
34(6) . . .
28(5) . . .
25(5) . . .
27(5) . . .
33(6) . . .
32(6) . . .
22(5) . . .
19(4) . . .
26(5) . . .
26(5) . . .
26(5) . . .
27(5) . . .
19(4) . . .
24(5) . . .
22(5) . . .
16(4) . . .
21(4) . . .
33(6) . . .
30(5) . . .
20(4) . . .
20(4) . . .
18(4) . . .
24(5) . . .
25(5) . . .
21(5) . . .
24(5) . . .
25(5) . . .
15(4) . . .
3.0(10) . . .
0.0(10) . . .
0.0(10) . . .
0.0(10) . . .
0.0(10) . . .
0.0(10) . . .
0.0(10) . . .
0.0(10) . . .
0.0(10) . . .
0.0(10) . . .
0.0(10) . . .
0.0(10) . . .
0.0(10) . . .
0.0(10) . . .
0.0(10) . . .
0.0(10) . . .
0.0(10) . . .
0.0(10) . . .
0.0(10) . . .
0.0(10) . . .
0.0(10) . . .
0.0(10) . . .
0.0(10) . . .
0.0(10) . . .
0.0(10) . . .
0.0(10) . . .
0.0(10) . . .
0.0(10) . . .
0.0(10) . . .
0.0(10) . . .
0.0(10) . . .
0.0(10) . . .
